STRUCTURAL SHEAR JOINTS ANALYSES, PROPERTIES AND DESIGN FOR REPEAT LOADING
George T. Hahn Mechanical Engineering, Vand...
171 downloads
1008 Views
21MB Size
Report
This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!
Report copyright / DMCA form
STRUCTURAL SHEAR JOINTS ANALYSES, PROPERTIES AND DESIGN FOR REPEAT LOADING
George T. Hahn Mechanical Engineering, Vanderbilt University
Kaushik A. Iyer U.S. Army Research Laboratory
Carol A. Rubin Mechanical Engineering, Vanderbilt University
WOo D H E A D
P u 13 I. I
sHING
LIMITED
02005 by ASME,Three Park Avenue, New York, NY 10016, USA (www.asme.org) Copublished in Europe by Woodhead Publishing Limited, Abington Hall, Abington, Cambridge CBl 6AH, England; www.woodheadpublishing.com All rights reserved. Printed in the United States of America. Except as permitted under the United States Copyright Act of 1976,no part of this publication may be reproduced or distributed in any form or by any means, or stored in a database or retrieval system, without the prior written permission of the publisher. INFORMATION CONTAINED IN THIS WORK HAS BEEN OBTAINED BY THE AMERICAN SOCIETY O F MECHANICAL ENGINEERS FROM SOURCES BELIEVED TO BE RELIABLE. HOWEVER, NEITHER ASME NOR ITS AUTHORS O R EDITORS GUARANTEE THE ACCURACY OR COMPLETENESS O F ANY INFORMATION PUBLISHED IN THIS WORK. NEITHER ASME NOR ITS AUTHORS AND EDITORS SHALL BE RESPONSIBLE FOR ANY ERRORS, OMISSIONS, O R DAMAGES ARISING OUT OFTHE USE OFTHIS INFORMATION. THE WORK IS PUBLISHED WITH THE UNDERSTANDING THAT ASME AND ITS AUTHORS AND EDITORS ARE SUPPLYING INFORMATION BUT ARE NOT ATTEMPTING TO RENDER ENGINEERING OR OTHER PROFESSIONAL SERVICES. IF SUCH ENGINEERING O R PROFESSIONAL SERVICES ARE REQUIRED, THE ASSISTANCE O F AN APPROPRIATE PROFESSIONAL SHOULD BE SOUGHT. ASME shall not be responsible for statements or opinions advanced in papers o r . . . printed in its publications (B7.1.3). Statement from the Bylaws. For authorization to photocopy material for internal or personal use under those circumstances not falling within the fair use provisions of the Copyright Act, contact the Copyright Clearance Center (CCC). 222 Rosewood Drive, Danvers, MA 01923, tel: 9787508400, www.copyright.com.
Library of Congress CataloginginPublication Data Hahn, George T. Structural shear joints : analyses, properties and design for repeat loading / George T. Hahn, Kaushik Iyer, Carol A. Rubin. p. cm. Includes bibliographical references and index. ISBN 0791802388 (hardcover) 1. Shear (Mechanics) 2. Bolted joints. I. Iyer, Kaushik. 11. Rubin, Carol A. 111. Title. TA417.7.SSH34 2005 621.8'82dc22
2005016167
British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library. Woodhead Publishing ISBN13: 9781845691196 Woodhead Publishing ISBN10: 1845691199 Cover graphic: Computed maximum principal stress contours in a butt joint with 0.6% interference that is subjected to a remote tensile stress of 80 MPa
TABLEOF CONTENTS Preface Acknowledgements Introduction
vii ix xi
SECTION 1. MECHANICAL BEHAVIOR OF SHEAR JOINTS AND DESIGN CONSIDERATIONS Chapter 1. BASIC FEATURES 3 1.1. Aspects of Shear Joints 3 1.2. OutofPlane Deformation, Microslip and Plasticity 6 1.3. Fasteners and the Fastener Load 8 1.4. The Bearing, Clamping and Adhesive Modes of Load Transfer 8 1.5. Stress Descriptors for Fatigue 11 Chapter 2. SHEAR JOINTS IN THE BEARING MODE 13 2.1. Stress Descriptors for Bearing Mode 13 2.2. Butt Joint 14 2.3. Doubler 19 2.4. Lap Joint 20 2.5. Lap Joints in the AdhesivePlusBearing Mode 27 2.6. Multiple Rows of Fasteners 29 2.7. Biaxial Loading and Effects of the Free Edge 30 2.8. Fastener Stresses 33 Chapter 3. CLAMPING, INTERFERENCE, MICROSLIP AND SELFPIERCING RIVETS 41 3.1. The Clamped, Frictional or SlipResistant Mode of Butt and Lap Joints 41 3.2. Fasteners in the Clamping Mode 54 3.3. Hole Expansion, Squeeze and Interference 54 3.4. Contact Pressure, Microslip and Tangential Stress 59 3.5. Selfpiercing Rivet 63 Chapter 4. FATIGUE OF SHEAR JOINTS 67 4.1. Stages of the Fatigue Process 67 4.2. Failure Modes and Locations 67 iii
iv
Structural Shear Joints
4.3. Fatigue Strength of Panels 70 4.4. Fatigue Strength of Fasteners 80 4.5. Fretting Wear and Fatigue 81
Chapter 5. DESIGN CONSIDERATIONS FOR REPEATED LOADING 87 5.1. Mechanical Performance 87 5.2. Considerations for Joint Durability 87 5.3. Joint Type and Mode Selection 90 5.4. NDI and Fretting 91 5.5. Fail Safe Design 92 5.6. Generalizing Finite Element Results 92
SECTION 2. COMPILATION OF FINITE ELEMENT RESULTS Chapter 6. LOAD TRANSFER IN SINGLE RIVETROW LAP JOINTS (CONVENTIONAL AND COUNTERSUNK) 99 6.1. Summary of Load Transfer Models 99 6.2. Load Transfer Calculations for Single RivetRow Lap Joints 99 6.3. Summary and Important Points 104 Chapter 7. COMPILATION OF RESULTS FOR OPEN HOLE PANELS AND BUTT JOINTS 107 7.1. Summary of Calculational Models for Open Hole Panels 107 7.2. Summary of Calculational Models for Butt Joints 107 7.3. Summary of Calculation Results for Open Hole Panels 107 7.4. Summary of Calculation Results for Butt Joints without Interference 107 7.5. Effects of Interference in Butt Joints 114 Chapter 8. COMPILATION OF RESULTS FOR LAP JOINTS 125 8.1. Summary of Calculational Models 125 8.2. Summary of Calculation Results 125 8.3. Summary of Calculation Results Including Interference and Clamping 129 Chapter 9. SINGLE RIVETROW LAP JOINTS UNDER BIAXIAL LOADING 151 9.1. Summary of Calculational Models for 2D and 3D Lap Joints under Biaxial Loading 151 9.2. Summary of Calculation Results for Pinned Connections under Biaxial Loading 151 9.3. Summary of Calculation Results for Single RivetRow Lap Joints under Biaxial Loading 151 Chapter 10. COMPILATION OF RESULTS FOR LAP JOINTS WITH SEALANTS AND ADHESIVES 157 10.1. Summary of Calculational Models for for Single RivetRow Lap Joints with Sealants and Adhesives 157 10.2. Summary of Calculation Results for Pinned Connections with Sealants and Adhesives 157
Table of Contents
V
Chapter 11. COMPILATION OF RESULTS FOR RIVETS 161 11.1. Summary of Calculational Models for Rivets 161 11.2. Summary of Calculational Results for Rivets 161 Chapter 12. DATA TABULATIONS 173 12.1. Summary Calculation Results for Single RivetRow Lap Joints 173 12.2. Summary Calculation Results for Double RivetRow Lap Joints 173 12.3. Summary Calculation Results for Rivet Installation Residual Stresses 174 12.4. Summary Calculation Results for Single RivetRow Joints Under Biaxial Loading 174 12.5. Summary Calculation Results for Single RivetRow Joints With Sealant 175 12.6. Summary Calculation Results for Variation of Panel Thickness in Wide Single RivetRow Joints 183 12.7. Summary Calculation Results for Joint Excess Compliance and Rivet Tilt 183
SECTION 3. CALCULATIONAL MODELS AND VALIDATION Chapter 13. FINITE ELEMENT MODELS 189 13.1. 2D Models of Butt Joints, Attachment Joints and Open Hole Panels 189 3.2. 3D Models of Single RivetRow Lap and Butt Joints (Standard and Countersunk Rivet Heads) 190 13.3. Double RivetRow Lap Joints (Standard and Countersunk Rivet Heads) 195 Chapter 14. THIN ADHESIVE LAYER ANALYSIS (TALA) FOR MODELING SEALANTS AND ADHESIVES INSTALLED IN JOINTS 197 14.1. Development of A Thin Adhesive Layer Analysis (TALA) 197 14.2. Conversion of Adhesive Solid Element to Spring Element for 2D Fem 197 14.3. Conversion of StressStrain Relationship to ForceDisplacement Relationship for Thin Adhesive Layer 200 14.4. Mechanical Behavior of Thin Sealant Layer 202 14.5. Shear Spring Dependence of Contact Pressure 205 Chapter 15. MATERIAL MODELS FOR THE FINITE ELEMENT CALCULATIONS 207 15.1. Materials Used in the Finite Element Calculations 207 Chapter 16. VALIDATION OF FINITE ELEMENT CALCULATIONS AND TALA 209 16.1. Finite Element Model Validation 209 16.2. Validation of The Thin Adhesive Layer Analysis (TALA) 210 Chapter 17. STRESS CONCENTRATION FACTORS IN MULTIPLE ROW JOINTS 217 17.1. Analyses of Multiple Row Joints 217 17.2. Estimating Fastener Loads in Multiple Row Joints 217
vi
Structural Shear Joints
17.3. Estimating Fastener Loads with 3D Deformations 218 17.4. A Superposition Method for Estimating SCFs 221 17.5. Validation 223
Chapter 18. ANALYSIS OF FASTENER TENSION AND CLAMPING STRAIN 225 18.1. Nomenclature 225 18.2. Clamping Model 226 18.3. Fastener Tension and Clamping Strain Predictions 227 18.4. Summary of Procedure 229 APPENDIX A. SUMMARY OF CALCULATIONAL MODELS 231 APPENDIX B. STRESS CONCENTRATION FATORFATIGUE STRENGTH (SCFFS) ANALYSIS 241 APPENDIX C. ANALYSIS OF FRETTING WEAR AND FATIGUE 249 APPENDIX D. SYMBOLS, ABREVIATIONS AND UNITS 253 REFERENCES 257 INDEX
PREFACE Engineers employ shear connections  riveted and bolted butt and lap joints  in a wide range of structures and machines. Ordinary stress analyses of joints are unable to define the features that ultimately govern fatigue and fretting and provide bases for design. Detailed analyses have only become possible in the past decade with advances in finite element methods and computing capabilities.This text places into context the results of over 150 detailed, 2D and 3D finite element analyses of aluminum and steel shear connections.The text examines the following joints, both single and multiple row, fasteners and modes of load transmission: butt joints lap joints attachment joints and doublers
bearing mode clamped mode adhesives mode bearing mode with hole expansion
pins standard head fasteners countersunk fasteners self piercing rivets interference fasteners
The analyses examine the fastener joint geometry, the adjacent region of the panel and the important design variables. The text connects global features such as nominal stress, excess compliance and fastener load, with the local conditions that affect fatigue and fretting. Among the important local conditions are the contact pressures, interface slips, residual stresses and the intensity and location of the stress concentrations. The text is divided into 3 sections designed for different audiences:
Section 1
Engineers and technicians seeking a better understanding of shear connections. The first section introduces the different joints and identifies the important variables. It offers stress contours and distorted meshes that complement easily grasped descriptions of the behavior of panels and fasteners for the different modes of load transmission. Engineers preparing to design shear connections resistant to fatigue.The pros and cons of the butt and lap joints for the different load transfer modes are discussed and a fail safe strategy is identified in the first section. In addition, a simple and general FSSCF (Fatigue StrengthStress Concentration Factor) analysis useful for preliminary design is identified and validated. The analysis offers estimates of either the fatigue strengths of joints or the vi i
viii
Structural Shear Joints
joint geometry meeting a given fatigue strength requirement. Expressions for estimating the bolt tension of clamped joints and the fastener load and SCF of multiplerow joints are derived in appendices. Engineers and technicians interested in fretting and in the fatigue strength of shear connections. An extensive selection of fatigue strength measurements for riveted, bolted, and bonded aluminum and steel joints is offered in the first section. The measurements are compared with the forecasts of the FSSCF estimation procedure. The contributions of fretting wear and fretting fatigue are also examined. NDE practitioners interested in knowing where to look for fatigue cracks and fretting damage. The stress concentrations in shear joints are responsible for fatigue damage and crack initiation. The locations of the stress concentrations, which depend on the joint type and mode of load transfer and are affected by hole expansion, are identified in the first section. Section 2
Engineers and researchers wishing to access more finite element analysis findings. A handbooktype, more detailed summary of the results of finite element calculations for fasteners and panels is presented in Section 2 of the book. Section 3
Engineers and researchers seeking to perform finite element analyses of shear connections. To assist workers with computations, the finite element models, meshes, boundary conditions and procedures used by the authors are described in Section 3. This includes TALA, a Thin Adhesive Layer Analysis for modeling joints fastened with either adhesive alone, or with rivets (or bolts) combined with a sealant or adhesive. Material models and parameters employed in the calculations are listed. Validation of the finite element methods in the form of comparisons with closed form analyses, other computations and measurements is presented.
ACKNOWLEDGEMEN The authors are indebted to John Wikswo of the Vanderbilt University Physics Department who is responsible for inspiring the initial phases of the research endeavor described in this book. The authors acknowledge the important contributions of the graduate students who contributed to this research. In alphabetical order they are: former PhD students Charoenyut Dechwayukul, Thongchai Fongsamootr, and Notsanop Kamnerdtong; and former MS students Khalid AlDakkan, Felicia Brittman, Yun Huang, and Charat Loha. They also wish to thank Pedro Bastias, a former PhD student and colleague, who provided much help and advice for the graduate students. Computations were performed with the ABAQUS finite element program provided by Abaqus, Inc. Most computations were performed on parallel systems in 3 major centers: the National Center for Supercomputing Applications in Illinois (SGI Power Challenge Array), Center for Advanced Computing at the University of Michigan in Ann Arbor (IBM SP) and Department of Defense Major Shared Resource Center at the U.S. Army Research Laboratory in Maryland (IBM SP and SGI Origin). Riveted lap joint specimens with and without a sealant were prepared Textron Aerostructures, Inc., Nashville, TN. with the help of Tom Warrion, Mike Floyd and Paul Nelson. Bill Keller of PRCDeSoto International, Inc. (formerly Courtalds Aerospace) provided the test sealants. Bill King of Emhart Teknologies, Mt. Clemens, MI and Daniel Hayden of General Motors Corp., Warren, MI provided assistance with fabrication and testing, respectively, of the Selfpiercing Riveted (SPR) joints. Changchun Liu and Tuomas Wiste, graduate students at Vanderbilt University, and, Shirleen Johnson of the graphic arts division at the U.S. Army Research Laboratory provided significant assistance with the drawings in this book. The work was supported by the Air Force Office of Scientific Research, Vanderbilt University, The Royal Thai Government and the General Motors Collaborative Research Lab (GMCRL) at the University of Michigan (Ann Arbor).
ix
INTRODUCTION This book draws on the results of 2 and 3dimensional, finite element analyses of shear joints performed by the authors and graduate students between 1992 and 2001 [l81. Much of this work has been published [9221,but many findings are reported for the first time. The preparation of this text prompted additional, and more detailed computations. The text presents these new findings which have modified some of the authors’ earlier interpretations. The analyses evaluate features relevant to joint performance with respect to fatigue and fretting failure. The computations treat the openhole panel and seven different joint configurations, including eight ways of fastening them, and 15 other joint variables: Joint Configuration 1. Panel with an open hole 2. Attachment joint 3. Butt joint 4. Single fastener row lap joint 5. Double fastener row lap joint 6. Adhesive lap joint 7. Double fastener row doubler
Panel material Elastic or elastic plastic behavior Panel width Panel thickness
Fastener Type H. No fastener (open hole) P. Pin S. Standard fastener head C. Countersunk fastener head A. Adhesive or sealant SA. Standard fastener combined with adhesive CA. Countersunk fastener combined with adhesive SP. Selfpiercing rivet
Joint Variables Fastener material Fastener head shape Interference Fastener clamping Number of fastener rows
Interface friction Uniaxial and biaxial loading Adhesive properties Adhesive thickness
An alphanumeric code employing the joint configuration number and fastenertype abbreviation (shown above) is defined in Appendix A. This code is used throughout the book to identify the calculational models employed. The book is divided into 3 sections: Section 1 (Chapters 1  5) describes the mechanical behavior of shear joints, the effects of major variables, failure modes, and design considerations for fatigue and fretting. xi
xii
Structural Shear Joints
Section 2 (Chapters 612) offers handbooklike summaries of the results of the finite element analyses in the form of stress contour plots, graphs and tables, with the bulk of the findings presented in Tabular form in Chapter 12. Section 3 (Chapters 1318) Describes the computational methods and their validation. This includes the finite element models of joints and thin adhesive layers, material behavior modes, spring models of multiple row joints, and an analysis of the fastener clamping force.
SECTION 1
MECHANICAL BEHAVIOR OF SHEAR JOINTSAND DESIGN CONSIDERATIONS
CHAPTER
BASICFEATURES 1.1 ASPECTS OF SHEAR JOINTS
Shear joints are structural details for fastening panels together to form a load carrying connection. Such joints are also referred to as shear connections or splices and they can be fastened with rivets, bolts, adhesive or welds. The term panel is used here to mean either sheet, plate, beam, cylinder or vessel. The contrasting features of four common shear joints are illustrated in Figure 1.1: Butt Joint. The butt or double shear joint, shown in Figure M a , is formed by fastening two abutting panels with overlapping side panels. The external load is applied to the abutting panels, creating a state of nearly pure shear in two planes of the fastener shank and pure inplane (2dimensional) deformation in the two center panels. The bending of the fasteners and outofplane movements of the side panels are restricted by closefitting fastener holes and presence of the middle panel, and are usually negligible.
Attachment Joint. This is a panel loaded along one edge and fastened to a relatively rigid supporting structure. The response is largely 2dimensional. The limiting case, treated in this text is for an attachment joint whose fasteners and support structure are rigid and fixed in space. Lap Joint. The lap or single shear joint is formed by fastening the overlapping edges of two panels. Figure l.lc illustrates that the shear load applied to the fasteners by the panels tilts the fasteners and bends the panels outofplane. The fastener tilt angle can amount to 1"3"; outofplane displacements of the panels to 1 mm to 2 mm. These are not negligible and are accounted for by the 3dimensional analyses in this text. Doubler. This is a panel fastened to a larger, main panel as a reinforcement. The connecting fasteners divert load to the doubler thereby reducing the stresses on the main panel. Although the magnitude of outofplane deformations may be small, the geometry is 3dimensional and the analysis must treat it as such. Multiple Row Joints. The shear connections in Figure 1.1 are depicted with a single row of fasteners for clarity. In practice, two or more rows of fasteners may be inserted to reduce
3
4
Structural Shear Joints
lpz
0 0 0
. c )
D
Pl
r
rttt 0 0 P
e n
Figure 1.1. Schematic drawings of 4 shear joints: (a) butt joint, (b) attachment joint, (c) lap joint and (d) doubler.
the local stresses generated in the fasteners and the panels. Figure 1.2 illustrates a lap joint with three fastenerrows, and introduces the terminology: “leading” and “lagging”, for the row of fastener holes (and not the fasteners themselves) closest to and furthest from the panel edge where the load is applied, respectively.The terms “front” panel and “back” panel
5
Basic Features
A
+
1
C
t
t
G
E 
t
t
+ H
F
0 0 0 
G
H
t
D
6
T
D
+ section AA
Figure 1.2. Model features and terminology: (a) (infinitely) wide joint. Edges AB and CD are stressed; edges EG and FH are stress free and (b) narrow joint with edges AB, CD, EG and FH stress free, and (c) Section AA with definitions of the leading and lagging row of holes of multiple row joints.
are used to identify the panels that can and cannot be visually inspected, respectively,when only one side of the joint is accessible. An important feature of multiplerow joints is that the outer rows of fasteners, the two rows of fasteners connecting the leading and lagging row of holes, support the largest loads. At the same time, the local stresses generated in the panels adjacent to the leading row of holes are always higher than at the lagging holes. Analyses of the fastener loads and stresses in multiple row joints are examined in Chapters 2.6 and 17.
Wide and Narrow Joints and Biaxial Loading. In some applications, shear joints are narrow and formed by short rows of one or two fasteners. For others, like the cylindrical aircraft fuselage, the joints are wide with long rows containing scores of fasteners. This text draws on the two types of shear joint models illustrated in Figure 1.2 and described fully in Chapter 13. One is infinitely wide, has a repeat distance of PI,and describes the conditions in the interior of a wide joint. The other is a model of a “narrow,” single fastener joint of width, L1, with stress free edges on all sides. When wide joints are loaded in simple tension, the inplane transverse contraction of the panels in the vicinity of the fastener holes is constrained and a state of biaxial stress is generated away from the free edges. The influence of this and other biaxial stress states and the
6
Structural Shear Joints
B
Figure 1.3. Example of a builtup shear joint. Shown is a section of a Douglas, longitudinal, laptype skinsplice for an aircraft fuselage [23]:Askin, Bfinger doubler and Clongeron.
proximity of the free edge on the stressses at the fastener holes is described more fully in Chapter 2.7. Builtup Joints. The performance of joints for some applications can be improved by combining two shear joint elements.The airframe fuselage joint illustrated in Figure 1.3 consists of a lap joint combined with two “finger” doublers [23]. The contoured finger doublers serve to distribute fastener loads more evenly. Design Aspects. Dimensions of the fastener relative to those of the panels, fastener geometry, fastener spacing, clamping and interference residual stresses due to fastener installation, panel surface finish including adhesives and sealants, are major design parameters universal to structural shear joints. Open Hole Panels. Open hole panels with straight and countersunk holes are not shear connections but their analyses are particularly useful for treating multiple row joints. Idealized examples, with a centrally located, circular hole, uniformly loaded in uniaxial tension are shown in Figure 1.4. Three variations of the open hole are considered in this text: (i) a straight empty hole, (ii) a straight hole filled with a close fitting fastener shank [24] and (iii) an empty countersunk hole (see Chapter 7.3). Unlike shear connections, no load is applied to the panel at the site of the hole. 1.2 OUTOFPLANE DEFORMATION, MICROSLIP AND PLASTICITY
OutofPlane Deformation, Clamping, Interference and Friction. The loading of the openhole panel and the attachment joint fastened with headless pins does not produce displacements or stress gradients in the outofplane directions provided the hole and pin diameters are uniform (straight hole). The gradients in a butt joint assembled with conventional fasteners are also usually negligible in the absence of lateral clamping. In these cases, 2dimensional analyses are appropriate. The tilting of the lap joint fasteners, which is accompanied by the bending of the panels, and clamping produce significant stress gradients in the thickness direction; these increase the peak stress and shift its location to the panel interior surface. The tilting also produces contact pressure peaks under the fastener head edge. For
7
Basic Features
t
t
t
t
A
L2
L2
0 D
Figure 1.4. Schematic of open hole panels: (a) empty hole and (b) filled hole.
these reasons, the lap joint and the clamped butt joint must be treated as 3dimensional problems. The analysis of shear joints is further complicated by friction and by interference at the fastenerpanel interfaces. Ciavarella and Decuzzi [25]have devised a closed form solution for the 2dimensional, frictionless, pinpanel contact problem for elastically similar material pairs without interference or clamping. However, analysts must resort to the finite element methods described in Chapter 13 to examine friction, clamping, arbitrary material pairs and the proximity of free edges even for 2dimensional models of joints.
Microslip. The loading of a shear joint is accompanied by microscalesize,relative movements of the components at the contacting, fastenerpane1 and panelpanel interfaces.These movements, referred to here as microslip, contribute to the total deformation of the joint and affect the stress distribution. Microslip in structural joints is controlled by friction and is a highly nonlinear type of deformation behavior. Consequently, even when the panels and fasteners of shear joints display linear elastic stressstrain behavior, the assembled joint will depart from linear behavior. The departures are evaluated in Chapter 5.6. Plasticity. The onset of plastic deformation, either local yielding at stress concentrations or general yielding, also contributes to departures from linear elastic behavior. These departures are obtained at relatively low nominal stresses in view of the large stress concentrations. For example, a single rivetrow, aluminum butt joint (yield stress = 500 MPa) will begin to yield locally when the applied (gross section) stress exceeds 87 MPa. Above this nominal stress the concept of the SCF fails to describe stress elevation and elasticplastic analyses are needed to define the local stresses and strains. Cyclic StressStrain Behavior. Elasticisotropicplastic analyses can evaluate the strains during the first loading cycle. When the joint is subject to repeated cycles of loading, more
8
Structural Shear Joints
sophisticated, elastickinematicplastic analyses that account for the hysteresis loop are needed to define the steady state plastic strain amplitudes [26281. The strain amplitude is a crucial descriptor of fatigue, but its evaluation calls for the finite element modeling of the joint for multiple cycles of loading and unloading that precede the steady state. Such modeling presents difficult problems because it is computationally intensive and because the constitutive theory is not fully developed. Some elasticisotropicplastic and elasticlinearkinematicplastic analyses of joints are described in this book, but these were performed mainly to evaluate the effects of local plasticity on contact pressure and slip.
1.3 FASTENERS AND THE FASTENER LOAD
Generic types of fasteners are illustrated in Figure 1.5. They include rivets, whose heads are formed in place by upsetting a blank, and bolts with preformed heads and retaining nuts. Rivets and bolts may have protruding heads, or countersunk heads. The fastener head and shank play important roles. The head allows the fastener to clamp the joint together and its rigidity limits local bending of the panels and important peak stresses. At the same time, the benefits of clamping in the panel hole are partly offset by the stress concentration in the panel underneath the edge of the rivet head. This tradeoff can be an important factor in design. The shank must support tensile stresses which can be very high when load transfer relies on high levels of lateral clamping.The compressibility of the shank is reduced adjacent to the more massive head; this introduces gradients of contact pressure and stress in the thickness direction for fasteners installed with interference. The fastener load, Q, is the load transmitted to the pin, rivet or bolt holding the joint together. For single fastenerrow joints, Q is the product of the gross section stress, 6, the panel thickness, t, and the fastener spacing or pitch, P1 (see Figure 1.2):
In multiple row joints, the load Q is distributed among all the rows, but not evenly! The fasteners in the leading and lagging rows of holes always support a larger portion of Q, with intermediate rows carrying progressively smaller portions. This is described more fully in Chapters 2.6 and 17.
1.4 THE BEARING, CLAMPING AND ADHESIVE MODES OF LOAD TRANSFER
The fastener load, Q, can be transmitted from one panel to the other by one or a combination of three modes of load transfer.
Bearing Mode. In the bearing mode, Figure 1.6a, load transfer proceeds mainly at the panel holefastener shank interface. Panel 1 presses against one end of the fastener shank (at A), and the other end of the shank presses against the opposite panel (at B) stabilizing panel 2. The bearing mode produces high levels of contact pressure and tensile stress at the panel hole periphery. A detailed analysis of load transfer by the bearing mode in a lap joint is presented in Chapter 6.
Basic Features
9
Figure 1.5. Examples of fasteners used in shear connections: (a) rivet with standard head, (b) countersunk rivet, (c) standard bolt, and (d) countersunk aircrafttype bolt, (e) selfpiercing rivet.
Clamping Mode. The clamping mode, also referred to as the frictional,slip resistant or slip critical mode, is illustrated in Figure 1.6b. A clamping force, Qc,is produced by torquing the bolt or upsetting the rivet. This force is also called the bolt tension. The resulting contact pressure at the panelpanel interface under the fastener head (at A, Figure 1.6b) produces the friction traction, pQc (p is the coefficient of friction) which transfers load from panel 1 to panel 2. In the clamping mode the fastener hole periphery remains largely unstressed.The maximum fastener load that is supported by friction is:
10
Structural Shear Joints
m
Q 3\
Q
Q Figure 1.6. Schematic representation of the 3 modes of load transfer in lap joints: (a) bearing mode, (b) clamping or frictional mode, and (c) adhesive mode. Note: The tilting of the fasterner, panel bending and attending tractions arising from the unbalanced shear couple are omitted for clarity.
where cp = 1 for lap joints and cp = 2 for butt joints'. As long as this load is not exceeded, the joint is said to be slipresistant or supporting load in the ,frictional mode2. Clamping can reduce the peak stresses generated in the panel by as much as 70% relative to the bearing mode. This major benefit is obtained at cost of higher stresses in the fastener shank.
Combined ClampingPlusBearing Mode. Beyond the load carrying capacity of the clamping mode (Equation 1.2), load transfer is accomplished by the combination of an essentially fixed clamping component and a growing bearing component. However, the benefits of clampingreduced peak stressespersist even after the bearing component becomes dominant. AdhesivePlusBearing Mode. The adhesive mode employs shear tractions supported by the adhesive layer, 3 in Figure 1.6c,to transfer load from panel 1 to panel 2. When combined
I The 2fold difference in the value of cp arises because clamped butt joints develop shear tractions on two surfaces compared to one for lap joints. For reasons discussed in Chapter 3.1, the panel does not slip into the bearing mode as soon as this value of Q is exceeded.
Basic Features
11
with rivets and bolts, the adhesive reduces the fastener load and the peak stresses generated at the fastener holes. The reduction in fastener load is directly related to the stiffness of the adhesive. However, even low modulus sealants, whose main function is to restrict moisture penetration, can reduce peak stresses substantially. This is examined in Chapter 2.5. 1.5 STRESS DESCRIPTORS FOR FATIGUE
Shear joints subjected to repeated cyclic loading are vulnerable to contact fatigue failure, which is initiated in the bulk. The distributions of the stresses, contact pressure and microslip, in the vicinity of the fastener hole and at the interfaces, are complex and nonuniform. The peak values of stress amplitude and mean stress are critical for forecasting the fatigue life of the joint. Cyclically loaded joints also experience fretting, the toandfro rubbing (cyclic microslip) of contacting panelpanel and panelfastener interfaces. Fretting can produce changes in the surface topography; it can promote wear and initiate fatigue failure, affecting the cyclic life of joints in special cases.
The Stress Concentration Factor (SCF). The peak tensile stress, (T*, is conveniently described by the stress concentration factor (SCF) defined as the ratio of the peak tensile stresstonominal (gross section) stress: SCF = (T*/(T.The SCF of the empty, openhole panel, SCF = 3, is widely known [29]. Figure 1.4 illustrates that the hole is distant from the site of load application. Elevated stresses arise from the small load that is redistributed locally when the panel is perforated. The loading of shear joint panels is distinctly different. Here the fastener hole is the site of load application.The combination of large fastener load applied to a small area produces even larger local stresses; the SCFs of single fastenerrow shear joint panels can be 2x to 4x the SCFvalue of the open hole. The magnitudes and locations of the SCFs of shear joint panels depend on the mode of load transfer (see Table 1.1) and many other factors. This topic is dealt with more fully in Chapters 2 and 3. The varia
TABLE 1.1. STRESS CONCENTRATION FACTORS, SCFS, FOR TENSILE LOADED, ALUMINUM, OPENHOLE PANELS, AND SINGLE RIVETROW LAP JOINTS MODE OF SCF ANGULAR Finite Element LOAD TRANSFER LOCATION' Model or Ref. OPEN HOLE PANEL L 1 , L2 >>D empty hole 3.00 0", 180" (29) filled hole 2.1 0", 180" 1H5 filled hole 2.85 22", 158" 1H5 LAP JOINT, P1/D=5. D/t=4 Bearing 6.1 3", 183" 4s1 Clamping 4.5 90" 5.12 I", 181" 4SA5 Bearing + Adhesive 1. The convention for angular location is given in Figure 2a. 2. SCF calculated for a low modulus sealant.
12
Structural Shear Joints
tions of contact pressure, microslip and tangential stress at joint interfaces are described in Chapter 3.4.
Fretting Factors. To quantify the possible influence of fretting wear and fretting fatigue, two fretting factors (F1 and F2) have been reported in the literature [30,31].The fretting wear factor, F1, is related to the depth of the wear scar.The fretting fatigue factor, F2, is an approximate expression of the integrated effects of contact pressure, microslip and the bulk tangential stresses. Both parameters were empirically derived to model the influence of fretting on the reduction in fatigue life in turbine engine dovetail joints; they have been used on occasion to design these components. Values of F1 and F2 and the severity of fretting fatigue and wear of shear joints are assessed in Chapter 4.5. Discussion of the influence of fretting and the reliability of these parameters is covered more fully in Appendix C.
CHAPTER
JOINTSIN THE BEARING MODE
SHEAR
2.1 STRESS DESCRIPTORS FOR BEARING MODE
In the bearing mode, a relatively large fastener load, Q, is applied to the small area of contact between the fastener shank and the panel. The area corresponds approximately with the projected area of the shank, A = Ds t (where Ds is the diameter of the shank and t is the panel thickness). In single fastener row joints, the concentration of load produces peak local stresses, o*,of order Q/A: (z*
=f(QIA) =f(QlDst) =f(oPi/Ds),and SCF = O*/O =f(Pl/Ds)
In addition, the stresses are affected by p, the coefficient of friction, which governs microslip at the joint interfaces and, in the case of lap joints, by the fastener shank diametertopanel thickness ratio, Ds/t, which affects panel bending. The geometry of the fastener head and its rigidity also play a role because the clamping forces applied by the fastener head reduce panel bending under the head. The number of fastener rows also has a large effect on joint response because, Qi, the actual load transmitted to the fasteners of a particular row, is a fraction fi, of the (total) fastener load: Qi = fi Q. Finally, the residual stresses attending shankhole interference have major effects. These are described in Chapter 3.3. It follows that the mechanical response of the jointincluding the joint compliance, rivet tilt, local stresses, strains, and displacements, the local contact pressure and slip, and the state of the fastenersdepends on the following variables: Joint response = f (fi (z P1/DslDs/t, p,interference, fastener head geometry) SCF = f (fi P1/Ds, Ds/t, p,interference fastener head geometry)
(2.3) (2.4)
The material properties of the panels, fasteners, and sealant or adhesive at the joint interfaces, the type of loadinguniaxial or biaxialand the proximity of free edges are additional variables.
13
14
Structural Shear Joints
Figure 2.1. The (311stresscontours in the thickness direction of a 3D model of a butt joint showing the absence of a significant stress gradient. The cover panel and half the center panel of a single rivetrow butt joint fastened with standard head rivets are shown. The applied stress is 60 MPa. (Model 3s1).
2.2 BUTT JOINT
This section presents results of 2 and 3dimensional analyses of a 1:2:11,aluminum butt joints in the bearing mode. The 2dimensional analyses preclude outofplane gradients and can only represent a joint secured with a headless pin. The 3dimensional models treat a joint fastened with rivets or bolts with standard heads and allow outofplane bending of the rivet shank and panels and rivet tilt. In spite of these differences, the results of the two sets of analyses are similar.The (311 stress contours in Figure 2.1 illustrate that outofplane gradients are virtually absent. The SCFvalues listed in Table 2.1 for the 2dimensional model and the center panel of the 3dimensional model, SCF = 6.4 and 6.3, respectively, are nearly the same. The SCFvalue at the faying surface of the cover plates, SCF = 6.4, is only 1.6% higher; fastener bowing is 0.2" when (3 = 60 MPa The findings confirm that the outofplane bending of butt joints is usually negligible and that results obtained with 2dimensional analyses, such as those in Chapter 7.2, are useful approximations for butt joints in the bearing mode2. Figure 2.2a shows the angular conventions used throughout this book. Features of the inplane 01 I stress distribution in the vicinity of a filled open hole are illustrated in Figure
' 1:2:1 are the relative thickness values of the butt joint cover, center and cover panels. Outofplane variations in stress are obtained in clamped joints (see Chapter 3.2).
Shear Joints in the Bearing Mode
15
TABLE 2.1. STRESS CONCENTRATION FACTORS, SCFS, FOR ALUMINUM ATTACHMENT JOINTS AND BUTT JOINTS IN THE BEARING MODE ANALYSIS
GEOMETRY AND FRICTION Narrow joint with single, headless fastener LI/Ds=5 p=O
SCF
ANGULAR Finite Element LOCATION I Model or Ref.
6.1
2", 178'
3P13
LI/Ds=5
p=0.2
6.3
4", 176"
3P16
LI/Ds=5
p=1.0 8.2
4",176"
3P18
L,,L2=m
p=0.2
184"
3P6
Wide, multifastenerjoint with single row of headless fasteners 2D analysis PI/D~=~ p=0.2 6.4
O", 180"
3P1
PI/D&
p=0.2 7.9 *
O", 180'
3P1
3D analysis, cover panel, faying surface
PI/D~=~
p=0.2 6.4
O", 180'
3s1
3D analysis, center panel, faying surface
PI/D,=5
p=0.2 6.3
O", 180"
3s1
2D analysis
2D analysis
4.5
4O,
1. The convention for angular location is given in Figure 2a. 2. SCF value estimated using the Seliger SCF dependence on Q/D.
2.2b. The inplane 011stress contours for the butt joint are shown in Figure 2.2~.It can be seen that the bearing mode produces intense contact pressures and compression on both sides of the panelfastener shank interface in a 120"sector centered on 0 = 270". The panel and fastener are unloaded on the opposite side of the hole in a 12O0sectorcentered on 0 = 90", where a gap between the fastener and the panel develops (Figure 2.2a). A stress concentration with peak tensile stresses forms in the panel adjacent to the hole periphery near the 0 = 0" and 0 = 180"locations (Figure 2.2~).The peak tensile stress displays a nearly linear dependence on the nominal stress and a small amount of hysteresis related to slip and friction as illustrated in Figure 2.3a; the corresponding SCF is essentially constant (Figure 2.3b). The peak stress and SCF at the 0" and 180"locations are here referred to as "net section" peak stress and "net section" SCF. The peak stress at the 0 = 90", r = 1.2 r~~ and the corresponding SCF are referred to as the "gross section" peak stress and "gross section" SCF (Figure 2.3a and 2.3b). The net section SCF is larger than the gross
Where r is radial distance measured from the center of the fastener hole and r H is the local radius of the stressed hole.
Structural Shear Joints
16 +90°
0 1
f180"
+835E*07
i554Ea7
00
I
+7 33 E m
+3 85 EIOB
~
2
3
+3 2 4 E U n 8 52 EUn .203E a 3 ZU E8
n 1:
a.01E m
2: 3:
e.21E m
4: + 4 . 8 5 E e
5: 8: 7: 8: 9: 0: 1:
+3.17 E+OB +1.43E+OB 2.02 E+07 1.8QE+# 3.57E+# 5.25 E+OB &#Ern8 2: 8.82 E m 3: 1.03 E+OB
Figure 2.2. Displaced mesh and 011stress contours on inplane sections of the panel adjacent to the hole edge: (a) example of the displaced mesh for wide, single fastener row butt joint showing convention for angular location, P1/Ds = 5, (b) filled openhole panel, SCF = 3 (1H5), (c) wide, single fastenerrow butt joint, P1/Ds = 5 , SCF = 6.4, (3P1), and (d) wide, = 125 MPa. single rivetrow lap joint, P1/Ds = 5 , Ds/t = 4, SCF = 6.1 (4S1), onom
section SCF for the bearing mode of load transfer, but the opposite is true for lap joints in the clamping mode. This is important because the location of the dominant SCF determines the mode of joint failure. Results for contact pressure, microslip and the tangential stresses at the shankpanel interface of butt joints are presented in Chapter 3.4.
Shear Joints in the Bearing Mode
17
1000 1
h
6ool 500
20
0
40
60
80
100
120
140
u (MPa)
ll
2
11r
"

z

        


160
Structural Shear Joints
18
looo
1
0
20
40
60
100
80
120
140
160
cr (MPa)
l o9
I
7 6
'I1
0
0

20

1 7 I 
~
40
60
80
100
120
140
u (MPa)
(4 Figtwe 2.3. (continued) (c) and (d) lap joint. Models (3s1)and (4329), (22).
160
Shear Joints in the Bearing Mode
2: 3: 4:
5: 8: 7: 8: 9:
0: I: 2: 3:
19
+4.24E+OB +3.79E+OB + 3 . 3 E+OB +2.88E+OB +2.45E+OB +2.mEW +I.fBE+OB +1.11 Ho8 4.61E W +2.13 I307 2.34EW 0.81 E W
Figure 2.4. Stress contours generated in a wide, 2row aluminum doubler (P2 = PI, P1/D, = 5, D$t = 4, p = 0.2 and 0 = 150 MPa) fastened with standard head rivets and no clamping (Model 7s1). The contours illustrate that stress variations in the thickness direction are negligible.
2.3 DOUBLER The stress contours for a 2row doubler (P2 = PI, P1/Ds = 5, Ds/t = 4) are reproduced in Figure 2.4. They illustrate that stress distribution, like that of the butt joint, is essentially 2dimensional with negligible variation in the thickness direction. According to the analysis of this particular 2row doubler (Chapters 17.2,17.3 and Table 17.4), about 10% of the load applied to the main panel is diverted to the doubler panel4 while a stress concentration, SCF s 2.8, is generated in the main panel.This SCF is in agreement with the value, SCF = 2.9, derived from the finite element model and Figure 2.5. This means that the 10% reduction in the stress carried by the main panel is offset by the 290% increase in stress at the main panel fastener hole edge. With a 4fold increase in the fastener row separation, P2 = 4P1, a larger stress reduction, about 20%, and SCF = 3.2 are obtained. Benefits are realized when the doubler straddles a detail in the main plate with a large stress concentration. For example, the 20% reduction in stress afforded by the doubler is equivalent to reducing a detail SCF = 6 to SCF = 3.8, this at the cost of the SCF = 3.2 concentration introduced at the main panel fastener holes. Larger benefits are possible with 4 and 6row doublers (see Table 17.4).
For the following values appropriate for this doubler: k/K = 0.18 and Ks/K z 1.5, the fastener load fraction, Q,/QO.1.
Structural Shear Joints
20
500 450
T
400 350
h 
300 250
b’ 200 150 100
50 0 0
20
40
60
80
100
120
140
160
u (MPa)
Figure 2.5. Variation of the net section stress adjacent to the fastener hole in the main panel of the wide, 2row doubler referred to in Figure 2.4 (Model 7s1).
2.4 LAP JOINT
Single RivetRow. Results obtained with 3dimensional analyses of lap joints differ from those for butt joints in one important respect: the effects of outofplane bending of lap joints are not negligible. Rivet tilt and outofplane bending of two lap joints are illustrated in Figures 2.6a and 2.6b. Both the tilt and bending increase with fastener 1oad.The 011stress contours are superimposed on the deformed meshes in Figures 2 . 6 ~and 2.4d. The angular variation of the inplane, tangential, 000stress (at the edge of the hole) at the panel top surface (z = 0), on the midplane (z = 0 3 ) and the bottom surface (z = t) are shown in Figure 2.7. The variations with the thickness direction are produced by the outofplane panel bending displayed by the distorted meshes in Figure 2.6. The panel bending displaces the highest stresses and the SCF to the interior face of both panels. An important consequence is that fatigue cracks are likely to initiate at the SCFlocation where they are hidden from direct observation by both the rivet head and the panel5. This complicates the task of nondestructive evaluation (NDE) of fatigue damage. Figures 2 . 3 ~ and 2.3d describe the variation with nominal stress of the peak 011stresses and SCFs at the depth z = t, the panel faying surface for the standard rivet head. The nearly linear variation with nominal stress at the net section and gross section locations and the
When cracks initiate at the faying surface of the back panel, the panelpanel interface acts as an additional obstacle to NDF detection.
Figure 2.6. Profiles of the displaced meshes and corresponding 011stress contours in the vicinity of the panel holes (with the fasteners not shown) for 2, wide, aluminum, single rivetrow lap joints, P1/D = 5, D/t = 4, nominal stress, onom = 125 MPa: (a) standard rivet head with (b) corresponding stress contours (4S1), and (c) 100"countersunk head with (d) corresponding stress contours (4C1). The shaded portions of the distorted meshes indicate the initial configuration. The displacements of the meshes are magnified 3x.
Structural Shear Joints
22
m
a I m
b"
90
60
30
0
30
90
60
@,O
(a) 1000
I
900 800 700 600
500 m
a
z
400
ok
300 200
100 0
100 200
90
60
0
30
30
60
90
8. a
(b)
Figure 2.7. The angular and withdepth variation of the tangential stress, adjacent to the fastener hole of wide, aluminum, single rivetrow lap joint panels (P,/D = 5, D/t = 4, = 125 MPa): (a) standard rivet heads (4S1), and (b) countersunk heads (4C1).
Shear Joints in the Bearing Mode
23
TABLE 2.2. PROPERTIES OF WIDE, TENSILE LOADED, ALUMINUM, 1 AND 2 RIVETROW LAP JOINTS IN THE BEARING MODE LAP JOINT
GEOMETRY
I . I RivetRow 1.1 Std. aluminum rivet head P,/D=5, D/t=4 1.2 Aluminum rivet 100"csnk to 112 panel thickness 1.3 Same as 1.2 but with steel rivet 1.4 Aluminum rivet 10Oocsnk to full panel thickness 2. 1 RivetRow 2.1 Std. aluminum rivet head P,ID=8, DiF4 2.2 Aluminum rivet 100°csnk to 112 panel thickness 2.3 Aluminum rivetlOOOcsnk to full panel thickness 3. I Std. aluminum rivet head 3. 2 Rivetrow P,/D=5, Dip4 3.2Aluminum rivet 100"csnk
EXCESS RIVET TILT COMPLIANCE, d G N degrees 27.5 3.6 34.4 4.2 28.3 41.2
4.0 4.1
SCF 6.1 9.8
8.8 12.1
LOCATION' F.E. MODEL 8 r z 3", 183' r,, t 4s1 3", 183' rll t 4c 1 lo, 181' r,, t 6", 186" rH t
4C2 4C6
7Sd 12.1d
4Sld 4C I
14.7d
4CSd
7.5
1.7', 1.7'
4.4b, 3.1'
20b, 3"' rH t
5s1
10.3
1.5b, 1.9'
6.1b,4.5'
3"', So'' rH t
5CI
a. Location of SCF given in polar coordinates. Convention for angular location, 8, is given in Figure 2a. The quantity, rH, is the local radius of the stressed fastener hole; z is the depth measured from the outer surface of the panel.
h. Leading row rivets c. Lagging row rivets d. SCF values estimated using Seliger (32) SCF dependence on PdD
dominant SCF are similar to those found for the butt joint.The gross section SCF of the lap joint exceeds that of the butt joint. The SCFs of a number of lap joints are listed in Table 2.2. Other features of the loaded lap joint including the excess compliance, rivet tilt, and stresses and displacements at key locations are tabulated in Chapter 12. Both the amount of bending and its distribution and the lateral constraint imposed by the rivet head affect the stress concentration. This is illustrated by the results for a wide aluminum lap joint (P1/D = 5, D/t = 4, CT = 125 MPa) with standard rivet heads which displays a rivet tilt of a = 3.7". The tilt, which is 10x larger than the bowing of a butt joint fastener, produces significant panel bending which elevates the tensile stresses at the panel faying surface. Yet, the net section stress concentration of the lap joint, SCF = 6.1, is less than the value obtained for a comparable butt joint, SCF = 6.4, which hardly bends at all. The muted affect of bending is related to the distribution of bending. The lateral constraint produced by the relatively massive and rigid rivet head limits the amount of panel bending directly under the head where the net section SCF is located. The bulk of the bending is shifted to the unclamped region outside the head. In addition, the contribution of bending in a lap joint is offset by the frictional component of load transfer that reduces the force on the rivet by 10% (see Chapter 6). In contrast, the countersunk rivets display a tilt, a = 4.2" (for a = 125 MPa), and the countersunk panel a net section SCF = 9.8. The 14% higher tilt angle and attending increase in panel bending account for a small part of the 61% increase in the SCF.Two other factors are at play. First, the main part of the bearing load is transmitted to the countersunk rivet by the noncountersunk faces at the lower half of the panel. As a result, the tangential tensile stresses are skewed toward the lower half of the panel at depths between 0 3 < z < t, and this adds to the concentration of stress near the interior panel face produced by panel
24
Structural Shear Joints
bending (compare Figures 2.7a and 2.7b). Secondly, the less massive and more compliant countersunk head allows more bending at the critical location under the head, as shown by the greater variation of the peak circumferential stress with thickness in Figure 2.7b. These findings illustrate that both the shape of the fastener and the rigidity of the fastener head affect the panel SCE
Double RivetRow. The stress contours and distortions of a two rivetrow lap joint fastened with standard head rivets are illustrated in Figure 2.8. It follows from the symmetry that the fastener loads applied to the two rows are identical and half the value of the single row joint described in the previous paragraphs. The net section SCFs of the single and double row joints in Table 2.2 illustrate two generalizations that apply to multiplerow joints: i. The local stresses at the leading row do not diminish in proportion to either the number of rows or the fastener load. In this case, doubling the number of rows reduces the SCFs at the leading row by only 28% and 38% for the standard and countersunk rivets, respectively. ii. The local stresses at the leading row are higher than at the lagging row. In this case the stresses at the leading row are 42% and 36% higher at the leading row for the standard and countersunk rivets, respectively. The origins of these unexpected variations of fastener load and the SCF in multiplerow joints are dealt with in Chapter 2.6. Influence of the PitcJdDiameter and DiametermhicknessRatio. Local stresses in the fastener and panel depend only on Q, the fastener load, as long as the separation of fasteners is large and the overlap of stresses from adjacent fasteners is negligible. In that case, the SCF varies linearly and directly with the PI/D, ratio (see Equation (2.2)):
where the value of v is influenced by other geometric variables. For very small fastener separations, P1/D, < 2, the SCF will be dominated by the net section (the reduced load bearing cross section of the panel) and will vary inversely with PI/D,. For intermediate values of PIID,, a transition from one to the other dependence is to be expected. Crude estimates of the 3 dependencies are offered in Figure 2.9 along with experimental results and the value derived from calculations. Seliger [32] measured the fatigue lives of single rivetrow lap joints with different rivet spacings in the range 4 < PI/Ds < 12, and compared these with the fatigue lives of unperforated samples of the panel material. He then deduced values of the (net section) SCF of the joints from the ratios of the stress levels that produced comparable lives. The Seliger results plotted in Figure 2.9 correspond with a fatigue life of N = lo7 cycles, conditions least likely to involve local yielding. His values and the calculated value for PI/Ds = 5 are in accord. However, they do not conform with Equation (2.5), possibly for two reasons. First, the value of the SCF measured for Pl/Ds = 12 may be understated because of the onset of yielding (See Appendix B). Secondly, the range 2 < P1/Ds < 6 probably corresponds with the transition. More work is needed to evaluate y~ and define the variation of the SCF in the transition regime. The effects of panel thickness on single rivetrow lap joints have been evaluated with finite element calculations by Fongsamootr (33); the variations of SCF with Ds/t are shown
Shear Joints in the Bearing Mode
L
25
i
(c>
Figure 2.8. Profiles of the displaced mesh and the 011stress contours for an aluminum, double rivetrow lap joint, Pl/D = 5, D/t = 4,nominal stress, onom = 125 MPa (5s1): (a) displaced mesh; displacements magnified 3x; shaded areas show initial configuration, (b) stress contours for hole #1, (c) stress contours hole for #2.
in Figure 2.10. The two sets of results (Figures 2.9 and 2.10) make it possible to generalize findings obtained for a particular, P1/Ds and Ds/tlap joint configuration. Although the Seliger's P1/Dsresults were obtained for lap joints, they offer approximations for doublers, butt and attachment joints as well. The Ds/t dependence does not apply to butt and attachment joints display little or no panel bending.
Structural Shear Joints
26 14112
10
$1 4i 8r
6
*I
m
I
OO
TRANSITION DEPENDENCE (SCHEMATIC) DERIVED FROM FATIGUE TETS OF 24ST ALUMINUM (AFTER SELLGER) FINITE ELEMENT CALCLJLATION FOR ALUMINUM LOP JOINT
0
1
1
2
4
1
1
6
8
,
10
1
12
14
P/DS
Figure 2.9. Estimates of the variation with the pitchtodiameter Ratio, PlIDs, of the stress concentration factor (SCF) for aluminum, single rivetrow lap joint panels including experimental results of Seliger [32] and Model (4s1).
1
PID=5
\
100' COUNTERSUNK HEAD
STANDARDHEAD
i i
Figure 2.10. Influence of the diametertothickness ratio, D/t, on the stress concentration factors for aluminum, single row lap joint panels, PI/D = 5 with standard head rivets after Fongsamootr [ 3 3 ] .
Shear Joints in the Bearing Mode
27
t
1 1
20
40 60 YOUNGS MODULUS,MPa
80
100
Figure 2.11. Influence of adhesive stiffness on the stress concentration factor (SCF) for aluminum, narrow, single rivet lap joint panels, L1/Ds = 5 , Ds/t = 4 (68,21).The calculations are for standard head rivets with a 300 ?madhesive layer (Models 3S8,3SA6,19,20,and 21, and for 100"countersunk head rivets with a 180 ymadhesive layer (Models 3C9,3CA6).
2.5 LAP JOINTS IN THE ADHESIVEPLUSBEARING MODE
This section describes findings for lap joints fastened with both rivets and adhesive6 where load transfer proceeds by both the bearing and the adhesive mode [21]. Results of finite element analyses of lap joints fastened exclusively with adhesive are summarized in Chapter 16 [6,21]. The installation of an adhesive at the interfaces of a pinned or bolted joint offers important mechanical benefits. Relatively stiff adhesives dramatically increase load transfer directly across the panels, thereby reducing the bearing load on the fastener, the amount of tilting and bending, and the peak stresses and SCF generated in the panel. Figure 2.11 describes the relation between the panel net section SCF and the stiffness of hypothetical adhesives. These calculations assume that the adhesive remains intact: does not fail or separate from the panel interfaces. This requires that the adhesive supports peak tensile and shear stresses that increase with the stiffness of the adhesive. Examples of the magnitude of these stresses are listed in Table 2.3. Polymer sealants, which are installed primarily to shield the joint interfaces from corrosion, are very compliant and may possess an elastic modulus as low as E = 1 MPa, and an equally low, pressure dependent shear modulus. This stiffness corresponds with the data points at the extreme left of Figure 2.11. Nevertheless, low modulus sealants can improve
The models treat joints with adhesive at both the panelpanel and fastenerpanel interfaces
Structural Shear Joints
28
TABLE 2.3. PEAK TENSILE AND SHEAR STRESSES SUPPORTED BY A 180 pTHICK LAYER OF ADHESIVE INSTALLED AT THE INTERFACES OF A 30.6 mmWIDE, SINGLE RIVETROW, ALUMINUM LAP JOINT, L1/D = 5, D/t = 4 After Fongsammootr (7) ADHESIVE TENSION PEAK TENSILE MODULUS", MPa STRESS, MPa
1.1 4.4 17.6 70.4
0.65 1.18 1.82 3.22
PEAK SHEAR STRESS, MPa
F.E.MODEL
0.5 1 1.41 2.95 5.08
4SA6 4SA 19 4SA20 4SA2 1
a. Combined with a pressure sensitive shear modulus
TABLE 2.4. PERCENT CHANGES IN THE MECHANICAL BEHAVIOR PRODUCED BY A 180 pTHICK LAYER OF SEALANTa INSTALLED AT THE INTERFACES OF RIVETED, SINGLEROW,ALUMINUM LAP JOINTS, P1/D = 5, D/t = 4 After Fongsammotr (7) and Kamnerdtong (8) F.E. MODEL RIVET HEAD PANEL THICKNESS, nim NOMINAL STRESS, MPa
4S8,4SA5 Standard 1.53 65
4S10,4SA7 Standard 1 .oo 65
Excess compliance Rivet tilt Inplane slip Outofplane slip Panelshank contact pressure Lateral separation of panels SCF
+I4 2" +42 +700 +16 40 16
.+I2 7" +52 +514 +2 1 57 18
4C9,4CA25 100"countersunk
1.53 60 .+I4 2" +4 +I26 +28 57 28
a. Desoto PR1776 Type B2 sealant, Youngs Modulus, E=l MPa
mechanical performance significantly.The computed changes in the mechanical response of single rivetrow lap joints are summarized in Table 2.4. These show that the sealant, acting like a lubricant, increases joint compliance and the inplane and outofplane movements of the panels.The SCFs are reduced by 16% to 35% along with lateral separation of the panel ends, fastener tilt and panel bending. These changes are accompanied by 10fold increases in the joint fatigue life, described in Chapter 4.3.
Shear Joints in the Bearing Mode
29
TABLE 2.5. VALUES OF THE FASTENER LOAD RATIOS, f, AND THE SCFS OF DIFFERENT, MULTIPLE ROW JOINTS WITH ALUMINUM PANELS AND RIVETS, P/D = 5, Dlt = 4 AND P2/P1= 1, DERIVED FROM THE 2 SPRINGS MODEL AND THE SUPERPOSITION METHOD JOINT TYPE
k/K
1row lap joint, std. rivet head (obtained from analysis 4C1)
ROWI* f SCF 1
6.1
4.3
ROW2 f SCF
ROW3 f SCF
ROW4 SCF
f
2row lap joint, std. rivet head
0.2
0.5
3row lap joint, std. rivet head
0.2
0.36 3.8
0.28 2.6 0.36 2.2
4row lap joint, std. rivet head
0.2
0.28 3.5
0.22 2.6 0.22 2.0 0.28 1.7
4row lap joint, std. rivet head, and 1% interference
0.4
0.31 3.6
0.19 2.4 0.19 1.9 0.31 1.9
4row lap joint, csk. rivet head
0.2
0.28 4.5
0.22 3.4 0.22 2.9 0.28 2.7
4row doubler, std. rivet head Panel Doubler
0.2
0.19
0.06
8row butt joint, pinned
0.5
3.2 1.2
0.33 3.8
0.5 3.1
0.06 2.3 0.8
0.19 2.3 0.8
3.2 1.2
0.17 2.3 0.17 1.9 0.33 2.1
* Leading row of holes
2.6 MULTIPLE ROWS OF FASTENERS
Additional load carrying capacity or a reduction in local stresses is achieved by adding one or more rows of fasteners to shear joints. However, progressively smaller benefits are realized with increasing number of rows. This is related to the distribution of fastener load and the contribution of the bypass load to the SCF [24,34].
Estimating Fastener Load. The load applied to one panel of a multiple row joint is progressively transferred to the facing panel(s) by successive rows of fasteners. The heavily loaded panel incrementally sheds load, while the initially unloaded, facing panel, is incrementally loaded. As a result of this sequence, there are disparities in the amounts of load supported by facing strips of panel between the same fastener rows.The load disparities are accompanied by mismatch in the amounts of extension and Poisson’s contraction displayed by the facing strips [34].To maintain continuity of the fasteners, the sum of the deformation produced by: (1)the fastenerfastener hole complex, and (2) the intervening panel strip, must be identical for facing strips between the same two rows. The load and deformation disparities together with the
30
Structural Shear Joints
compatibility requirement affect the fastener loads transmitted by the individual rows as well as the variations of fastener load within a row near the free edge (see Chapter 2.7). Onedimensional spring models, that account for the compatibility requirement and the interactions between the fastenerfastener hole combination and the intervening panel strip, have been used by Swift [24] and Muller [34] to estimate fastener loads. A 2springs model, devised by the authors is described in Chapter 17. The stiffness of one spring, k, characterizes the fastenerfastener hole response; the stiffness of the other, K, the response of the intervening panel strip.The models define fi, the fractions of the total fastener load acting at each fastener row, as a function of the stiffness ratio, k/K. Approximated values of the k/K ratio for different joints are listed in Table 17.1. Examples of the fastener load distributions for multiplerow shear joints are summarized in Table 2.5. According to the analysis, fastener loads are highest at the leading (or lagging) row of holes. Reduced fastener row spacing and a relatively more compliant fastenerhole response, which reduce the k/Kratio, favor more uniform load distributions and reduce the fastener load at the leading (or lagging) row.
Estimating the Net Section SCF. Panel stresses generated at a particular row of fastener holes by the bearingmode component of fastener load arise from the superposition of two stress fields. One is produced by the fastener load, Qi. the other by the bypass load, QBP, that is transmitted by the panel across the fastener hole to the next row of fasteners (refer to Chapter 17).The resulting SCF can be approximated by summing estimates of the SCFs associated with the two fields. An estimation procedure and validation are described in Chapter 17. Examples of the variations of the SCFs in different, multiple row shear joints are summarized in Table 2.5. These illustrate three important generalizations: (i) Increasing the number of rivetrows beyond two greatly diminishes returns for stress reduction at the leading row. For the lap joints of Table 2.5, an increase in the number of rows from two to three (a 50% increase in the number of fasteners) produces only a 12% decrease in the peak stress. (ii) With the stresses acting on the leading row 40% to 70% higher than on successive rows, the panel and the fasteners at the leading row are much more vulnerable to failure than the following rows. (iii) High stresses at the leading row can complicate the task of detecting fatigue damage, NDE, because the lagging row of holes of the front panel face the leading row of the back panel (see Chapter 1.1, Figure 1.2). For multiplerow lap joints with standard heads, the highest SCF is produced at two locations: (i) At the interior face of the leading row of the front panel, and (ii) Directly under the lagging row of the front panel on the far side of the of the panelpanel interface (the interior face of the leading row of the back panel). The detection of fatigue damage at this second location is very difficult when only the front panel is accessible. In that case, the front fastener head, the fastener headpanel interface, the entire front panel and the panelpanel interface are barriers to nondestructive detection. 2.7 BlAXlAL LOADING AND THE EFFECTS OF THE FREE EDGE
The SCFs produced by wide joints with multifastener rows display variability along the row. The fasteners immediately adjacent to the free edge display higher SCFvalues than those
31
Shear Joints in the Bearing Mode
TABLE 2.6. THE ELEVATION OF THE STRESS CONCENTRATION FACTOR, SCF, BY THE FREE EDGES OF NARROW, L = 30.6 mm SINGLE RIVETROW LAP JOINTS RELATIVE TO INFINITELY WIDE JOINTS WITHOUT FREE EDGES TYPE OF LAP JOINT Std. head, no sealant Std. head, sealed
PANEL THICKNESS SCFELEVATION mm ?h 1.53 1 .oo
1.53 1.oo
Countersunk head, no sealant Countersunk head, sealed
1.53 1 .oo 1.53 1.00
F.E.MODEL
6.0 4.6 7.3 5.1 6.7 5.2 7.8 6.8
located a distance >3P1 from the edge. The findings are summarized in Table 2.6. There appear to several sources of the stress elevations.
Biaxial Loading of SingleRow Joints. Iyer [1,35] has examined the effects of transverse loads on wide, single fastenerrow joints. His calculations provide estimates of the SCF for four different biaxial stress states:
v. This condition is obtained in a wide joint loaded in simple tension without transverse loads because the dimensional changes in the (inplane) transverse direction are constrained. (ii) 02/01 = v + 0.5. This condition is obtained in wide, longitudinal seams of cylindrical pressure vessels (iii) 0 2 / 0 1 = v + 1.This condition is obtained in wide, longitudinal seams of spherical pressure vessels. (iv) 0 2 / 0 1 = 0. This, the condition for a fastener close to the free edge, was not examined explicitly, but was evaluated with the results for iiii, above by extrapolation. (i)
02/01 =
Iyer’s findings, summarized in Figure 2.12, show that biaxial loading produces modest reductions in the net section SCF of shear joints, For example, the biaxial stress ratios, 02/01 = 0.25 and 02/01 = 0.75 associated with the uniaxially loaded joint and the cylindrical vessel reduce the SCF by 0.5% and 5% respectively relative to the value obtained for 0 2 / 0 1 = 0 by extrapolation. In other words, the nearzero biaxial stress ratio associated with fasteners next to the free edge would be expected to elevate the SCF by about 0.5% relative to the fasteners in a wide joint away from the edge.
SCF Elevation in Narrow, Single Row Joints. Calculations summarized in Table 2.6 compare the SCFs of wide (no free edges) lap joints, P1 = 30.6 mm, with those of otherwise identical narrow joints, L = 30.6 mmwide, single rivet joints with 2 free edges and a setback of P1R.The proximity of 2 free edges elevates the SCF by from 5% to 8%.The authors believe that the narrow joint may simulate the conditions experienced by fasteners in a wide joint
Structural Shear Joints
32
8t
LAP JOINT. 100' COUNTERSUNK HEAD
i i
LAP JOINT, STANDARD HEAD
\
:
0
5
0.2
,
1
0.4
0.6
0.8
1
02'9
Figure 2.12. The influence of the biaxial stress ratio, 02/01, on the stress concentration factors (SCF) of wide, single fastenerrow, aluminum butt and lap joint panels with standard head rivets (Models 2P22,23 and 24,3S16,17, and 18, and 3C17,18, and 19).
adjacent to the free edge. The elevations cannot simply be attributed to the loss of lateral stress at the free edge since the expected increase from this source is only about 0.5% (see preceding paragraph and Figure 2.12). It appears that the SCF elevation at the free edge arises from more subtle changes in the stress distribution. One possibility is that the elevation is related to the setbackthe margin between the fastener and the free edge. Increases of the setback distance increase the local value of PI and are expected to increase the SCF, and vice versa (see Chapter 2.4). It is not clear that a setback of 0.5P1 exactly reproduces the stress state obtained in the interior of a wide joint with a pitch of PI. The effect of setback on the SCF has not been examined here and bears further study.
Biaxial Loading of MultipleRow Joints. As noted in Chapter 2.6, there are disparities in the amounts of load supported by facing strips of panel between the same fastener rows. The load disparities and accompanying mismatch in the amounts of Poisson's contraction displayed by the facing strips affect the fastener load near the panel edge. Muller [34] has calculated that the mismatch elevates the load applied to the fastener adjacent to the panel free edge by 10°h7.The elevation is for a %row lap joint and v = 0.33 and is expected to increase with additional fastener rows and vary directly with Poisson's ratio. It should be noted that
'This result applies to a 3row. eight rivets per row, PI/D = 5.9, D/t = 3.2 lap joint with a set back of OSP1 at the free edge.The Poisson's ratio of the model is v = 0.33.
Shear Joints in the Bearing Mode
33
Muller employed finite element models with a free edge, and therefore including the effects described in the preceding two paragraphs. 2.8 FASTENER STRESSES
Butt Joints. The shear joint panels transmit the load, Q, to the fasteners. Figure 2.13a illustrates the basic loading of the fasteners in butt joints. The edge of the center panel bears against one side of the fastener shank with the load Q, and this is transmitted to the edges of the 2 cover panels on the opposite side. The shear force, Q/2, applied to Section AA produces a moment that is balanced by the shear force acting on Section BB. As the panels bear against the fastener, they compress the shank and generate high levels of contact pressure, whose intensity and angular distribution are described in Chapter 3.4. An expression for the peak tensile stresses, which are produced by bending at location c (Figure 2.13a), has been proposed by Timoshenko [3618.A fastener shank with a relatively large diametertolength ratio, e.g., such as the aluminum rivet model with Ds/H = 2, behaves as a relatively stiff beam that displays little bowing. In that case, the panels transmit essentially no lateral force to the fastener heads, and no net force to the fastener shank. As a result, the headshank, and nutshank junction corners (locations 3A and 3B) and thread roots close to the nut, which act as stress concentrators, remain unstressed.
Lap Joint Fasteners, Standard Head. Fasteners of lap joints are subject to four sets of loading shown schematically in Figure 2.13b: Set 1. The edges of the panels bear against the fastener on opposed sides of the shank with the force Q (locations 1A and 1B). This is analogous to the loading in the butt joint except that the moment of the shear force, Q on the midsection is initially unbalanced. The bearing loads compress the shank under the contacting surfaces. Set 2. Relative movement between the edges of the panels and shank is resisted by shear tractions, pQ, at locations 1A and 1B arising from friction. These shear tractions contribute to the unbalanced moment and apply tension to the shank. Set 3. The initially unsatisfied moment produced by the bearing loads at locations 1A and 1B tilt the fastener. The facing panels resists the tilting by generating the normal forces, QB, against the underside of the fastener head near the leading corner (location 2A), and the lagging corner (location 2B). These forces produce bending moments and they load the fastener shank in tension. The forces at Locations 2 and 3 are distributed along a 150" sector of the circumference of the shank and the underside of the rivet head (see Chapter 6). The stress contours for other sections through the fastener are not identical to those in Figure 2.14. Set 4. Relative movement between the panel and the under side of the fastener head is resisted by shear tractions ~ Q Bat, locations 2A and 2B arising from friction and the normal forces produced by tilting. These shear tractions also produce bending moments acting on the shank.
6*= 4HQhDs2
34
Structural Shear Joints
12A
/3A
1A
3B'
I
?+f 38
20
I
5 L  t 
t
1'laBI7
I , . bDs 4 pp
4 0.1 1[3De+Ds] (d)
Figure 2.13. Schematic representation of the forces acting on fasteners in joints in the bearing mode: (a) standard head rivet in a butt joint, (b) standard head rivet in a lap joint, (c) 100"countersunk rivet in a lap joint, and (d) generalized, concentrated force model of the forces acting on standard head fastener in a lap joint. The drawings identify the bearing forces (location l), the reaction forces (2), and stress concentrations at the shankhead corner (location 3).
A simplified, concentrated force model of the lap joint fastener loading is presented in Figure 2.13d. The locations of the different forces are based on the stress contours in Figure 2.14.The model defines the force, QB, as well as the net force, F33, and the average stress, (3s.33, supported by the fastener midsection:
Shear Joints in the Bearing Mode
35
Figure 2.14. Stress contours for the rivets of aluminum, single rivetrow lap joints, Pl/D = 5 , Ds/t = 4, o = 65 MPa: (a) 013stress contours, standard head, (b) 011stress contours, standard head, (c) 033stress contours, standard head, and (d) 033stress contours, 100"countersunk head (Model 4s8 and 4C9).
where DB= 1.55 Ds and (F33 /Q) is defined by Figure 2.15. For the rivet model with standard heads, Ds/H = 2, and (3 = 0.2, the above relations yield F33 = 0.45 Q, and this is close to the value derived from the finite element model in Chapter 6 (F33 = 0.44 Q).The authors believe this force model offers useful approximations for fasteners with different shapes. The four sets of loadings produce complex distributions of stress illustrated in Figure 2.16 which is derived from the stress contours of Figure 2.14a. The shank is loaded eccentrically and the distributions of shear and axial stress are antisymmetric. High axial stresses produced at the shank periphery near the headshank corner are 3x the average tensile stress on the shank midsection. The peak axial stresses are produced by the stress concentrations at two locations: the headshank junction corner and the roots of threads near the nutshank
Structural Shear Joints
36 1
al
2
0 Y '0
.2 0.5 m
E
0
z
0 0
1
2
3
D slH
Figure 2.15. Variation of the fastener head axial forcetofastener load ratio QB/Q (see Figure 2.1Id), and the average shank midsection forcetofastener load ratio, F33/Q, with the diametertolength ratio Ds/HI for lap joint fasteners with standard heads.
junction corner9. The present finite element models and Figure 2.16 do not offer reliable descriptions of the peak stresses at these locations because the finite element mesh is too coarse to model the fillet.The following expression for (TS*, the peak axial stress, employs the approximation that the peak and average shank midsection stresses are proportional: = B: (~s*/(~s.33 (TS* = (4/n)B[(F33/Q)/Ds2]Q or (SS* = (4/x)B(F33/Q) (Pl/Ds) (t/Ds) (T
(2.10A) (2.10B)
The quantity, B, was evaluated by fitting Equation (2.10A) to the fatigue test results (R = 1,l I N 5 2 10') reported by Sharp, Nordmark and Menzemer [37] for a 7075T6, single rivet lap joint (Pl/Ds = 5.3, t/Ds = 0.34) fastened with standard head aluminum rivets of
'For uniform, tensile loading of the shank. these stress concentrations are related to rF/Ds, the fillet radius (or root radius) toshank diameter ratio' [38,39].Specified headshank fillet radii for bolts correspond with r/Ds = 0.04 and an SCF = 4; thread root radii with 5.7 < SCF < 7.5 [39].There are two other complications: first, the stressed volumes of these stress concentrations are very small, and secondly, in many cases of interest, local stresses reach and exceed the fastener yield stress. As noted in Appendix B, this tends to reduce the effective SCF.
37
Shear Joints in the Bearing Mode

160
2
r
2
120
section 11
.s CI
d
80
s
M
g!
\section
\
22
40
80 1 
0
4
2
6
Distance (mm)
Figure 2.16. The axial, 033stress distributions in the shank of a standard head rivet in a wide, single fastenerrow lap joint, P1/D = 5, Ds/t = 4, CJ = 65 MPa, corresponding with the stress contours in Figure 2.12.
different materials (2024T3,2117T3,6053T61and 1100F).Accordingly, B = 2.8 for 1 IN I lo3and B = 4.5 for lo5 I N I 2 lo8. Equation (2.10) is used in Chapter 3.2 and 4.4 to relate
the performance of fasteners to their fatigue strength. However, it must be recognized that the generality of Equation (2.10) is uncertain; the quoted values of B are highly approximate and may not apply to steel bolts. Lap Joints, Countersunk Head. The countersunk head drastically alters the way forces are applied to the fastener and the resulting stresses. The axial component of the force transmitted to the underside of the countersunk head at location 2A in Figure 2 . 1 3 ~is
Structural Shear Joints
38
TABLE 2.7. INFLUENCE OF RIVET HEAD SHAPE ON PANEL SCF FOR SINGLE RIVETROW LAP JOINTS (P1/D = 5, D/t = 4) RIVET HEAD Standard head IOO"countersink to t/2 100"countersink to t/2 IOO"countersink to full thickness 61.6"countersink to full thickness
RIVET MATERIAL aluminum aluminum steel aluminum aluminum
TILT ANGLE
3.6" 4.2" 4" 4.0" 4.5"
SCF
F.E. MODEL
6.1 9.8 8.9 12.1
3s1 3cI 3c2 3C6 3c5
10.5
substantially reduced. This occurs because the inclined surface of the panel pulls away from the mating head when the panel is loaded and because only a component of the bearing pressure is directed axially. At the same time, intense axial forces are generated on the lagging side (location 5 ) when the wedgeshaped panel presses against the inclined surface of the head. As a result, the tensile stresses on the shank are not symmetrically distributed across the shank midsection but are skewed to the lagging side (Figure 2.14d). The distribution leads to higher peak shank tensile stresses in the countersunk rivet. The inplane component of the contact forces at location 5 produces a radial compression and a dishtype distortion of the top of the head (location 6). Both of these effects allow the upper panel bending to proceed under the rivet head, and this elevates the panel SCF (refer to Chapter 2.4).
Influence of Fastener on Panel SCF. As already noted in Chapter 2.4, fastener configuration and properties affect the panel net section SCF. Table 2.7 lists results for five different rivet shapes. Compared to the SCF for a standard head, the SCF for a 100"countersinkto'/Zpanelthicknessrivet is 61Yo higher. This is obtained because the bulk of the bearing load is applied to the noninclined part of the countersunk, top panel, the face of the hole between z = 0.5t and z = t, accentuating the stress concentration in the panel at z = t. In addition, the countersunk head allows more panel bending to proceed under the rivet head. A stiffer but otherwise identical steel rivet reduces the SCF by 10%. Countersinking to full thickness produces a further 23% increase in the SCF even though it is accompanied by slightly less tilting. This may arise from a further skewing of the bearing and tensile stress distributions toward the panel interior face. A 61.6"countersinktofullthicknessrivet favors a more uniform distribution of stress in the thickness direction. However, this shape is close to headless, allowing more tilting and bending under the head, and delivers a high SCEThese findings show that effective clamping by the rivet head combined with a uniform loading along the shank serve to reduce the panel SCF. Stresses in Fasteners. Estimates of the peak cyclic stresses generated in the fasteners of common, riveted aluminum and bolted steel lap and butt joint configurations are listed Table 2.8. The comparison reveals that the peak stress amplitudes for both the aluminum and steel butt joint fasteners and the aluminum lap joint fasteners are below the peak values in the panels; those for the steel lap joint exceed the peak stress in the steel panel. The
Shear Joints in the Bearing Mode
39
TABLE 2.8. ESTIMATES OF THE PEAK STRESS AMPLITUDES PRODUCED BY THE BEARING MODE IN COMMON STEEL AND ALUMINUM BUTT AND LAP JOINT CONFIGURATIONS
' Estimates apply to center panels of l:2:1butt joints
* Panel gross section stress
Peak panel stress amplitude, o.*=oa (SCF) For 2fastener row joint, the fastener load, Q,=O.So,Plt Average force on fastener midsection produced by tilting, F.,jj, derived from Figure 2.13. For aluminum lap joint (D,/H)=2, Fa,,3=0.45Q, and for steel lap joint (D,/H)=0.75, Fa.1~0.68Qa Peak bending stress amplitude, o,*=[4HQa/nD;] Stress amplitude produced in shank by tilting, o,*=3o,,,,=3F,,j,/0.7854D,Z * Stress amplitude produced by the stress concentration at the headshank and nutshank junctions, 0,*=1.330,,31*
'
'
lap joint fasteners are more highly stressed than butt joint fasteners. The peak stresses in the aluminum rivets are lower than those in the steel bolts. This can be traced to the 67% higher stresses applied to the steel joints and the 3fold larger Ds/Hratio of the aluminum rivet configuration, which is practical because of the lighter gages of aluminum panels. The implications for fatigue are examined in Chapter 4.4.
CHAPTER
3
CLAMPING, INTERFERENCE, AND MICROSLIP, SELFPIERCING RIVETS 3.1 THE CLAMPED, FRICTIONAL OR SLIPRESISTANT MODE OF BUTT AND LAP JOINTS
Defining the Clamping Force (Bolt Tension). The stress concentrations in a shear joint in the clamping mode depend on both friction and the clamping force or bolt tension, Qc, (Equation (1.2), Chapter 1.4). Clamping is obtained when the preassembly shank height', Ho. is less than 2h, the combined initial thickness of the two (or three) panels. The shank must then stretch during assembly to accommodate the misfit. The clamping force, Qc, is the elastic restoring force, which is related to E, the elastic strain of the shank after assembly:
Where E = (H  Ho)/Ho,H is the shank length after assembly, E is the Young's Modulus, and As is the cross sectional area of the shank. The average shank tensile stress is2:
While the key variable for clamping is the shank strain, E, it is convenient to use the nominal clamping, %CL, which is easy to evaluate, as a measure of E:
%CL = 100 (2to  Ho)/Ho
(3.3)
The distance between the rivet heads or between the bolt head and retaining nut *The tensile stress generated on the shank midsection of a clamped fastener is 50% higher at the shank surface than in the center.
41
Structural Shear Joints
42
But %CL, the percent misfit before assembly and %E, the percent misfit after assembly, are not identical. The shank strain is smaller than the nominal clamping because the shank extension is one of three accommodations to the preassembly misfit: i. The extension of the fastener shank: AH = (H  Ho) = E Ho ii. The compression of the panels by the fastener heads: 2At iii. Local deformation of the fastener hole edge and the fastener head at the headshank junction: AHL.The deformations arise from intense contact pressure at the fastener hole edge is illustrated in Figure 3.l(a). The percent shank strain is the nominal clamping reduced by the panel compression and the local deformation. %E
= %CL  100 (2 At/Ho + ~ A H L / H ~ )
(3.4)
The task of evaluating %E is difficult and has been approached empirically. For example, Bickford [40] has proposed an expression for the &Ho/2At ratio3, but without the value of AHL,neither the relation between %E and %CL nor the clamping force are defined. Chesson and Munse [41] Sterling et al. [42] and Christopher, Kulak and Fisher [43] have dealt with this problem by “calibrating” steel bolts. They measured the strain in the shank for given amounts of preassembly misfit related to the amount of bolt tightening (number of nutturns). The calibration defines both %E and %CL, but in the absence of values for the panel compression and the local deformation, the findings are difficult to generalize. The authors have devised an alternative treatment described in Chapter 18 that models the fastener and panels as linear springs. The analysis defines the shank strain and the clamping force for given amounts of nominal clamping. It also provides estimates of the relative contributions of shank strain, panel compression and local deformation. Results obtained for different joints are summarized inTable 3.1.These show that the effective clamping is about 30% to 45% of the nominal clamping. Clamping Residual Stress Field. Clamped panels are host to a residual stress field that interacts with the stresses introduced when the joint is loaded. For comparable E, Ho and to, the residual stress fields in butt and lap joint panels are similar. This residual stress field is axisymmetric and displays a prominent, annular region of intense normal compression under the fastener head (Figure 3.la) as well as circumferential and radial inplane compression at the outer edge of the hole, and an annular ring of circumferential and radial inplane tension that peaks at radius, r = 2.0 rH (Figure 3.lb and c). The field varies in the thickness direction; it is more intense at the top of the cover panel than at the top of the center panel. The examples of the 01 and 02residual stresses obtained on the top surface of the cover panel in Figure 3.1 correspond with the level of clamping (%CL = 0.85, %& = 0.41) employed in steel joints. When the joint is loaded the circumferential residual stresses contribute to the 01 1stress concentration located at r = 2 . 0 r ~as shown in Figure 3.2a and 3.2b. For this reason, the SCFs associated with the clamping mode increase with the amount of clamping.
2AtkHo = Asli/Ac and Ac = rr/4 [(DB+ 0.1 H)*  DH*]where Ac is the effective area of contact under the bolt head and DBand DHare the diameters of the bolt head and the fastener hole, respectively
Minimum principal stress.
03,
provides a sense of contact pressure due to clamping. (a)
Maximum principal stress, q,gives a sense ofDee contours. q is identical to oeeforr ? 1.4 H r at e= 900.
(b)
Intermediate principal stress, fi, similar to a,for r ? I . I m. (c)
Figure 3.1. Principal stress contours of the cover panel residual stress field produced by the %C1 = 0.85 clamping of a wide, steel, 1:2:1 butt joint, P1/D = 5, Ds/t = 4, with standard head fasteners: (a) 0 3 , (b) 01 and (c) 02 (Model 3s3).
TABLE 3.1. DISTRIBUTION OF ACCOMMODATIONS TO THE INITIAL CLAMPING MISFIT I MATERIP
JOINT
H,
D,
CLAMPING D,
(mm) (mm) (mm) Aluminum Aluminum Steel
3.06 6.12 6.12 108
6.12 6.12 6.12 22
9.79 9.79 9.79 33
%CL
SHANK
DEFORMATION DISTRIBUTION (%)
Misfit STRAIN
(mm) 0.5 0.0153 0.5 0.0306 0.85 0.052 1.4 1.3
Shank Anal.'
%E 0.15 0.24 0.41 0.35
' Anal. Analyses and results in Chapter 18 and Table 18.1 FEA  Finite element analyses Exp.  Experimental determination for a A354BD bolt (43)
43
I Panels I
MODEL
Locat
1 FEA2 I E x ~ Anal.' . ~ ~ I Anal.' 4s30
3
4 5
*458E+O7 +263E+07
+7m~+m
(4 Figure 3.2. The 01 1stress distributions for a wide, single rivetrow, steel butt joint panel in the clamping mode (PI/Ds = 5 , Ds/t = 4, %CL = 0.85, %E = 0.41 and p = 0.2): (a) Residual stresses (0= 0), (b) Clamping mode stress field for (5 = 126 MPa, and (c) Post transition stress field for (3 = 200 MPa with relatively weak clamping mode and strong bearing mode components and (d) Post transition field for o = 260 MPa with dominant bearing mode component (Model 3s4). 44
Clamping, Interference, Microslip, and Selfpiercing Rivets
45
A with clamping (actual) without clamping
m (4
I
‘
clamping pre.msion, oco 0
Figure 3.3. Schematic representation of the variation of net section stress, ON, with applied stress, 6,showing the effect of clamping: (a) butt joint, (b) lap joint. The friction attending the clamped mode can support an applied stress, o = OC. When oc is exceeded, the panels of “idealized” joints will macro slip into the bearing mode, alleviating the net section stress. In actual joints, microslip produces small elevations of the net section stress when o < oc, microslip, micro tilt, and local deformation postpone the transition to macro slip to o = OMC.
Stress Carrying Capacity of Fkiction Tractions. When the clamped joint is loaded, interfacial tractions are generated along the clamped interfaces and the applied load is transmitted from paneltopanel and fastenerheadtopanel by friction. Initially, to a first approximation, no load is transferred to the fastener shank. Increases in net section stress arising from shankpanel contact are absent; the net section stress remains fixed at the residual stress
Structural Shear Joints
46
TABLE 3.2. NOMINAL STRESS SUPPORTED BY THE FRICTIONAL TRACTIONS OF CLAMPED B U l T AND LAP JOINTS JOINT TYPE
&'
QC2 (kN)
Butt joint, steel, H0=6.12 mm Center Panel Cover Panel
0.0041
Butt joint, Al, H0=6.12 mm Center Panel Cover Panel
0.0024
Lap joint, Al, H,= 3.06 mm
0.0018
25.12
125 300
1.2 2.8
28 28
27 67
I .3 3.1
27 22
57
1.9
25
5.00
3.53
I , &shankstrain 2. Q,fastener tension 3. a,applied stress supported by frictional tractions of clamping mode (Equation 3.5) 4. o,,applied stress corresponding with transition from clamping to bearing mode
5. f,,fraction of applied stress supported by bearing mode when o=q; %f,,=lOO(slope of aNacurve)/SCF,
level, as shown schematically in Figure 3.3. The most stress that can be supported by the friction tractions of clamped joints, OC, is4:
where Q c = E E ASH(Equation (3.1)), cp is the number of interfaces transmitting frictional tractions? cp = 2 for butt joints and for lap joints with relatively rigid fasteners. The values of oc that can nominally be supported by clamping are listed in Table 3.2 for the joints and conditions evaluated here.
Clamped ModetoBearingMode Transition. When the applied stress exceeds the value of panels are expected to slide (undergo macroslip), ending the clampedmode or slipresistant phase. Further increases in applied stress would then be transmitted by the sliding panels to the fastener shank in the bearing mode accompanied by the intensification of the OC, the
Assuming idealized Coulomb friction. These are the interfaces that allow the joint t o slip into the bearing mode. In lap joints with relatively rigid fasteners, two interfaces, the panelpanel interface and the interface between the underside of the fastener head and the panel, must slip (9= 2). In lap joints with relatively compliant fasteners, slip at the fastener headpanel interface is obviated by the shearing of the fasteners (9= 1).
Clamping, Interference, Microslip, and Selfpiercing Rivets
47
net section stresses and SCF. The transition is expected to be marked by a distinct change in slope of the (TN vs (T curves from zero slope to a slope equal to the SCF, as shown schematically in Figure 3.3. The transitions displayed by the finite element models of the clamped joints, illustrated in Figure 3.4, depart from the idealized picture in three ways:
1. The net section peak stress is not fixed in the clamped state but increases slowly with applied stress. 2. The transition is not abrupt. 3. The stress corresponding to the transition, (TCM, is higher, and in some cases close to 3x the value of (TC. The origins of these departures are identified in the next section. Microslip, MicroTilt and Local Deformation. As load is transferred across the panelpanel interface by the frictional shear tractions, stress is gradually transmitted to portions of panels under the fastener head and around the shank. The stressed parts of the panels strain elastically, producing small relative displacements or microslip, which bring the panels into bearing contact with the fastener shank. As a result, a slowly growing portion of the fastener load is transmitted in the bearing mode while the joint is fully clamped. The calculations indicate that 26% of the applied load is transmitted by the bearing mode in the fully clamped condition6.This is accompanied by the formation of a corresponding “net section” SCF and the increase of ON with applied stress while the joint is in the clamped state as illustrated in Figures 3.2b, and 3.4a and 3 . 4 ~The . formation of a net section SCF in the clamped state is expected for joints with no clearance between the fastener shank and panel hole as is the case for riveted connections. Bolted connections with clearance can accommodate microslip without panelshank contact, and this is expected to delay bearing contact and the development of the net section SCF until (TC is exceeded. Microslip, by transmitting part of the load to the shank without reducing the capacity of the frictional tractions, adds to the stress the joint can support in the clamping mode. This . other elevates (TCM, the stress at the clampedtobearing mode transition, by ~ 2 6 %Two effects, “microtilt” and the local deformation at the fastener head panel hole contact, also elevate the transition stress. Frictional tractions applied by the lap joint panels to the underside of the fastener heads tilt the fastener small amounts. The “microtilt” elevates the contact pressure at the corner of the fastener head thereby increasing the frictional tractions. As noted earlier in this chapter and illustrated in Figure 3.la, clamping produces intense pressure at the fastener headpanel hole edge contact. The pressure deforms the hole edge and displaces the underside of the head by a small amount into panel hole. The authors believe the resulting interlocking of the fastener and the panel interferes with onset of the bearing mode. The interlocking is limited to panels in contact with the fasteners, including both lap joint panels but the cover panels of the butt joint, but not the butt joint center panel. Consistent with this, Table 3.2 illustrates that the elevation of the transition stress, OCM/OC, is small for the butt joint center panel, large for the butt joint cover panel and lap joint panels, and increases with the amount of clamping.
The percent of the applied load supported by the bearing mode, %fBM, is the slope of the ON  o curve in the clamped state divided by the bearing mode net section S C F %fBM = 100 slope/SCFN
Structural Shear Joints
48 2000,
+Net Section, Loading *Net Section, Unloading e Gross Section, Loading +Gross Section, Unloading
1500
L 1 E. 1000
B 500
0
1
!
50
500
100
150
200
250
300
350
400
o (MPa)
A (a)
5.0
6
4.5 4.0 3.5
Net Section
3.0 z
rn
2.5
2.0
1.5
1.o ClampingModified Net Section 00
7
0
50
100
150
200 250 o (MPa)
300
350
400
(b)
Figure 3.4. Variations with applied stress of the peak net section stress, gross section stress and corresponding SCFs for a clamped (%CL = 0.85, %E = 0.41), wide, single fastener row, steel butt joint panel, Pl/D = 5 , Ds/t = 4, (a) and (b) center panel. (figure continues)
49
Clamping, Interference, Microslip, and Selfpiercing Rivets 1600
1
1400 1200
E+
Net Section,
o
Gross Sectio Gross Sectio
E
1000
p" 800
E. 8
8
600 400 200
0
7
400 200
J
a (MPa)
3.5
3.0 I
2.5

2.0

Net Section
v)
Gross Section
0.0
c 0
50
100
150
200
250
300
350
400
a (MPa)
(4 Figure 3.4. (continued) (c) and (d) cover panel (Model 3S4), [22].
Clamping Mode Stress Field. When the clamped joint is loaded, additional stresses are superimposed on the clamping residual stresses and this produces a distinct clamping mode 01 1stress fields in the panels. With increasing applied load, this stress concentration associated with the residual stress field intensifies and rotates toward 8 = 90" (the loading direction) and a second concentration emerges at 8 = 0" & 180" and r = rH. Both of these
50
Structural Shear Joints
features are visible in Figure 3.2b which describes the field obtained when the fastener load reaches the value that can be supported by friction Q = Qc. Under these conditions, elevated stresses are found in three characteristic locations:
1 . Net Section (butt and lap joints): 2. ClampingModified Net Section (butt joints): 3. Gross Section (lap joints):
8 = 0" & 180" and r = rH. 0 < 8 < 65" & 180 < 8 < 135" and r = 2.0 rH. 8 = 90" and r = 1.5 rH.
where r = 1.5 rH represents the distance to the fastener head edge and r = 2.0 rH. a radial beyond the fastener head. The SCF appropriate for the fatigue of clamped joints is defined in terms of the elevation of the stress range (rather than the peak stress): SCF" = (o* ORESIDUAL)/G. This definition is employed in Figure 3.4 and 3.5 and in Tables 3.23.5. The definition is more complicated when the minimum of the stress cycle applied to the joint is none zero. The likely location of the crack initiation site: net section, modified net section or gross section depends on both the stress range SCF and the mean stress which is affected by the local residual stress. The high levels of clamping employed in steel joints produce higher residual tensile stresses in the cover panels of 1:2:1 butt joints than in the center panel. These contribute to higher Values of the peak stresses, mean stressvalues and the stress ratios, R7 in cyclically loaded joints but do reduce the stress amplitude. There is a tradeoff between elevated mean stress and reduced stress amplitude when clamping is presentboth must be considered in design. This is illustrated in Figure 3.3. The higher mean stress and Rvalues render the cover panels more vulnerable to failure than the center panels. As is the case for the bearing mode, the panel bending of lap joints shifts the net section and gross section SCF to the faying surfaces (z = t). The variations with applied stress of the peak stresses and SCFs at the faying surface of a clamped lap joint are described in Figure 3.5a and 3.Sb; the values of the dominant SCF are listed in Table 3.3. These results demonstrate that the SCFs attending the clamping mode are substantially lower that those for the bearing mode: 66% and 40%lower for single fastener row butt joints and lap joints, respectively. In summary, the following points are particularly noteworthy when clamping is present:
1. The contact pressure underneath the fastener head is nonuniform. It increases with applied stress. 2. Microslip and bearing are possible as soon as external stress is applied when nonzeroclearance fasteners are used. 3. In terms of primary load transmission mechanism, two modes are possible: clamping and bearing. But in terms of stress concentration, three physical locations are significant: gross section, clampingmodifiednetsection and net section. All three Dhvsical locations must be monitored. 4. The transition from the clamping to bearing mode with increasing applied stress is difficult to relate to the onset of macroslip or sliding in the joint. Combined ClampingPlusBearing Mode Regime. Beyond OCM only the bearing field intensifies. As the bearing field becomes a progressively larger component of the combined
'The stress ratio R = GMIN/GMAX
Clamping, interference, Microslip, and Selfpiercing Rivets
51
1000 900
800
+friction
coefficient = 0
+friction
coefficient = 0 2
+friction
coefficient = 0.4
700
k
’
600
500 400
300 200 100 Lt”LtYI
0
20
40
60
80
100
120
140
160
120
140
160
u (MPa)
(4 60
50
40
z
30 v)
20
10
00 0
20
40
60
60
u (MPa)
100
(b)
Figure 3.5. Variations with applied stress of the peak net section stress, and net and gross section SCFs for a clamped (%CL = 0.5, %E = 0.18), wide, single fastener row, aluminum lap joint panel, P1/D = 5 , Ds/t = 4,for different values of the friction coefficient: (a) net section stress, and (b) net and gross section SCF (Model 4329), [22].
field, the net section SCF increases, gradually approaching the value obtained in the absence of clamping. An example of the “combined” clamping and bearing field is illustrated in Figure 3.2~.It displays a dominant net section and a weak clampingmodified net section stress concentration. The corresponding variations of the peak stresses and the SCFs are illustrated in Figure 3.3. For the butt joint center panel, the fraction of the applied stress
Structural Shear Joints
52
TABLE 3.3. VALUES OF THE DOMINANT SCF FOR CLAMPED BUTT AND LAP JOINTS, AND LAP JOINTS WITH SELFPIERCING FASTENERS C (mmIGN) dor=2 o/o,=3
BUTT JOINT, CENTER PANEL PlID=5, PIIDB=3,D/t=2
’,1.7
1.5 I, 2.2
3.4 I
4.4
1.8 I, 2.0
1.7 I
2.4 I
Single fastenerrow, aluminum, p=2 1 MPa BUTT JOINT, COVER PANEL P,/D=5, PlIDB=3,D/t=2
1.9
3.4 I
4.4
Single fastenerrow, steel, q=107 MPa
5.5
I
3.6
I
3.4 I
Single fastenerrow, aluminum, r+=21 MPa
5.5
I
3.5
I
5.9
Single fastenerrow, steel, q=107 MPa Two fastenerrows, steel, q=107 MPa
MODEL
3s2 3s4 3s3
I
I
LAP JOINT, PI/D=5, PI/DB=3,D/t=4 Single fastenerrow, aluminum, r+=l 5 MPa 3.6 4.4’ 4.3 I WIDE SINGLE FASTENER ROW, 57540 ALUMINUM LAP JOINTS WITH CARBON STEEL, SELF PIERCING RIVETS, a=55.6 MPa (44 13.7 __ __ PIIDs=15, D/t=3 PI/Ds=9,D/t=2.5
12.2
PlIDs=9, D/t=l.67
16.7
I
’
__ 
__ _
Net section Clamping modified net section Gross section
TABLE 3.4. COMPARISON OF THE SCFS OF WIDE, 1 AND 2FASTENERROW JOINTS IN THE BEARING AND CLAMPING MODES; PI/D = 5, P f l = 5 Joint Type
SCF Irow joint
2row joint
SCFBp
FE MODEL
2.5
3s1
29
2.5
4SII5S1
0
1.8
3S2,3S4
% change
BEARING MODE Butt joint, Al 6.316.4 center panekover panel
4.5
Lap joint, Al
4.4
6.1
30
‘
CLAMPING MODE Butt joint, steel center panel
1.8
1.8
1. Estimated using superposition method described in Chapter 17
53
Clamping, Interference, Microslip, and Selfpiercing Rivets
TABLE 3.5. ESTIMATES OF THE PEAK STRESS AMPLITUDES PRODUCED IN TYPICAL ALUMINUM AND STEEL BUTT AND LAP JOINTS IN THE CLAMPING MODE
Ds, m m H. mm
Qa, N Fa,33r N BE BEN DING*, MPa ~ ~ . T I L T I N G *MPa , G,TILT+SCF*, MPa om*,MPa FS
a
6.12
I
19.1
I
6.12
I
19.1
I
I
5512 0 Ob, 29‘
182 82
5512 3800
0 0
Ob,8‘ Ob, 10‘
Ob, 13‘ Ob, 17‘
my
“UY
“OY
’GY
25
60
25
30
182
0 Ob, 3‘ 0 0
__
__
refer to Table 2.8 for calculational details with clearance without clearance
transmitted by the bearing mode when cs > CJCM is approximated by (1 oc/o).Accordingly, the value of the net section SCF in the transition region is:
where the SCFBis the stress concentration produced by the bearing mode alone, and the factor 6 = 1.1,corrects for stress field overlap. Figure 3.2d illustrates the field obtained when the applied stress is 2x the value of (TCM and the bearing mode dominates. The variation in stress during cyclic loading (illustrated for the highest applied stress in Figure 3.3b) displays stickslip hysteresis as a result of the frictional tractions. It appears that hysteresis attending clamping reduces the local stress variation during repeated load cycling. These findings have important implications. They show that the benefit of the clamping mode, the reduced SCF and reduced stress range, persists after the capacity of the clamping mode has been exceeded. The SCFs produced by the clamping mode are expected to display P ~ / D Band  DB/tdependencies similar the P1/D and D/tdependencies displayed by the bearing mode (Figures 2.9 and 2.10). Butt and lap joints display smaller excess compliance values in the clamping mode compared to the bearing mode (Table 12.10). While the enhanced stiffness leads to a less uni
54
Structural Shear Joints
form distribution of fastener loads in multirow joints it does not elevate the SCF at the leading row of holes of a butt joint. The effects of clamping on contact pressure and microslip at the fastenerpanel and panelpanel interfaces are described in Chapter 3.3.
Double Row Butt Joints. The SCFvalues for the leading row of holes in clamped, single and double fastener row butt joints are presented in Table 3.4 and compared with single and double row lap joints in the bearing mode. Doubling the number of fastener rows of an undamped lap joint the SCF of the by B Y 0 , and a similar reduction is expected for the undamped butt joint. However, the finite element calculations reveal that the same doubling has virtually no effect on the SCF of the center panel of the clumped butt joint. This appears to be a consequence of the low value of the SCF of the clamping mode and the nearly identical SCFBP,the corresponding bypass SCF (see Chapter 17). The estimate of the S C F B ~ derived from the single and double row results, SCFBP= 1.8. is smaller than the corresponding value, SCFsp = 2.5, for bearing mode joints. This is reasonable since the fastener hole is shielded from the bypass stress in clamped joints. While clamping offers large reductions in the SCF of the butt joint, the benefits of multiple rows are sacrificed.
3.2 FASTENERS IN THE CLAMPING MODE
The forces supported by fasteners in the fully clamped condition have two components. One arises from the small part of the total fastener load, about 26%, which is transmitted to the shank by the bearing mode in the absence of clearance. This produces the same type of shear, bending and tension stress distributions as described for the bearing mode in Chapter 2.6, but with a nearly 4fold reduction in the peak stresses. For installations with clearance, this bearing mode contribution to the clamped state is eliminated almost entirely. The second component is the axial tension in the shank produced by clamping and described by Equation (3.2.).These stresses are elevated by the stress concentrations at the head and nutjunction corners and thread roots. For static loading, the two sets of stresses are simply superimposed. For cyclic loading, the bearing mode stresses cycle about the invariant clamping stress which can be viewed as the mean stress. This implies that clamping, without clearance, produces a nearly 4fold reduction in the amplitude of the cyclic stresses experienced by the shank, and a 100% reduction with clearance. But clamping also introduces high level high mean stresses. Estimates of the fastener stresses in the clamping mode are listed in Table 3.5 and can be compared with stress amplitudes produced by the bearing mode under comparable conditions in Table 2.8. These tables illustrate that both the peak panel and peak fastener stress amplitudes are reduced by clamping. Cyclic stresses in bolts with clearance are expected to be vanishingly small, however, the peak mean stresses at the headshank and nut shank corners are elevated to levels that approach or exceed the fastener yield strength.
3.3 HOLE EXPANSION, SQUEEZE AND INTERFERENCE
The fatigue strength of a shear joints in the bearing mode is improved by the cold, forced expansion of the panel hole. The benefits are related to the plastic deformation and residual
Clamping, Interference, Microslip, and Selfpiercing Rivets
55
stresses that are introduced by the expansion of the hole. The stresses, in turn, are affected by differences among several methods for producing the expansion. Mandrel. An oversize mandrel is forced through the hole before the fastener is installed [45]. The pressure acting on the hole face is released when the mandrel is removed. Elastic deformation is recovered but the portion of the expansion associated with plastic deformation and the attending cold work and residual stresses remain. Upset and Squeeze. A large squeeze force is applied to the driven end of a rivet to plastically upset (and expand) the rivet shank as the head is formed [34,48,47].In this case, elastic expansion of the shank is recovered and part of the pressure acting on the hole face is released when squeeze force is released. The portion of the hole expansion produced by the permanent expansion of the shank and attending stresses in the panel remain. The relations among squeeze force, the upset, and the amount of hole expansion which depend on the rivet material and dimensions, have been measured and calculated by Muller [34] and Szolwinski and Farris [46]. Interference. A fastener with a shank larger than the hole or a “taperlock’’ fastener whose shank expands during installation is inserted and remains in the hole. There is no release of the pressure on the hole face and the expansion and panel stresses produced during installation remain. A key parameter for the three methods is the initial hole expansion, %X, (obtained before pressure release) defined as:
%X = 100 (D  Do)/Do
(3.7)
where D and Do are the final and initial diameter of the hole. For cases where elastic modulus of the mandrel or the interference fastener is much higher than the panel, the hole expansion corresponds with the interference: %I = 100 (Ds  Do)/Do
(3.8)
Where the fastener and panel possess the same modulus, the expansion is reduced by the elastic contraction of the fastener shank. %C8[48] and:
%OX= O S ( 1 + p) % I
(39)
Axial Variation of the Hole Expansion. The hole expansions produced by the upset and interference methods can vary along the axial (thickness) direction of the fastener hole. Variations of the expansion are obtained even when the interference is uniform and the shank and panel moduli are comparable. The large, rigid fastener head restricts the contraction of the adjacent shank relative to that displayed by the shank at the joint midsection. Figure 3.6a illustrates for 1% interference that the calculated expansion of the hole at z = 0, adjacent to the head, is 50% larger than the value obtained at z = t, the shank midsection. Even larger
* % C = ‘%oX(l v)/(l + V) (48).
Structural Shear Joints
56
I I
I
I
Figure 3.6. Calculated axial variations of the hole expansion produced by (a) 1% interference (4s20) (1) and (b) 18.9 kN squeeze (46). The hole expansion is magnified 1OX.
axial variations have been calculated for the hole expansion produced by upsetting with a large squeeze force [34,46].For the example illustrated in Figure 3.6b, the hole expansion in the panel on the side of the driven head varies by a factor of five. The possible effects of the axial gradients of hole expansion on the residual stresses are not established and are neglected here.The authors and others [34,46] focus attention on the expansion produced at the panel faying surfaces (at z = t) because this is the location of the stress concentrations produced by the bearing mode.
Residual Stresses Produced by Hole Expansion. A high level of contact pressure must be applied to the periphery to expand the hole. The pressure subjects both the panel and the fastener (or mandrel) to radial compression. The expansion of the hole by elastic deformation is accompanied by circumferential expansion of the panel adjacent to the hole and attending tangential tension. The values of p, orand 088 (the contact pressure and the radial and tangential stresses) generated at the panel periphery by elastic deformation are related to the amount of hole expansion [48]: p
=
=  080 = E (%X)/[lOO(l
+ p)]
(3.10)
Clamping, Interference, Microslip, and Selfpiercing Rivets
57
where p is Poisson’s ratio9. The values of Or and 000 decay exponentially in the panel with radial distance from the hole edgelo. The stress state in the rim promotes the onset of yielding at the periphery [49] when P = 0y/2, or when:
%X = (0y/2E) [100(1 + p)]
(3.11)
where oy is the yield stress, or when %X = 0.3 for 2024T3 panels ((TY= 324 MPa). An annular plastic zone surrounding the hole forms with increased expansion, extending into the panel a radial distance, ry.The plastic zone grows quickly,ry/ro = 1.3 at %X = 0.4 to ry/ro = 1.6 at OhX = 0.811, occupying the bulk of the panel under the rivet head under these conditions. The elasticplastic state alters the orand 000stress distributions12.The main changes are illustrated in Figure 3.7: 1. The plastic deformation accompanying hole expansion diminishes the tangential tension within the plastic zone. The tangential stress is 0 0 0 = 0 at the hole edge when %X = 0.613 (or p = oy) and it is 0 0 0 < 0 (compressive) for larger amounts of expansion for when the pressure at the interface is maintained after expansion. 2. For upsetsqueeze hole expansion, the pressure at the interface is reduced (but not eliminated) when the squeeze force is released. Figure 3.7b illustrates that this makes the tangential residual stress acting in the plastic zone more compressive. 3. The complete release of contact pressure with Mandrel type hole expansion is expected to produce even higher values of tangential compression and a diminution of the tangential tension away from the hole. 4. The peak tangential tension shifts from the periphery to the plastic zone boundary. 5. For large values of hole expansion, i.e. 0.6 < %X < 3.0, the plastic deformation tends to increase the panel thickness. Clamping by the rivet heads resists the growth of panel thickness and leads to the formation of outofplane compressive residual stresses in the annular region, 0.2 < r/ro < 0.6 [34]. As a result, the portion of the load applied to the joint that is transmitted by the clamping mode increases with the amount of hole expansion. Calculations by Muller [34] indicate that with %X = 3, as much as = 40% of the applied load could be transmitted by the clamping model4. A different model for evaluating the clamping stress produced by squeeze and unloading is treated by Deng and Hutchinson [50].
Equations (3.10) and (3.11) apply to 2dimensional problems, neglect friction and are valid for a large circular, elastic panel with a small hole. when the amount of interference is uniform along the axial direction of the fastener shank and around the circumference [48]. They approximate the conditions in a shear joint panel. l o For elastic behavior, oee = ar= p(r/ro)z where ro is the hole radius and r the radial distance from the interface t491. l 1 Estimates derived from 2dimensional finite element analyses for elasticperfectly plastic material behavior, oy (2024T3) = 324 MPa, p = 0.2, and multirivet constrains along the panel edges. In the absence of such constraints, the zone grows exponentially [49,50]: ry/r = exp [(p/ay)  0.51. l 2 A 2Danalysis of hole expansion without pressure release for elasticperfectly plastic behavior offers the following relations [49]: or= p + oy ln(r/ro) when ro I r < ry and or= 0.5ay(r/y1ro)~where y~ = exp[(p/oy)  0.51 when r > ry, and oee = (ay  p) + oy In(r/ro) when ro S r 5 ry and = 0.5oy(r/y1ro)~where y~ = exp[(p/oy)  0.51 when r > ry l 3 For 2924T3 Al with ay = 324 MPa. l4 The estimates apply to a three rivet row lap joint subjected to a cyclic stress of oa = 40 MPa [34].
Structural Shear Joints 1.2
1
7
0.8
0.8
0.4
0.4
*
** o E iz
____
U
_ *  .
.fim 0.4 
pE 0.8
'I
*E o iz U .8 0.4 m
E
/
z0
0.8 20, Elastic +H+

20, ElasticPerfectlyPlastic
30, ElasticPlastic, pressure partially released ~~
1
2
3
rlro
Figure 3.7. The variation with radial distance from the edge of the fastener hole in a 2024T3 panel (oy = 324 MPa) of the radial and tangential residual stresses, or and 0613, produced by different amounts of hole expansions, %X:(a) the residual stresses produced by 2dimensional, elasticperfectlyplastic deformation [49], and (b) the residual stresses produced by 2dimensional elastic deformation, 2dimensional elasticperfectlyplastic deformation [49], and 3dimensional, elasticplastic upset followed by the release of the squeeze force [34].
Effects of Hole Expansion on Bearing Mode Stresses. The tangential residual tensile stresses produced by hole expansion can be viewed as a mean stress to which bearing mode cyclic stresses are added when the joint is loaded. The net effect is not a simple addition. For the case where the panel remains elastic, Figure 3.8 shows that while the residual tension increases with hole expansion, the net section SCF (the slope of the o vs ON curve) decreases markedly. Stress contours produced by elasticplastic behavior when bearing mode stresses are added to the interference stress field are illustrated in Figure 3.9. These also show that hole expansion and attending plasticity completely remove the net section stress concentration at the hole edge. The peak cyclic stress variations are a small fraction of the applied cyclic stress and their location is shifted radially away from the hole to the plastic zone boundary [34]. Large stress variations are replaced by cyclic plastic deformation. The net effect is a dramatic improvement in the fatigue strength of shear joints which is described more fully in Chapter 4.3.
Clamping, Interference, Microslip, and Selfpiercing Rivets
59
1000 1
0%
900 800
700
e
0.3%
A
0.6%
600 m 500
B
400 300 200
0
20
40
60
80
100
120
140
160
u (MPa)
Figure 3.8. The influence of the nominal stress, 6,and 0.3% and 0.6% interference (0.2% and 0.4% hole expansion) on the peak net section, tangential stress, ON, for fully elastic behavior of an aluminum butt joint panel. The results are for a 2D analysis of a wide, single row joint, P1/Ds = 5, Ds/t = 4 fastened with aluminum pins (Model 3P40).
There are two additional effects of hole expansion. The attending residual stresses reduce the joint excess compliance. This produces modest increases of the fastener load generated at the leading row of holes. The elevated contact pressure at the shankhole interface together with friction acts to reduce microslip and fretting. This is described in the next section. 3.4. CONTACT PRESSURE, MICROSLIP AND TANGENTIAL STRESS
Variations of contact pressure, microslip and tangential stress around the periphery of the fastener hole in a butt joint are illustrated in Figure 3.10.These results, obtained in the bearing mode, are derived form elasticplastic calculations, and illustrate the complexity of the distributions. The bearing mode produces relatively high contact pressures with relatively steep gradients along the circumference. Peak values of microslip (Figure 3.10~)are found at locations with little contact pressure (Figure 3.10a). The peak value of tangential stress (Figure 3.10b) corresponds with the site of the SCF. In lap joints, the variations of contact pressure, microslip and tangential stress are similar but are affected by panel bending. The largest values at the hole periphery are obtained at z = t, adjacent to the interior panel surface, as shown in Figure 3.11. For comparable geometries and loads, the peak values of contact pressure, microslip and tangential stress are generally higher for lap joints than for the
:
+I.=
:
+1.12 E+13g +B.WE+07
:
E
a
:
+7.!37 E+07 +6.33EW +475E+U7 +3.14 7 +1.53 E+07
.
+1.51 E+@3 +I.%E+CB + I . 17 E+CB +i.m~ + ~ 1 8 e.33 E+07 +6.&1E+07
:
: : :
:
c4.94€+07 7
:
+3.ww
:
+ I 5 5 E+07  1 47 E+(3B
I
4 4 4 + 4 4 4 4 4 4
T
Figure 3.9. The maximum principal stress contours surrounding the fastener hole in a 2dimensional mode of a wide, singlerivet row, 2024T3 aluminum butt joint, Pl/Ds = 5 , Ds/t = 4, (TY = 324 MPa for aluminum rivets installed with 0.6% interference (0.4% hole expansion): (a) residual principal stress contours after hole expansion, and (b) principal stresses after hole expanded panel subjected to a nominal stress, (T = 54 MPa (model 3P41). Righthand figures show inner section magnified x 2.
60
200
100
90
45
0
45
90
135
180
225
270
225
270
e (degrees) (a) urnW a )
6oo
1
100
~
200
90
45
0
45
~
90
135
180
e (degrees) (c)
Figure 3.10. The variation of (a) contact pressure, (b) tangential stress and (c) microslip around the periphery of a wide, single fastenerrow,pinned butt joint panel (P1/D = 5 , D/t = 4, Model 3P25) in the bearing mode for an applied stress, o = 125 MPa.
62
Structural Shear Joints
+z=O.loading 0 z=O,unloading Et z=0.5t, loading C z=0.5t,unloading z=t.loading A z=t,unloading
100
0 90
60
0
30
30
60
90
60
90
0, "
(4
07' 90
'
60
I
"
0
30
0
I
30 c>
(b)
Figure 3.11. The variation of (a) contact pressure, and (b) microslip around the periphery of a wide, single rivetrow, standard head, aluminum lap joint panel in the bearing mode as a function of the depth, z, P1/Ds = 5 , Ds/t = 4, p = 0.5, (3 = 125 MPa (Model 4s1).
Clamping, Interference, Microslip, and Selfpiercing Rivets
63
TABLE 3.6. VALUES OF THE CONTACT PRESSURE, MICROSLIP AND TANGENTIAL STRESS GENERATED UNDER THE FASTENER HEAD OF A LAP JOINT IN THE CLAMPING MODE (Pi/Ds = 5, Ddt = 4, D f l s = 1.6)
butt joint. The influence of clamping on the contact pressure, microslip and tangential tension generated directly under the edge of the fastener head is described in Table 3.6. Figure 3.12 summarizes the effects of first installing 1% interference (0.65% hole expansion) in an aluminum butt joint panel, then loading the panel to a stress, CJ = 125MPa, and finally unloading. Before hole expansion, contact pressure at the interface and tangential tension in the adjacent panel are absent. Loading the panel produces a peak microslip of 6 = 60 pm at the 8 = 30" and 150" locations. The expansion produces high contact pressures and tangential stresses and these are intensified in some locations when the joint is loaded (Figures 3.12a and 3.12~).Friction combined with the high contact pressures lead to a 5fold reduction of the peak microslip and the microslip the amounts of microslip (Figure 3.12b). The implications for fretting wear and fatigue are examined in Chapter 4.5 3.5 SELFPIERCING RIVET
The selfpiercing rivet has a countersunk head and a hollow shank. In selfpiercing riveting (SPR), a joint is formed by forcing the highstrength tubular rivet through overlapping panels of a softer material using the axisymmetric punch and die arrangement illustrated in Figure 3.13 [44]. The upper sheet is pierced through its entire thickness by the rivet and the lower sheet is pierced only partially. Piercing forces also cause the lower sheet to flow into the die cavity locally and conform to the cavity shape. The piercing operation naturally produces interference, clamping and intimate frictional contact. In addition, the dimplelike, outofplane contours of the panels, similar to those seen in joints formed by the clinching process, resist the shearing of the panel and interfere with the transfer of the fastener load to the rivet shank. The inplane shear tends to produce lateral panel separation, tension in the shank and a clamping action by the rivet. Consequently, the performance of SPR joints has similarities to conventional rivets installed with interference and clamping. Consistent with this, the FEA analyses show that the peak stresses are generated at the 8 = 90" location under the rivet head, essentially the same location found for fully clamped, frictional mode load transfer [44].The SCFs calculated for three SPR joints are listed in Table 3.3. It should be noted that the calculations for the selfpierced joints account for neither the clamping, interference nor the compressive residual stresses introduced by the piercing operation. For this reason, they probably overestimate the SCFs of the joints.
600
500
400
2 $
300
(0
e 200
100
180150120 90 60 30
0
30 60 90 120 150 180
H"
(a)
U 0%, Unloading
+ 1%.Loading b
60
r

r
180150120 90 60 30
&
hterlerence Step
.A
Unloading
0
30 60 90 120 150 180
200 150
50 0
W
50 100
I$
180150120 00 80 30 0
30 60 90 120 150 1 0
0v (C)
Figure 3.12. Influence of 1% interference on (a) contact pressure, (b) microslip and (c) tangential stress for a wide, single rivetrow, aluminum butt joint, PI/Ds = 5 , Ds/t = 4,p = 0.5, o = 125 MPa (Model 2P26). 64
Clamping, Interference, Microslip, and Selfpiercing Rivets
65
Figure 3.13. Schematic of the punch and die arrangement for installing self piercing rivets. The clamping force, P2, is applied to prevent lateral movements as the punch forces the rivets through the sheets [44].
Some perspective on the virtues of the selfpiercing fastener is obtained from a comparison with conventional fasteners. To facilitate this, the SCFs displayed by the same selfpierced installations in the form of a joint with P1/D = 5 and D/t = 4,are estimated with the aid of Figure 2.9. The adjusted values, SCF = 8, 8.9, and 11.1are comparable to the value, SCF = 8.8, obtained by Iyer (1) for an aluminum lap joint fastened with a conventional, countersunk, steel rivet.
CHAPTER
FATIGUE OF SHEAR JOINTS 4.1 STAGES OF THE FATIGUE PROCESS
Fatigue, the loss of load carrying capacity with repeated loading, proceeds in three stages: (i) crack initiation, (ii) stable crack growth and (iii) fracture. In the crack initiation stage, the repeated cycles of tensile stress and plastic strain progressively damage the microstructure of the material in isolated locations. The accumulated damage ultimately produces a fully formed, microscopic crack. The percycle damage increases either with the local stress amplitude or the mean stress. For this reason cracks initiate at the sites of stress concentration, or sites combining high stresses and intense fretting. Locations of reported crack initiation sites, important for NDE, are identified in Figure 4.1 [34,51541.In the second, or crack growth stage, the crack extends by small, regular, submicron and micron size increments with each repeated loading cycle.The growth trajectory is normal to the direction of cyclic tension. The growth stage ends with the stress cycle that produces a crack length just short of the critical value corresponding with crack instability.The fracture stage proceeds during the next and terminal cycle which produces rapid, unstable extension of the crack, and the rupture of the remaining bridges of unbroken material of either the panel or the fastener. The three stages of the fatigue process are generic for metallic materials and structural components. However, the fatigue failure of structural shear joints can be more complex because it results from mechanical contact at multiple locations between the panels and fasteners and between the panels themselves. The finite element models featured in this text treat the intricacies of mechanical contact. But, the finite element models featured in this text do not contain cracks and so do not model crack growth or fracture. The reader is referred to references [52,55571 for detailed finite element and fracture mechanics analyses of growth.
4.2 FAILURE MODES AND LOCATIONS
Shear joint panels exhibit three distinct fatigue failure modes important for NDE [34,51541; fasteners are vulnerable to two failure modes. These are related to the crack initiation sites. i. Net Section Failure. For joints dominated by the bearing mode without clamping or interference, the crack initiation and stress concentration sites are found near the net
67
(a) 4
4
4
4
4
4
4 I
4 I
4 I
4 I
4 I
4 I
t
t
t
t
t
t
(b)
t
t
t
t
t
t
Figure 4.1. (a) Reported fatigue crack initiation sites observed on the faying surfaces of butt and lap joint panel: Locations 13 are observed for clamped aluminum and steel joints [51541, with Locations 12 close to the leading edge of the fastener head, Location 4 is observed for aluminum joints with interference [34], and Location 5 is observed for steel and aluminum joints with relatively low levels of interference and clamping [52]. (b) SCF locations computed in butt and lap joints with interference. The SCF moves from the 8 = 0" to 8= 45" with increasing applied stress. (c) SCF locations computed in butt and lap joints with clamping. The boundary of the fastener head is indicated by the dotted line. 68
69
Fatigue of Shear Joints
Stress Concentrations
Stress Concentrations
A
Stress Concentrations . .
Figure 4.2. Schematic representation of the net section, the clamping and the hole expansionmodified net section and the gross section modes of panel fracture. The connection between the location of the SCF and the fracture path is illustrated: (a) Net section mode for bearing mode joints, (b) Modified net section modes for joints with clamping and interference, and (c) gross section mode for clamped lap joints with large hole expansions and fretting fatigue failures [34,51541.
section locations (Figure 4.la) at the faying surface. These sites may also exhibit fretting wear. Fatigue cracks formed at these locations extend into the panel in the twodirection (normal to the loading direction) and in the threedirection (towards the exposed panel surfaces). They either intersect adjacent fastener holes or merge with cracks initiated at the adjacent holes. This produces the type of panel fracture shown in Figure 4.2a. ii. Clamping and InterferenceModified Net Section Failure. For butt joints with hole expansion and those in the clamping mode, high stresses are generated away from the hole edge at angular locations typically 20" < 8 < 70" (Figure 4.lb). Fatigue cracks formed at these locations extend into the panel the twodirection (normal to the loading direction), and either intersect or just graze adjacent fastener holes or merge with cracks initiated at the adjacent holes. Fretting wear is invariably present in the failure region. This produces the type of panel fracture shown in Figure 4.2b. iii. Gross Section Failure. The dominant stress concentration in lap joints in the clamping mode, as well as the site of intense fretting site for butt and lap joints is located under the fastener head at the gross sectionlocation (Figure 4.land 4.2c), either directly under the leading edge of the fastener head or at the faying surface. Gross section failures are also produced by joints with large amounts of hole expansion, but these initiate at the ) cracks initiated there, grow faying surfaces ahead of the fastener head (r = 2 r ~ Fatigue in the twodirection and tend to bypass adjacent fastener holes. This produces the type of panel fracture shown in Figure 4.2~. iv. Fastener HeadShank Corner or Thread Root Failure. Rivets and bolts harbor stress concentrations at the fastener headshank junction corner and, for bolts, at the thread roots near the retaining nutshank transition (Figure 2.13b). The cracks tend to initiate at these locations, grow normal to the shank axis and truncate the fastener. This is the
70
Structural Shear Joints
likely mode of failure for lap joint fasteners butt joints fasteners with threads exposed to bending stresses [39]. v. Shank Failures. Cracks initiated by the bending of butt joint fasteners will form at the periphery of the shank, half way between the fastener heads (or head and nut), when thread roots are not involved. These cracks will grow normal to the shank axis. This is not a common mode because the panels are likely to fail before the fasteners under these conditions. The mode of failure is a signature of either the dominant mode of load transfer (bearing vs clamping), hole expansion, or fretting fatigue. For clamped lap joints it is difficult to distinguish between conventional and fretting fatigue betause both mechanisms favor the gross section mode. The fatigue lives of joints show a stronger correlation with the SCF, stress amplitude and mean stress rather than the specific mode of failure, and this is examined in Chapters 4.3 and 4.4.
Multiple Site Damage, MSD. The failure of wide shear joints with many fasteners in a row involves a complex evolution in structural response. Cracks do not initiate simultaneously at each fastener hole because of the stochastic nature of the fatigue process and variations in nominally identical fastener installations. The local stiffness of the panel is reduced after one or more cracks emerge from a fastener hole. This changes the distribution of the fastener loads: the load transmitted to the cracked panel hole is reduced while the loads transmitted to adjacent holes (holes not yet cracked) are elevated. As a result, the rate of growth of the local crack slows, and the likelihood of the initiation of cracks at adjacent fasteners increases. This favors a more uniform distribution of fatigue damage, the formation of multiple, cracked fastener holes, referred to as “multiplesite damage” (MSD), [52,58641. It also extends the life of the growth stage. It has been proposed that MSD makes it more difficult for stiffeners to arrest unstable cracks extending in shear joints of fuselage structures (58641. Similarly, in multiple fastener joints with fatigue vulnerable fasteners, the fracture of the first fastener does not immediately compromise the shear joint. However, the failure will transfer more cyclic load to adjacent fasteners with additional fastener failures and load redistribution until the joint severs. 4.3 FATIGUE STRENGTH OF PANELS
Components of the Fatigue Life. The term, fatigue strength, is used here to denote the stress amplitude a component can support for a specified fatigue life, i.e., a given number of stress cycles The fatigue life is the sum of the number of stress cycles attending the initiation and stable growth stages’. For convenience, the crack initiation life is arbitrarily defined here as the number of cycles consumed by the nucleation of the crack and its growth to 1 mmlength.2The crack growth life is the number of cycles consumed by continued growthfrom the lmmlength to instability and fracture.
1 The life of the fracture stage is 1 stress cycle and is negligible. Defined in this way, the initiation life includes the nucleation of the crack and the increment of growth affected by the SCF. It also represents, approximately, the life consumed while the crack is small enough to be hidden by
the rivet head.
Fatigue of Shear Joints
71
In the recent past much effort has been invested in fracture mechanics methods to predict the growth life of shear connections. This is important because the growth life corresponds with the inspection life, the period when cracks can be detected by NDI, and its definition makes it possible to schedule inspections so cracks will be detected before the joint fails. Prediction methods for the initiation life are complicated by the need to define the local stress amplitudes, i.e., the relevant SCF of the joints.
SCFFS Analysis of Shear Joints. A number of worker have demonstrated that the SN curve (stress amplitudecycles to failure relation) of a notched component is approximated by the SN curve of the material divided by the SCF of the notch [65,66]. It is the basis for an estimation procedure, which the authors refer to here as the “Stress Concentration FactorFatigue Strength (SCFFS) Analysis”. The analysis makes it possible to estimate the fatigue strength of components with stress concentrations when: (a) the SN curve for the material (unnotched samples) and (b) the relevant SCF of the joint are known, and provided: (c) any loss of fatigue life from fretting, corrosion and other sources are negligible. Since the SCF is a concept derived from linear elastic material behavior, the method is only reliable as long as stresses within the stress concentration do not exceed the yield stress. The basis for the SCFFS analysis, other limitations and validation of the method are presented in detail in Appendix B. The SCFFS analysis was successfully employed by Seliger [32] in 1943 to derive SCF Values for riveted aluminum lap joint panels from SN measurements. In the absence of independently evaluated SCF values for the panels it was not possible to confirm Seliger’s findings. The SCFvalues reported in Chapters 2 and 3 belatedly validate Seliger’s findings (see Appendix B) and can test the reliability of SCFFS analysis. In the remainder of this sections, predictions of the analysis are compared with fatigue test results for aluminum and steel butt and lap joints in both the bearing, clamping and adhesive modes of load transfer. The comparisons illustrate that the SCFFS analysis can provide useful strength predictions for shear connections when these are subjected to low, nominal stress amplitudes and display fatigue lives, N > lo5  lo6 cycles. SCFFS Analysis of Aluminum Lap Joints Panels in the Bearing Mode. Predictions of the of SN Curves of riveted aluminum lap joints in the bearing mode obtained with the SCFFS analysis are compared in Figures 4.3 and 4.4 with fatigue test data for the joints collected by the Strength and Analysis Group of EDSU [67]. The tests examined multiple rivet and multi row joints involving different PI/Dvalues and stress cycles with different values of means stress. The appropriate SCF values were obtained using the data reported in Chapters 2 and 3 and adjusted for pitch and panel thickness, using Figures 2.9 and 2.10, and number of rows using methods described in Chapter 17. The analyses employ the average material SN curve for the material derived from the range of results reported in the literature (see Figure B.3). The Gerber diagram (Figures B.2) was used to adjust the material SN curve for the mean stress applied to the joint. No information about either the amounts of clamping and interference installed in these joints or the negative contribution of fretting fatigue is available. The reduction of the SCF associated with these sources was offset by neglecting fretting fatigue and the 8% to 10% increase in the SCF for fastener holes adjacent to the free edge. In spite of the uncertainties introduced using estimates of the material SN curve, the predictions are in reasonable accord with the measurements for lives, N > lo6.As is the case for
Structural Shear Joints
72 60
"
1
.
1
1
' ' , , . . ,
,
LAP JOINT TESTS 0 oavs N MEASUREMENTS FOR 2024.T3
mm
ALUMINUM, 2 RIVETROW LAP JOINT! WITH SNAPHEAD RIVETS, P / D = 4 2, D/t=42, am=G9MPa, SCF=42 SCFFL ANALYSIS
 (oa/SCF) vs N CURVE FOR 2.24T3 m
FOR om=G9MPa DERIVED FROM
mo
CONVENTIONAL SN CURVE AND A GERBER DIAGRAM 00
n o
[fLw
0
20 
BRACKET SHOWS SCATIER OF MATERIAL oa/SCF vs N MEASUREMENTS FOR 2024.T3 FOR SCF=l I
0
'
;
1o4
1o5
I
1
1o6
1o7
1o8
60umm
0
LAP JOINT TESTS oavs N MEASUREMENTS FOR 2024 T3
ALUMINUM, 2 RIVET ROW LAP JOINT WITH SNAPHEAD RIVETS,P/D:4 2, D / t = 2 4, om=69MPa, SCF=5 2
40 
onmnmn
ANALYSIS  (o*/SCF) SCFN FL CURVE OF 2024T3 vs
FOR om=69MPaDERIVED FROM I?
z
CONVENTIONAL SN CURVE AND GERBER DIAGRAM
ammm
SCF=5 1
O 1o4
h
) 1o5
, 1o6 N
1
1o7
1o8
Figure 4.3. Comparisons of fatigue test data for 2024T3 aluminum, 12 rivets, 2 rivetrow lap joints fastened with snaphead rivets [30] with the predictions of the SCFFS analysis: (a) D/t = 4 and (b) D/t = 2.4. In each case, the test results are represented by discrete data points. The solid line is the prediction of the SCFFS analysis (Model 5S1), [67701.
73
Fatigue of Shear Joints
*O
I
O F THE MEAN OF 3 UaN
"0
0
CURVES FOR 7075T6 AL, FOR SCF=l
01
0
,
I
1o6
1o5
1o4
1o8
10'
N
(a) ..,
.
.
,
.
.
.
,
(
.
LAP JOINT TESTS
60
m 40
0% vs
cum
N MEASUREMENTS FOR 7075T6
ALUMINUM, 2 RIVETROW LAP JOINT WITH 2017ST3 COUNTERSUNKRIVETS P/D=3.1, D/t=2.1, t=3.00mm, om=60MPa, SCFz6.2 SCFFL ANALYSIS
om
 (oa/SCF)vs N CURRENT FOR 7075T6 AL
a
=
FOR om=60MPa DERIVED FROM THE
BRACKET SHOWS SPREAD O F THE MEAN OF 3 usvs N CURVES FOR 7075T6 AL, FOR SCF=1
0
1o4
A
1o5
,
,
. , . , , A
1o6 N
I
1o7
1o*
(b)
Figure 4.4. Comparisons of fatigue test data for 7075T6 aluminum, 12 rivets, 2rivetrow lap joints [30]with the predictions of the SCFFS analysis: (a) joint with snaphead rivets, (b) joint with countersunk rivets. In each case the test results are represented by discrete data points. The solid line is the prediction of the SCFFS analysis (Models 5s1and 5C1), [67701.
74
Structural Shear Joints
the open hole panels (Figure B.l), the predictions understate the fatigue strength with a growing divergence for shorter lives, N < lo6, when the peak stress exceeds the yield stress. SCFFS Analysis of Steel Butt Joint Panels in the Clamping Mode. Predictions for bolted and riveted steel butt joints in the clamping mode are compared with SN data for the joint materials in Figures 4.5 and 4.6 [53,54,71751. Included are joints fabricated from three grades of steel, A514 (oy = 827 MPa), A440 (oy = 349 MPa) and A7 (oy = 235 MPa). Material SN data for the A514 steel is from the same plates used to fabricate the joints. The SN data for the other steels are taken from the literature and do not correspond with the actual joints. All of the tests were performed on 1:1.6:13butt joints, a design which assured that the fatigue failures would be confined to the center panels because the nominal stresses supported by the center panels of these joints are 25% higher than the stresses applied to the cover panels. The estimates of the SCFs derived for the joints are based on the reported initial bolt tension reduced by 10% to account for relaxation during the fatigue test [74,76].The test results for the riveted butt joint display considerable variability consistent with the observation that in this case the rivet clamping force varied between 5 KN and 89 KN [74]. The SCFFS predictions for the three grades of steel grade agree reasonably with the joint test results in range lo5 < N < 2 x lo6. Calculations summarized in Table 3.3 illustrate that SCFs in the clamped state at the net section, clamping modified net section and gross section locations are comparable. Consistent with this finding, the center panels of the clamped A514 and A440 joints displayed examples of the three types of failures (Figure 4.1). SCFFS Analysis of Aluminum Lap joint Panels in AdhesivePlusBearing Mode. The SCFFS analysis is useful for estimating the influence of sealants and adhesives on the fatigue lives of shear connections [481. This is illustrated in Figure 4.7 for 3rivet, single rivetrow, 7075T6 aluminum lap joints assembled with a lowmodulus, polymer sealant at the panelpanel and fastenerpanel interfaces. The SCFvalues for the sealed joints were obtained with the Thin Adhesive Layer Analysis (TALA) and the sealant properties described in Chapters 14 and 15 [6,21].The SN curve of 7075T6 is adjusted for the mean stress and different SCFvalues. The SCFreduced SN curve intersecting a particular joint test results (oa,N) defines the SCFvalue attributed by the SCFFS Analysis. The numbers next to the data point are the SCFs of the joints calculated with the TALA. The results in Figure 4.7 show that the two sets of SCFs agree to a good approximation. Consequently, both the fatigue tests and the TALA/SCFFS analysis show a low modulus sealant can produce a  10fold improvement in the fatigue life. Analogous findings for bonded steel joints have been reported by Albrecht and Sahli [77]. SRFFS Analysis of Aluminum Lap Joints with Hole Expansion. The residual stresses and local plasticity introduced by hole expansion and described in Chapter 3.3 produce substantial improvements of the fatigue strength of shear joints. Findings for the effect of hole expansion on the fatigue strength of aluminum lugs are summarized inTable 4.1 [7880].The lugs are loaded like the center panel of a butt joint with hole expansion produced with steel pins or bushings installed with interference. The conditions examined include small amounts
1:1.6:1 are the relative thickness valus of the butt joint covercentercover panels.
Fatigue of Shear Joints
1
~ 5 1 STEEL, 4 CLAMPED BUTT JOINTS IN 2 CONFIGURATIONS
300
' r
*O0
Dm
75
..
vs N FOR3/4 IN THICK
( J ~
A514 STEEL PLATES (R=O,SCF=l) SCFFS ANALYSIS (oa/SCF vs N FORA514)
A514 STEEL CLAMPED BUTT JOINTS FATIGUE TESTS
 0 2ROWS, 4A490 BOLTS R=O, 1.6<SCF<17 3ROWS, 6A325 BOLTS looR=O, 1.7s SCF S 1 8 0
U '
1o3
'
'
'
'
'
"
1
1
1o4
1o5 N
.,
1o6
10'
, . , , . .
A440 STEEL, CLAMPED BUTT, JOINTS A440 STEEL PLATES, R=O(ESTIMATED) SCFFS ANALYSIS
=
0 FATIGUE TESTS O F CLAMPED
440 STEEL BUTT JOINTS
brn
0
1o3
1o4
1o5 N
1o6
10'
(b)
Figure 4.5. Comparison of fatigue test data for clamped, steel butt joints with the predictions of the SCFFS analysis (a) AS14 steel butt joints with A490 bolts [52],and (b) A440 steel butt joints with A325 bolts [S3,54,7173].
Structural Shear Joints
76
ATSTEEL, RIVETED AND CLAMPED BUTT JOINTS
cr2vs N FOR A7STEEL
PLATES, R0 SCFFSANALYSIS (0. /SCF) vs N FOR A7
150
FATIGUE TESTS OF RIVETED
L
L
0
1o3
1o4
.
~
1os
1o5 N
1o7

~~,_
_ m m ~
A7STEEL, BOLTED AND CLAMPED BUTT JOINTS

200 
 o2
vs
..
h r tJm
150oy
N FOR A7 STEELCC'\
PLATES, R=O
SCF FS ANALYSIS (aa/SCF) vs N FOR A7
FATIGUE TES'I'S OF CLAMPED A7 STEEL B U I T JOINTS, R=O
**. 5.2
100
C,
Cl 2 ROW, 2 BOLTS JOINTS 1 7 5 SCF 5 2.0 0 2 ROW, 4BOLTS JOINTS
50
0
c)*@*.
m
.._.
SCF=1 6
.)
I 
..= ._..._
1.75 SCF 5 2.0
1
1
,
Y
Figure 4.6. Comparison of fatigue test data for clamped, A7 steel butt joints with the predictions of the SCFFS analysis [737.51.
,
80
,
I
7075T6 RIVETED LAP JOINT FATIGURE TESTS AND SCFFS ANALYSIS
 S N CURVES FOR DIFFERENT
70
SCFVALUES
1 OOmmTHICKPANELS,STD HEAD
0 NOTSEALED 0 SEALED 1 53mmTHICK PANELS,STD HEAD 0 NOTSEALED H SEALED 1 O O m m THICK PANELS,CTSNK HEAD
60
50
omax=oY
TABLE 4.1. INFLUENCE OF INTERFERENCE AND HOLE EXPANSION ON THE FATIGUE STRENGTH OF ALUMINUM LUGS [7&80]
__
I t=9.0 mm DTD363A' a=44.45 mm d=19.05 mm t9.02 mm
0.2 0.4 0.56' 0.6 1.o
77
28 34 47 56
I
I [77,791
I
Structural Shear Joints 50
~
s
A 40
.
~
I
0
z W
a 30

3
0
I
+Std. Head, Ds=4.85mm, t=2.3mm
2 L
20
A
I
z W
3
$ 10
.d
n
z
0 7
I
Ctsk. Head, Ds=4.00mm, t=l.6mm Ctsk. Head, Ds=4.85mm, t=2.2mm
A.
X (%) corresponding with onset of yielding
B.
X (%) correspondingwith formation of compressive tangential stress at hole edge
1
A B
1
2
3
HOLE EXPANSION, X (%)
Figure 4.8. Improvements of the fatigue strength (stress amplitude at N = 3X105 cycles) of 3 rivetrow, 2024T3 lap joints produced by hole expansion after Muller [43] and Szolwinski and Farris [46,47].
of interference (or hole expansion), i.e. < 0.4, that preclude the development of compressive residual stresses and local yielding. In these cases, the improved fatigue strength can be linked with the reduction in the net section SCF as illustrated in Figure 3.8. The variation of the increase of the fatigue strength of lap joints with hole expansion produced by upset and squeeze reported by Muller [34] and Szolwinski and Farris [46,47] are summarized in Figure 4.8. In this case, increases of the fatigue strength are not obtained until the hole expansions exceeds %X = 0.3% to 0.4% which correspond with the onset of yielding and the formation of compressive tangential stresses at the hole edge. It appears that the relaxation of residual stress that accompanies the release of the squeeze forcea relaxation absent when expansion is produced by interferencereduces the benefits of hole expansion. Figure 4.8 shows that the fatigue strength increases rapidly with hole expansions in the range 0.3< %X<0.7. The smaller improvements obtained with larger expansions may be related to the increasing amount of clamping attending hole expansions %X > 0.7. The improvements produced by upset and squeeze hole expansion involve stress states that cannot be characterized with an elastic SCF (see Chapter 3.3). As a temporary expedient, an empirial strength reduction factor (SRF) is used to here to express the relation between the material SN curve and that of the joint4. The SRFvalues appropriate for multiple row lap joints fabricated with different amounts of hole expansion and tested by
79
Fatigue of Shear Joints 240

0 X0.4%; 10% improvement
220

A X0.7%; 25% improvement
200

180
L
XI %; 30% improvement 0 XI 5%;35% improvement
~
160

140

E. 120 100 . .S_R.......... _F q
.....
60
20 40
0
1
I
1
1.OE+04
,



ScF4.6
I
,.
....  .......  6..........    F.....  .............................     .m.. .....9.. 
SRF=4 .... .. ..'......'.......
,
n .
.
~
A Y
......... .P.. .................
..............
I
,
1.OE+05
1.OE+06
N (cycles)
Figure 4.9. Fatigue strength of 2024T3 aluminum lap joints fastened with rivets installed with different amounts of upset and squeeze leading to different amounts of hole expansion after Szolwinski and Farris [46,47].The elevations of the fatigue strength produced by hole expansion are expressed in terms of the diminished values of the strength reduction factor (SRF).
Szolwinski and Farris [46,47] are identified in Figure 4.9. The SRFvalues for a particular hole expansion vary with stress amplitude and increasing amounts of local yielding similar to the deviations from a fixed SCF noted in Figure B.l. SRFFS Analysis of Aluminum Lap Joint Panels Fastened with Selfpiercing, Steel Rivets. The finite element analyses of lap joints fastened with selfpiercing rivets (Chapter 3.5) model the shape of the joint and the fasteners after piercing. They do not treat the residual stresses introduced by the piercing operation or subsequent plastic deformation during loading. The authors believe the stressstrain states generated in these joints are analogous to those produced by hole expansion and clamping (Chapter 3.3) and, unlike the F.E. models, do not lend themselves to characterization by an (elastic) SCF. For this reason, Figure 4.10 employs the strength reduction factor (SRF) introduced in the previous section to describe the joint performance and the SCF to characterize the behavior of the finite element models. The fatigue tests of 57500 Aluminum lap joints fastened with selfpiercing steel rivets, taken together with the SN curve for the material [44,81], reflect strength reductions in the range 5 < SRF < 7, as shown in Figure 4.10. The stress concentration factors, SCF = 12.2,13.7 and 16.7, derived from the finite element analyses are more than two times these values and grossly understate the fatigue strength of the joints. The discrepancy emphasizes the inadequacy of the elastic SCF when yieldlevel residual stressstrain states are installed in the joint.
Structural Shear Joints
80
30"8
*\ '8
2
=Drn
SINGLE RIVET, 45mm WIDE 5754 0 ALUMINUMLAP JOINTS FASTENED WITH CARBON STEEL SELF PIERCING RIVETS ~
20 
 SCFFSANALYSIS
(oa/SCF vs N FOR 57540AL)

FATIGURE TESTS OF JOINTS P,/D=ll3,D = 4 m , t=lmm,SCF=13 7
SRF=6
&a_,
Figure 4.10. Comparison of fatigue test data for narrow, single fastener 57540 aluminum lap joints fastened with self piercing, carbon steel rivets [81] with the predictions of the SCFFS Analysis [44].
4.4 FATIGUE STRENGTH OF FASTENERS
Estimates of the stress amplitudes generated in riveted and bolted butt and lap joints are summarized in Tables 2.8 and 3.5, and relevant generalizations are offered in Chapters 2.8 and 3.1. The fatigue test results for aluminum and steel joints in Figures 4.3 to 4.6 represent cases where the failures proceeded in the joint rather than in the fasteners. Estimates of the cyclic stresses generated in the panels and fasteners of joints similar to those of Figures 4.34.6, and for comparable conditions, are listed in Table 4.2. The two examples offer insights into the factors contributing to the extended fatigue of the fasteners in these cases.
Aluminum Lap Joint. The riveted aluminum lap joint described in Figure 4.4 is similar to the ones for which test data is supplied in Figures 4.3 and 4.4. The joint is subjected to a relatively high mean stress. The estimated peak panel stress amplitude, oa*= 86 MPa is close to the fatigue strength of the panel material corrected for the peak mean, FS 80 MPa, The equality implies a panel life close to N = lo6 cycles.The estimated peak fastener stress amplitude, oa* = 28 MPa, is below the estimated fastener fatigue strength, FS74 MPa (corrected for the om*= 140 MPa mean stress). This is consistent with a fastener life N > lo6 and the finding that the fasteners outlast the panels.

Clamped Steel Butt Joint. The panels are subjected to a peak stress amplitude close to the fatigue strength of the steel panels in Figure 4.5 consistent with a panel life of N = lo6 cycles. The clamping subjects the bolt to a yield stresslevel mean stress, om*= 845 MPa. According to the Gerber diagram, for a yieldlevel mean stress (90% of the ultimate
Fatigue of Shear Joints
81
TABLE 4.2. ESTIMATES OF THE PANEL AND FASTENER STRESS AMPLITUDES AND FATIGUE STRENGTHS FOR JOINTS AND CONDITIONS COMPARABLE TO THOSE OF FIGURES 4.3 AND 4.5 JOINT TYPE Bearin
n ,, MPa .  PANEL STRESSES AND FATIGUE STRENGTHS
' Wide joint with 2 rows of rivets, P1=30.6mm, Ds=6.12 mm, H=3.06 mm
* Wide 1:1.6:1joint with 2 rows of fasteners, Pl=66.9 mm, Ds=19.1 mm, H=28.6 mm Stress applied to center panel Fatigue strength adjusted for applied mean stress The 2 values quoted are for 2024T3 and 7075T6, respectively Approximate value for A514 and A440 steel panels Peak value produced in shank by fastener tilting, o,,33*=3Fa,33/ a D 2 * Estimate of peak value at beadshank junction and thread root stress concentration, cra*=3o,33* For bolted joint with shankhole clearance l o For riveted joint with no clearance I ' Peak mean stress For hardened steel nut and given level of mean stress
'
strength) the hardened bolt still retains about 20% of its fatigue strength, or FS 60 MPa. This is more than adequate for a joint with clearance for which the peak stress amplitude is vanishingly small and accounts for the survival of the bolts. However, the peak stress amplitude generated by a tight fitting bolt or rivet is close to the FS and could this could lead to occasional fastener failures. In the absence of clamping and for a lower applied stress (oa= 50 MPa instead of 100 MPa, see Table 2.8), a hardened bolt is expected to survive, but the highly stressed panel will fail prematurely. 4.5. FRETTING WEAR AND FATIGUE
Fketting Wear. Repeated loading of structural shear joints produces fretting: microscale cyclic slips (relative toandfro movement) at the interfaces between panels and fasteners. Depending on the contact pressure, slip amplitude, surface finish and lubrication and the number of load cycles, fretting can produce significant amounts of abrasive wear. The
82
Structural Shear Joints
Figure 4.11. Locations in a shear joint subject to fretting damage. Locations A (for butt joints) and A’ and B (for lap joints) at the shankhole periphery are active in the bearing mode. Location C and C’ in butt joints and C’ in lap joints are active in the clamping mode.
generation of wear particles is promoted when slipping regions are exposed to high contact pressure along with high tangential tractions.The locations of the interfaces susceptible to fretting wear in joints with standard head fasteners have a bearing on NDE and are illustrated in Figure 4.11. The inclined portion of the head on the leading side of countersunk fasteners is also exposed to high pressures and large slips. The amount of wear expressed by the depth of the wear scar is proportional to the fretting wear parameter, F1, which is defined in Appendix C. Figure 4.12 illustrates, for the bearing mode, the variations of F1 in a lap joints around the periphery of fastener hole for different amounts of clamping and interference. The largest amounts of wear are to be expected in the locale of the peak F1values which are obtained in the vicinity of the netsection location. For joints in the clamping mode, the largest values of contact pressure are obtained directly under the fastener head at the headpanel interface, particularly at the leading edge of the head. Large pressures are also obtained at the panelpanel faying interfaces under the fastener head. Peak values of F1 and the corresponding depths of the wear scar are summarized in Table 4.2. For stress amplitudes that provide relatively long fatigue lives, Nm5 cycles, the estimated depths of wear scars are in the range 0.4 pm < y < 3ym at locations A and A’, and 3 pm < y < 30 pm at location C. Under these conditions fretting wear in the absence of corrosion is not expected to be a serious problem. Fretting Fatigue. The process by which fretting reduces the fatigue life of contacting parts, called fretting fatigue, is described more fully Appendix C. The locations in shear joint interfaces where conditions may favor fretting fatigue are identified in Figure 4.10. Many workers, including the present authors and Birkemoe et a1 [53,54] have observed fretting wear debris at the bolt headpanel interface of steel butt joints (location C ) , and conclude from this that fretting “contributed” to the fatigue failure of these joints. The conclusion is open to question because fretting is not always accompanied by crack initiation. To shed more light on the possible role of fretting fatigue, the values of the fretting fatigue parameter, F2, at locations A, A’ and C (Figure 4.11) have been calculated for butt and lap joints. The origin, use and limitations of F2 as a rough, orderof magnitude indicator of the likelihood of fretting fatigue is discussed more fully in Appendix C. The variation of F2 at
83
Fatigue of Shear Joints 2.5 
j : 3
0 F t , 4s21 W ZZt.4822
2.0 
E cd
A Z=1,4823

1.5
B i
1.o
I
0.0 90
60
30
0
30
60
90
0,
(a)
1
T
1
8o 70
i
6o

B
40
1
/
0 z=t, 4s20 H
A
II
I
9 30
20 10
0 90
60
30
0
(bj
z=t, 4822 Z=t, 4823
30
!
60
90
Figure 4.12. Variation of the fretting parameters with angular location and amounts of interference and clamping for wide, singlerivetrow,aluminum lap joints with standard head rivets (Models 4Sl9,4S20,4S21,4322and 4s23):(a) F1 fretting wear parameter and (b) F2 fretting fatigue parameter.
Structural Shear Joints
84
TABLE 4.3. ESTIMATES OF THE PEAK VALUES OF THE FRETTING WEAR, F1, AND FRETTING FATIGUE PARAMETER, F2, FOR JOINTS AND CYCLIC STRESSES OFFERING EXTENDED CONVENTIONAL FATIGUE LIVES
I
P1=30.6mm, PIIDs=S F2fretting fatigue thresholds: Aluminum 4.210’ Pa’m, Steel 50*109 Pa2m
the panel periphery with angular location is illustrated in Figure 4.12b. The peak values of generated by aluminum and steel butt and lap joints for 2row joints and stress ampli. tudes that normally assure a long fatigue life are listed in Table 4.3. Values for butt and lap joints at locations A and A at the periphery of the panel hole are below the “ ~ n d e r s t a t e d ” ~ threshold for fretting fatigue. Hole expansion (interference) markedly reduces the severity of fretting at the panel hole periphery. Note that under these conditions, crack initiation does not usually occur at the hole periphery, but in the interior.The findings indicate that fretting fatigue at the A and A locations is unlikely in butt and lap joints with standard head fasteners but more likely with countersunk rivets in the absence of hole expansion. For the same local value of F2, conditions for fretting fatigue of clamped panels with standard fastener heads are believed to be more favorable at C , where the rubbing of the fastener leading edge is accompanied by a steeper pressure and tangential stress gradient, than at C’ at the faying surfaces. Similar conditions are obtained in lap joints with standard heads in the absence of clamping as a result of panel bendingh. High contact pressures and tangential stresses are not obtained at the leading edge of a countersunk rivet which is more compliant.Table 4.2 shows that the F2values generated by clamped aluminum and steel butt joints are below the threshold. The F2values for the clamped and unclamped aluminum lap joint are close to or just exceed the threshold, respectively. For the special conditions evaluF2
The threshold values apply to the fretting conditions produced by a steep pressure gradient at a sharp edge similar to the conditions under the edge of the fastener head at location C (Figure 4.1 I).They “understate” the threshold at the periphery of the fastenerhole interface, locations A and A’. where the attending pressure gradients are shallow by comparison. There is no gradient in butt joints in the bearing mode because the contact pressure between the head and panel top surface is negligible.
Fatigue of Shear Joints
05
ated here and in the absence of hole expansion, the conditions at location C pose a marginal risk of fretting fatigue of lap joints in the bearing mode and both butt and lap joints in the clamping mode.. Three examples of fretting fatigue documented in the literature illustrate the difficulty of making generalizations about the conditions favoring fretting fatigue. 1. Fretting Fatigue of a h o w , countersunk riveted lap joint’ [34]. The fasteners were installed with a very large squeeze force (hole expansion, %X = 2.6) which produces a high, peak contact pressure at the faying surface, p = 100 MPa. Fretting conditions at the exposed surface of the “front” panel are not severe because the contact pressures under the leading edge of a countersunk head are not intense. Intense contact pressures are produced under the driven head of the same rivet. However the tangential stresses and slips generated at this locationthe Zagging row of holes of the “back” panel are reduced. Consistent with this, Muller [34] observed fretting fatigue at the faying surfaces on the leading side of the fastener at location C. The joint displayed a life of N = 4.8 x lo5 cycles at a stress amplitude of oa = 46 MPa and nearly twofold increase in life when a 0.1 mm PTFE sheet is inserted between the faying surfaces. However, the PTFE sheet failed to improve the life of joints with smaller amounts of hole expansion and correspondingly smaller contact pressures, presumably, because the role of fretting fatigue was diminished in these cases. 2. Fretting fatigue of a double strap, bolted butt joint8. Sharp, Nordmark and Menzemer [37], report that the unpainted butt joints joints supported a stress amplitude of 0, = 45 MPa (R = 0.33) for N = lo7 cycles. A zinc chromate primer applied to the fuying surfaces increased the fatigue strength 60%. The relatively high stress amplitudes supported by this joint require large values of bolt tension and a high level of clamping The reason fretting proceeded at the faying surfaces is not clear. Relatively thick cover panels (their thickness was not disclosed) would have shifted the peak tangential stresses to the center panel. 3. Fretting fatigue of a 3 rivet, single rivetrow lap joint9. In this case, Fretting fatigue proceeded at the faying surfaces (location B, Figure 4.11) where the sharp, curled edge of the fastener hole (at E) rubs against the adjacent, interior panel face [82].The curled edge has the potential of producing a high contact pressure and the steep pressure gradient that promote fretting fatigue. Figure 4.13 shows that the accompanying fretting wear produces a (dark) crescentshaped damage zone at the periphery of the fastener hole. Cracks initiated near the 26” and +206” locations where the fretting damage and the net section stress concentration overlap, locations relevant for NDE. This example of fretting fatigue involves special circumstances.The lap joint was subjected to a relatively high stress amplitude, Oa = 53 MPa and peak stresses’O that produced local yielding at the net section stress concentrations. Figures 4.1 l a and b illustrate that the yielding elongated the fastener holes
’ P I = Pz = 2 0 m m , D s = 4 m m , a n d t = 1 mm. Unpainted, and zinc chromate primer painted 7075T651 joint with 6.35 mmthick test sections. Particulars about the type of bolts, bolt tension, joint dimensions or the relative thickness of the center panel and cover panels are not reported. 91.8 mmwide, 3countersunk rivets, single rivetrow, 7075T6 lap joint, PI = 30.6 mm, P,/D = 5, t = 1.53mm; oa = 53 MPa, R = 0.1 with test interrupted after N = 3261 cycles. l o OMAX = 2 SCF oa = 690 MPa.
86
Structural Shear Joints
Figure 4.13. Examples of fretting damage and fatigue cracks produced in 7075T6 aluminum, 3rivet, single rivetrow lap joints ((3, = 53 MPa, R = 0.1 and N = 3261 cycles), (82).The dark, crescent shaped regions below the fastener hole are produced by the fretting at the panelpanel interface (location B, Figure 4.11). The Bmode of fretting is responsible for the 3 cracks that emerge from the fretted region. The location of the 4th crack (left side of 19b) is consistent with the conventional fatigue at the net section location. The fact that the conventional fatigue crack, left side of (b), and the fretting fatigue crack, right side of (b), are nearly the same length is a sign that fretting fatigue did not curtail the life of the panel.
11%.This facilitated a 15fold increase in the panelpanel slip which formed the wide, crescentshaped damage zone that overlaps with the net section stress concentration. This mode of fretting fatigue did not reduce the fatigue life significantly (see Figure 4.12 caption). The first two examples and the high F2values in Table 4.3 point to clamping, either from bolt tightening or rivet squeeze, as an important contributing factor. Overloading and the loosening of the joint are complicit in the third example. In each case fretting fatigue proceeded at the faying surfaces even though contact pressures and traction gradients are more intense at the panel surface directly under the edge of a protruding fastener head. In each case the joints were subjected to relatively high stress amplitudes. It should also be noted that the SCFFS predictions presented in Figures 4.34.6 do not account for fretting fatigue. Yet, with possibly one exception, they do not overstate the fatigue strength of the joints. While there is little doubt that fretting fatigue reduces the fatigue strength of some joints, it is not a problem common to all joints.
CHAPTER
5 DESIGN CONSIDERATIONS FOR REPEATED LOADING 5.1. MECHANICAL PERFORMANCE
Shear joints subject to cyclic loading are designed to satisfy three types of mechanical requirements: 1. Monotonic Strength. Joints must withstand the infrequent but extreme load conditions without gross yielding or fracture. Design procedures for assuring ultimate strength are described by Kulak [51], Bickford [40] and in other sources [37,83851. 2. Durability or Fatigue Life. Joints must survive the number of stress cycles and the amplitudes and mean stresses they will be subjected to during their design life. In the past, the design specification for durability and fatigue life has been derived from fatigue tests of candidate joints, which is a fully empirical approach. The SCFFS analysis provides a semiempirical approach that can reduce the number of tests required for preliminary design. But the authors do not regard it as substitute for experimental verification. The application of the method, its limitations and validation are covered in Chapters 4.3 and 5.2 and Appendix B. 3. Damage Tolerance. Damage Tolerance is the capability of detecting growing fatigue cracks and repairing or replacing damaged parts before the performance of the joint is impaired. It involves matching the joint design with appropriate NDE procedures and practical inspection intervals.The joint design must provide a crack growth life of duration sufficient for a number of inspections.The number and their scheduling are chosen so that the sum of the probabilities of crack detention corresponding with the instantaneous crack lengths exceeds unity. To accomplish this, the variation of the crack length with number of stress cycles during the crack growth life must be defined. Analytical methods for forecasting crack growth life are treated by Fawaz [55] and others [52,56,57,5944]. 5.2 CONSIDERATIONS FOR JOINT DURABILITY
The selection of a joint configuration capable of supporting a particular stress amplitude and mean stress for a specified number of stress cycles can be facilitated with the SCFFS
87
88
Structural Shear Joints
Analysis (Chapter 4.3). The analysis can be applied to both the panels and the fasteners, although SCFvalues appropriate for fasteners are not as well defined in this text. It is appropriate for joint configurations, materials and stress conditions for which there is no prior service experience. It does require that the SN curves of the panel and fastener material (for unnotched samples) be available. The method involves a number of uncertainties, identified later in this section. In view of this, joint configurations selected with the SCFFS analysis should be regarded as preliminary and require experimental verification, particularly when the public health and safety are involved. Panel Configuration. One of two approaches for selecting a viable panel configuration can be employed: Approach 1. The starting point is the selection of the features of a particular type of shear joint that define the joint SCF including P1/D,D/t, the number of rivetrows,fastener type and load transfer mode. In addition, the service conditions are defined by the cyclic load and stress ratio, R, to be supported by the joint, and the desired cyclic life, N.The nominal stress amplitude the joint can support is defined by the material SN curve (see Figure 5.la): o a (N, joint) = oa(N, material)/SCF.Together with the load amplitude, the stress amplitude defines the gross cross sectional area, and combinations of panel width and thickness. One or more iterations may be required to obtain a panel thickness consistent with the initially assumed D/tvalue. Finally, the dimensions are modified to provide an appropriate factor of safety. Approach 2. In this case, the starting point is the selection of the stress amplitude the joint is intended to support. Again, the cyclic load and stress ratio, R, to be supported by the joint, and the desired cyclic life are identified. Together, the load amplitude and the stress amplitude define the gross cross sectional area, and tentative combinations of panel width and thickness.The maximum joint SCF that can be tolerated is defined by the material SN curve (see Figure 5.lb): SCF = oa(N, material)/o, (N, joint).The next step is the selection of a particular type of shear joint including P1/D, D/t, the number of rivetrows, fastener type and load transfer mode, etc., that satisfies the SCF requirement. Width and thickness are then adjusted to accommodate the PI/D, and D/t of the joint. Finally, the dimensions are modified to provide an appropriate factor of safety. Fastener Configuration. The selection of a preliminary joint configuration also defines the fastener load amplitude, Qa, and diameter to length ratio, the Ds/H. Following the procedure outlined in Tables 2.8 and 4.2, these parameters are converted into an estimate of the peak fastener stress amplitude, oa*.The condition for fastener survivalthe mean stressmodified fastener FS exceeds the oa*is then tested. When the fastener material/configuration does not pass the test, appropriate adjustments in joint configuration or load transfer mode are made and an acceptable joint and fastener are obtained by iteration. Although a safety factor is always used to account for uncertainties, the following known sources of variation peculiar to structural shear joints and the fatigue process in general must be kept in mind. 1. Assembly Variability. The SCFvalues quoted in this text are calculated for idealized assemblies. Variations in the SCF due to dimensional and assembly process variations such as hole diameter, fastener hole misalignment and buckled rivets on a multifastener joint are not known.
Design Considerations for Repeated Loading
89
SN CURVE FOR MATERIAL
t On
oa(N)matenal 
oa(I.J)pme~',(N)mat
+ SCF
SN CURVE FOR PANEL
SN CURVE FOR MATERIAL
t Om
SCF=oa (Nmat + Oa(Nlpmel
Figure 5.1. Schematic representation of the estimation procedures for selecting a joint panel configuration with a specified fatigue strength: (a) Approach 1 and (b) Approach 2.
90
Structural Shear Joints
TABLE 5.1. COMPARISON OF BUTT JOINT AND LAP JOINT FEATURES
' 'I
~
lowe% L  low, M  moderate, H  high, H"  highest
2. Material Variability. The SN curves of structural materials display significant lottolot variability. This is a problem because the available SN curve measurements are rarely for the same lot as the panel material and because the minimum fatigue strength is rarely defined. 3. RRatio. The SN curve of the material must correspond with the mean stress or stress ratio, R applied to the joint'. Material SN data for the Rvalue of interest is frequently not available. In that case, an estimate of the material SN curve for the appropriate Rvalue can be derived from a Gerber diagram (see Figure B.2). However, the approximate nature of the Gerber relation can introduce an uncertainty as large as 20%. 4. The Cyclic Life. The SCFFS analysis is valid for relatively low values of stress amplitude when the peak stress levels within the stress concentrations do not exceed the yield strength: OMAX = OMIN + 20;, < (sy.This condition is obtained for N > lo5 to N > lo6cycles, a range sometimes referred to as highcycle fatigue. Estimates of the fatigue strength of joints for shorter cyclic lives (lowcycle fatigue) tend to be conservative. 5.3 JOINT TYPE AND MODE SELECTION
General features of butt joints and lap joints that affect their selection for service under fatigue conditions are summarized in Table 5.1.
Bearing Mode. For the bearing mode, comparable singlefastener row, 1:2:1 butt and lap joints (same panel thickness, PI/Dratio, fastener design, etc) harbor nearly the same SCF and are expected to display similar fatigue lives. The SCFs of butt and lap joints can be reduced by reducing pitch and adding additional fastener rows at the cost of more fasteners and more overlap, The major difference is that lap joints require half the overlap and half the fasteners of an equivalent butt joint and are therefore lighter. Another difference is that the risk of fretting fatigue is somewhat lower for butt joints than for equivalent lap joints.
Design Considerations for Repeated Loading
91
This advantage is partially offset by the stiffer shankhole interactions (higher k/Kvalues) in butt joints which elevate the lSfrowSCF of multiple row joints.
Clamping Mode. In the case of clamped joints, butt joints possess greater cyclic load carrying capacity than lap joints. In the fully clamped state, the SCF of the single fastener row butt joint is about half the value displayed by the equivalent lap joints. This translates into a twofold cyclic load carrying advantage for the butt joint that can compensate for the extra overlap and fasteners. It should be noted that additional fastener rows do not improve the fully clamped butt joint, but extra fastener rows are expected to reduce the SCF of the clamped lap joint. Another feature unique to the clamped, 1:2:1 butt joint is that the residual gross section tensile stress (mean stress) of the cover panels is higher than the value for the center panel. The fatigue lives of the cover panels are correspondinglyshorter. Optimum utilization of material is obtained from a joint with relatively thicker cover panels, e.g. from a 1.1:2:1.1 butt joint. AdhesivePlusBearing Mode. The results presented in Chapters 2.5 and 4.3 illustrate that the fasteners combined with adhesive offer benefits comparable to the clamping mode. While the findings in these chapters are confined to lap joints, similar improvements are anticipated for butt joints. Fastener Cyclic Stress Capacity. The peak stresses generated in butt joint fasteners in the bearing mode are much smaller than those generated in the corresponding panel. The cyclic stresses produced in lap joint fasteners are much higher and comparable to the peak panel stresses. The clamping mode offers a fourfold reduction in the peak cyclic stresses applied to fasteners installed without clearance, and a nearly complete isolation from cyclic stresses for fasteners with clearance. However, clamping does generate high levels of mean stress in both butt and lap joint fasteners. 5.4 NDE AND FRETTING
Detection of Fatigue Cracks. The stress concentrations of 1:2:1 butt joints are located at the faying, interior surfaces of the front or back cover pane12.The detection of cracks formed in the back cover panel from the vantage point in front of the joint is particularly difficult. To “image” the crack, the NDI probe must penetrate the fastener head, front cover panel and center panel, as well as one fastenerpanel and two panelpanel interfaces. The problem is almost as difficult for lap joints, where the stress concentrations are located at the interior surface of the front and back panel. In this case, the NDI probe must penetrate the fastener head, the front panel and the fastenerpanel and two panelpanel interfaces to detect a crack in the back panel. The detection problem is less severe for lap joints with countersunk fasteners, which restrict the stress concentrations to front panel. The fatigue crack detection problem for butt and lap joints can be eased at the cost of cyclic life by reducing the thickness of the front panels in the overlap region. In this way the
The terms “front” and “back” are used to distinguish between the panels that can and cannot be visually inspected, respectively, when only one side of the joint is accessible (See Figure 1.2).
92
Structural Shear Joints
front panel SCF can be elevated above the levels displayed by the center or back panel. However, the design must assure that the growth lives of fatigue cracks that form in center and back panels always exceed the cyclic life of the joint.
Fretting. Fretting debris is invariably present near already obscured interfacial cracks.The generation of fretting debris increases as a crack grows due to higher local compliance and slip amplitude. The presence of fretting debris in the vicinity of a growing crack can significantly reduce the signaltonoise ratio of the NDI measurement and therefore its reliability. The success of the SCFFS (which neglects wear) for elastic conditions, is a sign that fretting wear has a minor effect on the fatigue strength for large numbers of cycles; N > lo5.For failure under elasticplastic conditions, which corresponds to a relatively small number of slip reversals ( lo3  lo5 cycles), the influence of fretting wear over and above that of cyclic macroplasticity is not known. Definitive understanding of the importance of fretting wear in joints with clamping and interference stresses remains to be developed.
5.5 FAIL SAFE DESIGN
Butt and lap joint panels are vulnerable to failure along the leading row of fasteners or just ahead of it. Such fractures are catastrophic for a shear joint because they completely sever the load bearing cross section. Adding additional fastener rows reduces the stresses at the leading row, but this row is still the most highly stressed and the joint remains vulnerable to catastrophic failure. Multiple row joints do offer the possibility of exchanging some joint life for a fail safe feature. This is obtained with a design that assures that the fasteners at the leading row fail before the panel. Failure of the fasteners does not compromise the panel; the load is simply transmitted to the remaining rows. The nearest row of fasteners assumes the role of the fasteners of the leading and lagging row in a joint with one less row. Although this row must support elevated rivet loads and SCFs, Table 2.5 shows that the demands on the panel at the promoted row are only a little higher than those at the original leading row. While this makes it likely that the promoted row will ultimately suffer the same fate, the fatigue life of the joint will be extended substantially allowing for timely failure detection and repair.
5.6 GENERALIZING FINITE ELEMENT RESULTS
The results of the finite element analyses presented here are mainly for single fastener row, aluminum butt and lap joints with one configuration: P/D = 5 , D/t = 4.The analyses were performed for idealized rivetlike fasteners and examine a limited number of nominal stress levels. The results of analyses that employed linear elastic behavior can provide useful estimates of the SCFs, stress levels, strains and displacements for steel and other joint materials, bolted joints and a much wider range of shear joint configurations and nominal stresses.
Fastener Pitch, Diameter and Panel Thickness. Estimates of the SCF can be obtained for joint configurations in the range 4 < P1/Ds < 8, and 2 < Ds/t < 8, using the relations between these ratios and the SCF derived by Seliger [32] and Fongsamootr [33] in Figures 2.9,2.10 or 5.2. These relations were obtained for the bearing mode. The Pl/Ds dependence was
Design Considerations for Repeated Loading
1
93
STANDARD HEAD
1.4 I I I
\
.
COUNTERSUNK HEAD
LL
0 0
1
0.8 0

8
4
12
 0 0.8
(a)
8
4
12
Dlt
PID
(b)
Figure 5.2. Correction factors for estimating the stress concentration factors, SCFs, of butt and lap joints for 3 < P1/Ds < 13 and 2 < Ds/t < 8 given values for P1/Ds = 5 and Ds/t = 4, (a) variation of correction with P1/Ds after Seliger [32] and variation of correction with Ds/t after Fongsamootr [33].
obtained for single rivetrow lap joints, but is expected to approximate the behavior of multiplerow joints as well. The Ds/tdependence applies only to lap joints and doublers. Relations similar to those in Figure 5.2 may apply to the clamping mode when the dependence is expressed in terms of the pitchtofastener head diameter ratio, P ~ / D B .
Number of RivetRows. Analyses for single fastenerrows can be extended to joints with two, three, four or more rows, using expressions derived from the two springs model and the “superposition” approximation described in Chapter 17. Nominal Stress. Table 5.2 illustrates that for joints with the same elastic material properties, the peak stress scales with the nominal stress to a close approximation and the SCF remains approximately constant. Contact pressures scale within about lo%, excess compliance, fastener tilt and various displacements scale less reliably. The departures arise from and depend on the relative contributions of interface slip and elastic strain to joint distortion. The positive departures indicate that the relative amounts contributed by interface slip diminish as the nominal stress is increased. Applications to Steel and Other Panel Materials. Departures from linear elastic behavior of a steel lap joint relative to an otherwise identical aluminum joint are summarized in Table 5.3. The peak stresses and contact pressures for the steel and aluminum joints are almost
Structural Shear Joints
94
TABLE 5.2. COMPARISON OF LOAD TRANSFER MODES
F.E. MODEL NOMINAL STRESS. MPa
4s8 65
4s 1 125
RELATIVE DEPARTURE FROM LINEARITY, % 4S8,4S I 125
Excess compliance, m/GN Rivet tilt, degrees
32.98 2.5 1
27.46 3.6
17 34
Inplane rivetpanel slip,pm Inplane panelpanel slip,pm Outofplane slip, pm
8.98 48.4 3.7
16.47 91.3 5.9
4.8 1.9 2 1
Peak tensile stress, MPa Peak shankhole contact pressure, MPa
396
767
0.7
453
779
12
TABLE 5.3. RELATIVE DEPARTURES FROM LINEAR ELASTIC BEHAVIOR OF AN ALUMINUM, SINGLE RIVETROW LAP JOINT, P1/D = 5, D/t = 4, ARISING FROM INTERFACE SLIP
F.E. MODEL JOINT MATERIAL NOMINAL STRESS. MPa
4s 1 aluminum 125
4s5 steel I25
RELATIVE DEPARTURE FROM LINEARITY, Yo 4s I , 4s5 steel 125
Excess compliance, d G N Rivet tilt, degrees
28.5 3.6
1 1.72 1.32
22 8.5
Inplane rivetpanel slip,pm Inplane panelpanel slip,pm Outofplane slip, pm
15.35 94.3 6.4
6.39 32. I 2.8
23 0.8 30
Peak tensile stress, MPa Peak shankhole contact pressure, MPa
76 1
766
0.7
859
866
0.8
identical and display no departure. This means that estimates of these quantities derived from calculations for the identical aluminum joint, corrected for differences in nominal stress, are reliable. The excess compliance, tilt and certain displacements of the aluminum joint, modified by the aluminumtosteel elastic modulus ratio, understate the values for the steel joint by as much as 30%. These discrepancies arise because the relative contributions of interface slips to displacement values are larger in the otherwise stiffer steel joint. More accurate estimates can be made by taking the departures into account.
Design Considerations for Repeated Loading
95
Rivets vs Bolts. The proportions of the rivet with “standard” head are similar to those of standard hexagonal bolts:
Shank diametertohead height ratio, Fastener head diametertoshank diameter ratio,
RIVET 1.6 1.6
HEXAGONAL BOLT 1.5 1.5
Results obtained for joints fastened with rivets with the “standard” head approximate joints fastened with snug fitting bolts.
SECTION 2 COMPILATION OF FINITE
ELEMENT RESULTS
CHAPTER
LOADTRANSFER IN SINGLE RIVET=ROW LAP JOINTS (CONVENTIONAL AND COUNTERSUNK) 6.1 SUMMARY OF LOAD TRANSFER MODELS
The finite element models, 4S1,4C1 and 4S5 (see Tables A.2 and A.3), used to obtain these data are described in detail in Chapter 13;the material properties for the various models are described in Chapter 15.The content of this chapter is taken from References [2] and [3]. 6.2 LOAD TRANSFER CALCULATIONS FOR SINGLE RIVETROW LAP JOINTS
Lap joints are different from butt joints in that significant outofplane distortion occurs in the form of rivet tilting and panel bending. As a result there are outofplane load transfer paths not found in an idealized twodimensional butt joint analysis. These can be seen in Figs. 6.1(a)6.1(~).Figure 6.l(a) shows a loaded, single rivetrow lap joint with conventional rivets; the distortion is exaggerated for clarity. Figures 6.l(b) and 6.l(c) show free body diagrams of the upper halves of the conventional and countersunk rivets and the corresponding panel pairs with the forces that act on them. The four load transfer paths will be the loading direction components of the following forces: (1) the shear across the rivet midsection, (N2 + Fl), shown in the top part of Fig. 6.l(b), (2) the axial force on the rivet shank midsection, (N1+ F2),shown in the top part of Fig. 6.l(b), (3) the friction force between the upper and lower panel, (F3), shown in Fig. 6.1(c), and (4) the normal force between the upper and lower panels, (N3), shown in Fig. 6.l(c). In addition, the rivet and the rivet head must support large axial forces: (1) the axial rivet shank load at the head (equal to the shear force at the rivet head), (Nl), shown in Fig. 6.l(c), and (2) the axial rivet shank load at the midsection, (Nl+F2), shown in the top part of Fig. 6.l(b).
99
100
Structural Shear Joints
i
I'
3 , N1+F2
N13'
N11'2
N2
N2+Fll'+NI 1'
 N13'+F2F13'
(b)
Figure 6.1. (a) A loaded singlerivet lap joint (distortions are exaggerated for clarity), (b) Free body diagram of the upper half of a standard head (top) and a countersunk head (bottom) rivet. See 6.l(a) for prime definitions. N = normal force, F = friction force, (c) Free body diagrams of the two sets of panels (figure continues).
101
Load Transfer in Single RivetRow Lap Joints
+ 2926.25 N
I + 2926.25 N
I IDDCD D A h l C l "r
r
L I 3
rnl.LL
F3
\
\ N3 LOWER PANEL
(C)
+ 2926.25 N
F11'= component of F1 in l'direction F13'= compontent of F1 in 3'direction N11'= component of N1 in l'direction N13'= component of N1 in 3'direction
Figure 6.1. Continued.
The local and global axes are defined in Fig. 6.l(a), and Figures 6.l(c) and 6.2 identify the various contact surfaces. The local (primed) axes represent the directions normal and tangent to the tilted rivet. At each contact area ( a l , b l , cl, d l , el for Models 4s1 and 4s5, and a2, b2, c2, d2, e2 for Model 4C1) there is a normal force and friction force acting at the panel surfaces. The local normal and friction forces represent the contact pressure and the contact
Structural Shear Joints
102
TABLE 6.1. DEFINITIONS OF EVALUATED FORCES
1 (=NS+F4N3) UI’
I Total local inplane forces for 4C I
I upperpanel I

LI’
I Total local inplane forces for 4C1 (=F3+N4+F5) I lower panel I

I (=F 1 1’+N 11’+N2+F3)
shear acting on each contact area. These forces are evaluated and resolved into either the 1’direction (localinplane) or the 3’direction (localoutofplane).Then the local components are transformed into the 1direction (globalinplane) and the 3direction (globaloutofplane) using the angle of rivet tilt. The normal and friction forces at all contact surfaces are obtained by multiplying the average contact pressure or the average contact shear by the contact area. Free body diagrams of the forces acting on each panel are shown in Figs. 6.1. The forces acting at the panel ends are calculated from the tensile stress ((5) and crosssectional area of the panels (F = 125 MPa * 1.53mm * 15.3 mm = 2926.25 N). The variables shown in Figs. 6.1 are defined in Table 6.1. At the countersunk portion of Model 4C1, both the friction and normal forces have components in the localinplane and the localoutof plane directions; therefore these forces must be resolved into the 1’ and 3’ directions. Figures 6.2(a) and (b) show typicai contour plots illustrating values of contact pressure distributions for the aluminum models 4s1 and 4C1. Table 6.2 presents the local in and outofplane loads obtained for the models. The load labels refer to the notation described in Figs. 6.1.
Load Transfer in Single RivetRow Lap Joints
103
Figure 6.2. (a) Contour plot of contact pressure for Model 4s1 at contact surfaces a l , b l , c l , d l and e l , (b) Contour plot of contact pressure for Model 4C1 at contact surfaces a2, b2, c2, d2 and e2, onom = MPa.
104
Structural Shear Joints
TABLE 6.2. FORCES FOR MODELS 4S5,4S1 AND 4C1 AT ALL CONTACT SURFACES
The applied tensile load is transferred by means of the four load transfer paths listed above. Table 6.3 shows the magnitudes and percentages of load transferred within the joint, for the models, through the four different load paths. Table 6.4 shows axial rivet shank loads for the two aluminum models at three locations: (1) the head of the upper rivet, (2) the middle cross section of the rivet, and (3) the head of the lower rivet.
6.3. SUMMARY AND IMPORTANT POINTS
The load is transferred through the lap joint by the four global1 components of the following forces: (a) (b) (c) (d)
9091% from shear at the midsection of the rivet shank 13% from tensile axial force at the midsection of the rivet shank 79% from friction force between the upper and lower panel ()13% from normal force between the upper and lower panel.
There is not a significant difference in shear force and tensile axial force across the midsection of the rivet shank in the standard and countersunk models. There are small differences in friction force and normal force between the upper and lower panels for the standard and countersunk models because the standard rivet heads clamp the panels more effectively than the countersunk rivet head does. The steel model displays slightly higher friction and normal forces than the aluminum model.
Load Transfer in Single RivetRow Lap Joints
105
TABLE 6.3. LOAD TRANSFER AT THE UPPER RIVET MIDSECTION AND UPPER PANEL OF ALUMINUM MODELS 4S5,4S1 AND 4C1 Load Transfer Path IOCE
4s5
Total Force IN) ’ plane( 1 3‘)*  global inplane( 1c 4S1 4S5 I 4S1 4C 1
1 Shear force across rivet
midsection (% of total applied force)
2650 2629 2665 (91%) (90%) (9 1Yo)
2650 (91%)
2.Axial force on rivet shank midsection (% of total applied force)
1207 1288 1312 (41%) (44%) (45%)
28 (1%)
3.Friction force between upper & lower panel (% of total applied force)
268 (9%)
268 (9%)
4.Normal force between the upper and lower panel (% of total applied force)
1378 1106 1036 (47%) (38%) (35%)
22 1 (8%)
207 (7%)
I 1 1
iponent)* 4C1
2624 (90%)
2658 (9 1Yo)
81 (3%)
97 (3yo)
220 (8%)
206 (7%) 77 (3%)
~
5.Total force Sum of 1 through 4 (YOof total applied force)
2884 (99%)
* see Figs. 6.1 for directions
TABLE 6.4. AXIAL RIVET SHANK LOAD FOR MODELS 4S1 AND 4C1 AT THE UPPER AND LOWER RIVET MIDSECTION Rivet shank Uuuer rivet head Upper rivet midsection Lower rivet head Lower rivet midsection
Model 4S1 746 1288
746 1288
Total force (N) Model 4C1 765 1312 984 1314
4. There is a higher force acting at the rivet shank upper portion, and at the rivet head lower portion, for the countersunk head model than for the standard head model. The peak stress occurs at these locations. 5. In spite of the fact that load transfer is essentially the same in the standard and countersunk head models, there is a large difference in the panel stress concentration factor (SCF = 6.1 and SCF = 9.8 for the standard head and countersunk head model, respectively).
CHAPTER
7 COMPILATION OF RESULTS FOR OPENHOLEPANELS AND BUTTJOINTS
7.1 SUMMARY OF CALCULATIONAL MODELS FOR OPEN HOLE PANELS
Table A.5 presents the calculations done for open hole panels. The finite element models used to obtain these data are described in detail in Chapter 13; the material properties for the various models are described in Chapter 15. The content of this section is taken from Reference (1). 7.2 SUMMARY OF CALCULATIONAL MODELS FOR BUTT JOINTS
Tables A.l,A.7 and A.8 in Appendix A present the various calculations done for butt joints. The finite element models used to obtain these data are described in detail in Chapter 13; the material properties for the various models are described in Chapter 15. The content of this section is taken from References [l] and [9]. 7.3 SUMMARY OF CALCULATION RESULTS FOR OPEN HOLE PANELS
Stress concentration factors (SCF), defined as the ratio of the maximum tensile stress to the nominal stress based on one repeat section, were evaluated for four different holes, one straight, three countersunk, and one straight hole with a pin. SCFs are listed in Table 7.1. Figures 7.1 and 7.2 compare the stress distributions for an open hole panel with a panel containing a pin. 7.4 SUMMARY OF CALCULATION RESULTS FOR BUTT JOINTS WITHOUT INTERFERENCE
Table 7.2 presents a summary of the distortion parameters from a 2D analysis of an elastic butt joint with headless fastener under a nominal, remote stress of 125 MPa, without interference and with p = 0.2. 107
108
Structural Shear Joints
TABLE 7.1. STRESS CONCENTRATION FACTORS DUE TO HOLE COUNTERSINKING Model 1 H I 1 H2 IH3 1 H4
Hole Geometry Straight hole
SCF 3.0
100' countersink upto 112 the panel thickness
3.38
61.6" countersink through  the entire panel thickness
3.23 3.5 2.85
100" countersink through the entire panel thickness Straight hole with pin
I H5
+1.71 E m +1.42Em +1.14Em : *.50E+07 : +s.@5EH37 : +2.79 E+07
: : '
I
1510
15
45
30
75
90
8 (degrees) 1.0 1
(b)
Figure 7.1. Long plate with open empty hole: (a) 011 contours with plate bottom fixed, pin has modulus of sheet (aluminum) (b) Distribution of bulk stresses adjacent to the hole. Stresses = 125 MPa. are normalized by applied stress onom
Compilation of Results for Open Hole Panels and Butt Joints
2: 3:
4 5: 6: 7: 8:
109
+3.07E+OB +2.TgE+OB +2.52 E+OB +2.24EE+08 +l.geE+OB +l.BE+# +1.8E+OB
0: e . 3 5 E+07 1: + 5 . 5 5 M 7 2: +2.74E*07 3: 6.40 E+Q5
1
L*
Figure 7.2. Long plate with open pinfilled hole: (a) 011 contours with plate bottom fixed, pin has modulus of sheet (aluminum) (b) Distribution of bulk stresses adjacent to the hole. = 125 MPa. Stresses are normalized by applied stress onom
The effects of the friction coefficient, p, pinplate material combinations, finite plate dimensions and biaxial loading on the normalized contact pressure, p . R/Q, contact angle, 80,and the normalized tangential stress around the hole, oee * WQ,are summarized in Figures 7.3 and 7.4. The results are precise for the conditions for which these calculations were performed (R = 3.06 mm, and Q = 1836 kN/m), and will be close for other values, but not precise, due to slight nonlinearities in the problem (as discussed in Chapters 1.2 and 5.6).
110
Structural Shear Joints 
p=O (3P2)
0.60
0.50 0.40
U $0.30 P
0.20 0.10 0.00 90
0
45
8 (degrees)
0.50 .2, AlEpoxy (3P9)
0.40
a 0.30 2
d
0.20
0.10
p = l , TiAI (3P12)
i
\ \\\
0.00 90
45 8 (degrees)
0
(b)
Figure 7.3. Normalized pinplate contact pressure, p.R/Q, as a function of angular location, 8,along the hole circumference (see Figure 2.2(a) for angular location convention). (a) p = 0,0.2 and 1, infinite plate, aluminum alloy pin and aluminum alloy plate, (b) p = 0.2 and 1, infinite plate, and four pinplate material combinations (figure continues).
Compilation of Results for Open Hole Panels and Butt Joints
1i
4
4
Oa50 0.40
U
6? 0.30 d.
111
AIAI (3P2) SteelAl(3P3) TiAI (3P4)
:::: 0.00
+
90
45
0
8 (degrees) (c>
Finite Plate, AIAI (3P13) Finite Plate, SteelAl (3P14) Finite Plate, TiAI (3P15)
0.60
0.50 0.40
U
3P 0.30
Infinite Plate, MetalMetal
0.20
0.10 0.00
90
45 8 (degrees)
0
(4 Figure 7.3. (figure continued) (c) p = 0, infinite plate, and four pinplate material combinations, (d) p = 0, finite and infinite plate, and the metallic pinplate material combinations considered in the study. Under these conditions, the contact pressure distribution is essentially a single curve (figure continues).
0.50
p=0.2, Infinite (3P6)
0.40 p = l , Infinite (3P10)
ti0.20 0.10 0.00 90
45 8 (degrees)
0
(el p=O, AIAI (3P19)
0.60 =0.2, AIAI (3P21)
0.40
d
0.20
p=0.2, AIAI (3P16)
0.00 90
0
45 8 (degrees) (4
Figure 7.3. (figure continued) (e) p = 0.2 and 1, finite and infinite plate, aluminum alloy pin and aluminum alloy plate, (f) p = 0 and 0.2, finite plate, two pinplate material combinations and two types of loading (uniaxial and biaxial). TABLE 7.2. SUMMARY OF DISTORTION PARAMETERS FOR A WIDE ELASTIC PINNED BUTT JOINT, Pi/D = 5, UNDER A NOMINAL, REMOTE STRESS 125MPa, WITHOUT INTERFERENCE AND WITH p = 0.2, Q = 3825 kN/m, MODEL 3P1, AITER IYER [l] Feature
Value
Loading end displacement, pm
307 1
Inplane slip, pm
038
Peak contact pressure, MPa
522
Compilation of Results for Open Hole Panels and Butt Joints
0.60
T
113
,u=I (3P10)
0.40
8
0.20 0.00 0
45
90
45
0.20 8 (degrees)
0.60
0.50
3
p = l , AIAI (3P10) p = l , SteelAl (3P11) ‘ “,A1 (3P12)
p=0.2, AlEpoxy (QP9)
//cc‘””
0.40
p=O.2, AIAI (3P6)
a
0.30 6?5 0.20 b
0.10
0.00 0.10
45
0
45
90
0.20
0.30 8 (degrees)
Figure 7.4. (a) Normalized tangential stress, oee.lUQ, around the hole as a function of angular location, 8, along the hole circumference (see Figure 2.2(a) for angular location convention). (a) p = 0,0.2 and 1, infinite plate, aluminum alloy pin and aluminum alloy plate, (b) p = 0.2 and 1,infinite plate, and four pinplate material combinations. (figure continues)
114
Structural Shear Joints
0.40 U
i?k
0.30 0.20
i
ACEpoxy(3P5)
/ \\
SteelAl (3P3) TiAI (3P4) AIAI (3P2)
b
0.10
I
\\
0.00
0.10
90
45
0
45
90
0 (degrees)
(c)
0.70
0.60 0.50 0.40 U 2 0.30 5 0.20 b 0.10 0.00 0.100.20
Finite Plate, SteelAl (3P14) Finite Plate, TiAI (3P15) Finite Plate, AIAI (3P13)
Infinite Plate, MetalMet
0
0 (degrees)
(4 Figure 7.4. (figure continued) (c) p = 0, infinite plate, and four pinplate material combinations, (d) p = 0, finite and infinite plate, and the metallic pinplate material combinations considered in the study. (figure continues)
7.5 EFFECTS OF INTERFERENCE IN BUTT JOINTS
Figures 7.5(a) and (b) and 7.6 illustrate the angular variation of contact pressure about a pinned hole undergoing cyclic stress for three different values of friction and interference. Figure 7.7 shows the slip amplitude, 6 (the difference between the load and unload value of the local slip displacements), for an aluminum pin with 1% interference.
Compilation of Results for Open Hole Panels and Butt Joints
p=0.2, Finite (3P16)
115
\ A
0.66 U
6? 0.46 & b 0.26 0.06 0.14' 8 (degrees)
(el
=0.2,AIAI (3P16)
8 (degrees)
(f)
Figure 7.4. (e) p = 0.2 and 1,finite and infinite plate, aluminum alloy pin and aluminum alloy plate, (f) p = 0 and 0.2, finite plate, aluminum alloy pin and aluminum alloy plate, and two types of loading (uniaxial and biaxial).
Figures 7.8 and 7.9 present the angular variations of fretting wear parameters F1 and F2 for different values of interference and friction. The peak values of F1 and F2,their angular positions and corresponding values of contact pressure and slip, are described in Figs. 7.10(a) and 7.10(b) and in Tables 7.3 and 7.4.
Structural Shear Joints
116
500 0
Loading
n Unloading 400 m
a 5
f
300
! a' 200
100
0
180150120 92 83 3 0
30 60 90 120 150 180
0 tj'
'
(a)
603 500
i_i
a
A
Unloading
2m
180150120 90 60 30
0
30 60 90 la3 150 180
0'
(b) Figure 7.5. Angular variation of the contact pressure about the pinned hole with the cyclic stress applied and partially released for the aluminum pin: (a) p = 0.5 and 0% interference (b) p = 0.2 and 2% interference.
Compilation of Results for Open Hole Panels and Butt Joints 600
,
1 ..
117
I
I .
1 , '
I '

1 ' .
I '
.!
180150120 90 60 30 0
. I " I "
I . ' I . ' I"
30 60 90 120 150 180
e"
Figure 7.6. Angular variation of the contact pressure about the pinned hole with the cyclic stress applied and partially released for the aluminum pin, with p = 0.5 and 1 % interference.
9 ,
I
7 6 5 ! 4
m
3
2 1 0
1 180150120 90 60 30
0
30 60 90 120 150 180
d Figure 7.7. Angular variation of the slip amplitude about the pinned hole with the cyclic stress applied and partially released for the aluminum pin and 1 % interference.
Structural Shear Joints
118
+ 0% Interference + 1% Interference
E cd
+ 2% Interference
4 7
LL d
180150120 90 60 30
30 60 90 120 150 180
0 0O
(a)
3.0
2.5
2.0
E cd
4
1.5
Y
LL
d
1.0
0.5
0.0
180150120 90 60 30
0
30 60
90 120 150 180
X Axis
(b) Figure 7.8. Angular variation of the fretting wear parameter, F1, about the pinned hole with the cyclic stress applied and partially released for the aluminum pin and with 1%and 2% interference: (a) p = 0.2 (b) p = 0.5.
Compilation of Results for Open Hole Panels and Butt Joints
119
70 60
50 40
30 20
10
0 180150120 90 60 30
0
30 60 90 120 150 180
0O
Figure 7.9. Angular variation of the fretting wear parameter, F2, about the pinned hole with the cyclic stress applied and partially released for the aluminum pin and with 1% and 2% interference, and p = 0.5.
Figure 7.11(a) illustrates a typical, calculated variation with angular location, 8, of the fretting wear and fatigue parameters F1, F2 and the tensile stress in the panel, adjacent and parallel to the hole. Figure 7.11(b) shows the variation of the hysteresis loop width around the pinhole interface as a function of friction, load and interference. Table 7.5 gives angular locations of peak values of F1 and F2 and circumferential tensile stresses adjacent to the pinhole interface.
Structural Shear Joints
120
3
0,7,
I
1
0
% Interference
(4
1
o
t 1
0
% Interference
(b) Figure 7.10. Variation of the fretting parameters with interference and friction coefficient: (a) F1 (b) F2.
Compilation of Results for Open Hole Panels and Butt Joints
121
TABLE 7.3. INFLUENCE OF INTERFERENCE ON THE ANGULAR LOCATION, 8, OF THE PEAK VALUES OF F1, AND CORRESPONDING VALUES OF 6 AND p AT THE PINHOLE INTERFACE FOR EIP BEHAVIOR Pin Material,
Model
P
% Interference
F1
0 range
6
P
(kPa.m)
(O)
(pm)
(MPa)
Al, 0
3P25
0.2
0.44
13.1
24.8
336.1
Al, 1 Al, 2
3P26 3P27
0.2
0.10
13.7
4.8
416.7
0.2
0.08
4.6
2.9
536.3
Al, 0
3P28
0.5
0.72
13.3
19.7
301.5
Al, 0.5
3P29
0.5
0.24
13.7
7.9
244.0
Al, 0.75
3P30
0.5
0.10
13.6
2.5
326.3
Al, I Al, 2
3P3 1 3P32
0.5
0.09
13.6
2.0
376.3
0.5
0.10
31.5
1.9
403.6
TABLE 7.4. INFLUENCE OF INTERFERENCE ON THE ANGULAR LOCATION, 8, OF THE PEAK VALUES OF F2, AND CORRESPONDING VALUES OF 6 AND p AT THE PINHOLE INTERFACE FOR EIP BEHAVIOR Pin Material,
Model
CL
% Interference
F2
(10'0Pa2.m)
€)range (O)
6
P
(p) (MPa)
Al, 0
3P25
0.2
11.33
13.0
24.8
336.1
Al, 1
3P26
0.2
1.48
13.8
4.8
416.7
Al, 2
3P27
0.2
Al, 0 Al, 1
3P28 3P3 1
0.5
18.25
4.0
25.0
151.7
0.5
1.50
31.5
2.3
287.1
Al, 2
3P32
0.5
 The stresses in the panel, adjacent and parallel to the hole remain compressive and F2 does not have any significance.
Structural S h e a r Joints
122
1700
r, N' LL
* 7
LL
*

I
1300 1200 1100 1000
900 800 700 600 500 400
300 200 100 0 180150120 90 60 30
30 60
0
90 120 150 180
0,
(4
0'0°16 00014
__
1
++ p = 0.2, Ao = 112 MPa + p=05,Ao=112MPa 4p = 0, AD = 112 MPa t p = 0.2, A a = 180 MPa 4 p = 0.2 (0.5% I),
00012 0 0010 
0.0006 0.0004
0.0002 0.0000 90
60
30
0
30
60
90
0.
(b) Figure 7.11. (a) Angular variation of F1, F2 and the tensile stress, 0,in the panel, adjacent and parallel to the hole interface for the case of p = 0.2 and 0% interference (b) Angular variation of the hysteresis loop width around the pinhole interface as a function of p,load and interference.
Compilation of Results for Open Hole Panels and Butt Joints
123
TABLE 7.5. INFLUENCE OF INTERFERENCE ON THE ANGULAR LOCATION, 8, OF THE PEAK VALUES OF F1, F2 AND CIRCUMFERENTIAL TENSILE STRESSES ADJACENT TO THE PINHOLE INTERFACE FOR ELKP BEHAVIOR Pin Material,
Model
p
% Interference
AO (MPa)
F1
wo)
F2
w0)
OW
wo)
Al, 0 Al, 0
3P33
0.0
112
4.5
3p34
0.2
112
22.5
13.5
4.5
Al, 0
3p35
0.3
112
22.5~13.5
13.5
4.5
Al, 0
3p36
0.5
112
13.5
13.5
4.5
Al, 0.5
3p37
0.2
112
4.5
4.5M.5
22.5
Al, 0
3p38
0.2
180
22.5
13.5
4.5
Al, 0.5
3p39
0.2
180
13.5
4.5
4.5
CHAPTER
COMPILATION OF RESULTS FOR LAP JOINTS
8.1 SUMMARY OF CALCULATIONAL MODELS Single RivetRow Lap Joints. Tables A.2 and A.3 present a summary of the calculations done for single rivetrow lap joints with standard and countersunk heads, respectively. Table A.7 in Appendix A shows the calculations performed for evaluation of the effects of interference and clamping on single rivetrow lap joints. The finite element models used to obtain these data are described in detail in Chapter 13;the material properties for the various models are described in Chapter 15. Double RivetRow Lap Joints. Table A.4 in Appendix A presents a summary of the calculations done for double rivetrow lap joints. The finite element models used to obtain these data are described in detail in Chapter 13;the material properties for the various models are described in Chapter 15. The content of this chapter is taken from References [1,1317,19,20,35].
8.2 SUMMARY OF CALCULATION RESULTS
Single RivetRow Lap Joints. Table 12.1 contains the results of nine calculations for single rivetrow lap joints. The data includes joint compliance, rivet tilt, total inplane slip at the rivetpanel interface and the panelpanel interface, total outofplane slip, peak tensile stresses and peak contact pressure. Table 8.1 lists calculated stress concentration factors and their angular locations for the five elastic models. The angular locations of the peaks are the likely sites of fatigue crack initiation when the fatigue process is not assisted by fretting. A normalized peak compression, NPC, defined as the negative ratio of the peak compressive stress to the nominal tensile stress based on one repeat section, is also presented.
125
126
Structural Shear Joints
TABLE 8.1. CALCULATED STRESS CONCENTRATION FACTORS IN THE PANELS OF THE RIVETED ASSEMBLIES
TABLE 8.2. IMPORTANT STRESSES GENERATED IN THE RIVET SHANK
Table 8.2 summarizes some of the important stresses generated in the rivet shank. Figure 8.1 shows a zoomedin profile of the displaced mesh and corresponding tensile stress contours for the single rivetrow lap joint. Double RivetRow Lap Joints. Table 12.2 in Chapter 12 contains the results of calculations for double rivetrow lap joints. The data includes joint compliance, rivet tilt, total inplane slip at the rivetpanel interface and the panelpanel interface, total outofplane slip, peak tensile stresses and peak contact pressure.The data presented are valid for elastic, double rivetrow, aluminum alloy lap joints with standard and countersunk aluminum and steel rivets. They are compared with similar analyses for single rivetrow joints.
3
1 85 E 4 8
Figure 8.1. Zoomed in profile of the displaced mesh and corresponding tensile stress (011) fields generated in the two holes in model 4C6. In the latter, the rivet is not shown and displacements are magnified 3x in the displaced mesh profiles, onom = 60 MPa.
Figure 8.2. Zoomed in profiles of the displaced mesh of model 5s1 and corresponding tensile stress ( 6 1 1 ) fields (b) in hole #1 (c) in hole # 2. The shaded in region in (a) is the initial configuration and displacements are magnified 3x, Onom = 125 MPa.
127
Structural Shear Joints
128
TABLE 8.3. CALCULATED STRESS CONCENTRATION FACTORS (SCF) AND NORMALIZED PEAK COMPRESSION (NPC) VALUES IN THE PANELS OF THE THREEDIMENSIONAL RIVETED ASSEMBLY
I
Model
SCF Hole #1 Value 8,"
Noncountersunk aluminum rivet 5S1 Countersunk aluminum rivet 5C1
Countersunk steel rivet 5C2
upper panel lower panel upper panel lower panel upper panel lower panel
Hole #2 Value 8,"
NPC Hole #1 Hole #2 Value 8," Value 8,"
4.4
6.2 to 10.9
3.1
3.1 to 8.7
3.8
90
3.1
90
3.1
8.7to3.1
4.4
10.9to 6.2
3.1
90
3.8
90
6.1
9.8 to 15.6
4.5
0 to 9.8
5.8
90
4.0
90
3.0
16.1 to 8.6
4.2
12.1 to 8.6
2.7
90
4.3
90
5.9
10.7 to 13.2
4.2
8.2 to 15
4.5
90
3.8
90
2.8
8.7t02.5
4.0
8.6to 3.1
2.6
90
4.1
90
~~
~
TABLE 8.4. IMPORTANT STRESSES GENERATED IN THE RIVET SHANK Model
Noncountersunk aluminum rivet 5s1 Countersunk aluminum rivet 5c1 Countersunk steel rivet 5C2
Peak ShankHole Compressive Stress ((T,,),MPa rivet rivet #I #2
Peak Shear Stress (al3), MPa rivet rivet #1 #2
Peak Axial Tensile Stress (a333), MPa rivet rivet #I #2
Peak Axial Compressive MPa Stress rivet rivet #I #2
240
240
126
126
174
174
95
95
353
321
175
143
160
224
115
164
338
335
168
133
200
266
116
157
A displaced mesh for model 5S1 is illustrated in Fig. 8.2. Table 8.3 shows calculated values of the stress concentration factor (SCF), defined as the ratio of the maximum tensile stress to the nominal stress based on one repeat section, and its angular location at the two sets of holes in the model. Figure 8.2 illustrates contours of important stresses developed in the rivets under load: (i) 011, arising from contact between the rivet shank and upper and lower panels, along the
Compilation of Results for Lap Joints
129
TABLE 8.5. MAXIMUM SCF AND SAF VALUES IN THE PANELS OF DOUBLE RIVETROW LAP JOINTS
loading axis, (ii) 013, shear stress present in the rivet, and (iii) 0.33, axial stress present in the rivet. Table 8.4lists peak values of the stresses generated in the rivet shank. The SCF’s obtained for the doublerow assemblies are compared in Table 8.5 with those obtained for comparable singlerow assemblies subjected to the same, remote, repeat distance load and nominal stress. Defining the “nominal” rivet load as the remote, repeat distance load divided by the number of rivet rows, a “nominal” Stress Amplification Factor (SAF), defined as the peak tensile stress divided by the product of the nominal rivet load and the remote repeat distance panel crosssectional area, may be evaluated. The SAF (equal to SCF * N, where N is the number of rivet rows) and SCF are identical for a single rivetrow assembly. Table 8.5 contains values for the SAFs for the noncountersunk and countersunk cases. The SCF’s express the relation between the peak tensile stresses generated in the panel and the remote nominal stress. The values obtained for the doublerow assemblies are compared in Table 8.6 with those obtained for comparable singlerow assemblies subjected to the same, remote, repeat distance load and nominal stress. To examine the origin of the variation in the distribution of in and outofplane load transmission with the number of rivet rows, the peak rivet shear stress, 013, indicative of inplane transmission, and the peak rivet axial stress, 033, indicative of outofplane transmission, are examined. These are listed in Table 8.7. Two parameters which are easily deduced and indicate the relative proportions of in and outofplane load transmission are listed. 8.3 SUMMARY OF CALCULATION RESULTS INCLUDING INTERFERENCE AND CLAMPING
Single RivetRow Lap Joints. Table 8.8 shows the magnitudes of stresses and plastic strains generated in the upper panel, parallel and immediately adjacent to the hole surface as a function of depth, due to the installation step, i.e., interference or/and clamping.
Structural Shear Joints
130
TABLE 8.6. PANEL HOLE SCFS AND SAFS IN DOUBLE RIVETROW LAP JOINTS Joint Type (Model)
Hole
Panel
Single RivetRow SCF = SAF
Upper
6.1
4.4
8.8
Lower
6.1
3.1
6.2
Upper
3.1
6.2
Lower
4.4
8.8
#
NonCountersunk Aluminum
1
Rivets 2
(5s1)
Double RivetRow SCF SAF
Countersunk
Table 8.9 shows the magnitudes and gradients of stresses and plastic strains generated in the lower, noncountersunk hole due to the accommodation of 1% and 2% interference (models 4C25 and 4C26), and Table 8.10 shows the same values generated in the upper, countersunk hole because of the installation step. Figures 8.38.5 show the variations with the angular location, 8,of the contact pressure, and the inplane slip in the upper panel of the Stype models. Table 8.11 shows values of several
TABLE 8.7. COMPARISONS OF PROPORTIONS OF SHEAR AND ROTATION IN RIVETS IN DOUBLE ROW LAP JOINT MODELS Single RivetRow (MPa)
Rivet Model 5s1
#
1
1
5C2 2
q3
I
239
Double RivetRow
0 Id033
(013) ((013)Z+(033)Z)0~s
Compilation of Results for Lap Joints
131
TABLE 8.8. FEATURES OF UPPER PANEL HOLE DEFORMATION DUE TO THE INSTALLATION STEP (INTERFERENCE AND/OR CLAMPING) IN THE NONCOUNTERSUNKASSEMBLIES
TABLE 8.9. FEATURES OF THE NONCOUNTERSUNK (LOWER) PANEL HOLE DEFORMATION DUE TO THE INSTALLATION STEP (INTERFERENCE AND/OR CLAMPING) IN THE COUNTERSUNK ASSEMBLIES Pernag (%)
ow,MPa
PEee
(“w
310.2 130.2 z=2t
73.0
TABLE 8.10. FEATURES OF THE COUNTERSUNK (UPPER) PANEL HOLE DEFORMATION DUE TO THE INSTALLATION STEP (INTERFERENCE AND/OR CLAMPING) IN THE COUNTERSUNK ASSEMBLIES Model
Depth
ow,MPa
z=o
158.8
z=0.5t
4C25
I I
101.6
z=t
I
0.00
r
0.00
0.05
0.05
269.3
I
I
I
I
PEee (%I
Pernag (YO)
0.09
0.09 ~~
1.1
0.00
0.00
z=O.St
0.5
0.00
0.00
z=t
29.4
0.00
0.00
z=o
4C27
Structural Shear Joints
132
600
+z=O,loading + z=O,unloading
500
400
Qz=0.5t, loading
4
C z=0.5t.unloading
+
1
loo 0
\
E
90
60
z=t,loading
A z=t,unloading L ..
30
0
30
I
E
60
90
0, o
(a> _
goo
,
I
I
B z = t , l o a d i n g , 4S20, +z=t,unloading,
700
600
a"
2
$
500
n 400
300 200 100
0 90
60
30
0
30
60
90
0, O
(b)
,
Figure 8.3. (a) Variation of contact pressure at the shankhole interface with angular location and depth for Model 4S19, (b) Variation of contact pressure with angular location at depth z = t, where contact pressures peak, for Model 4S20.
Compilation of Results for Lap Joints
133
800
0 z=t, loading, 4822,0.5%CI, 0%1 z=t, unloading, 4322,0.5%CI, 0%1 0 z=t, loading, 4323,0.5%CI, 0%1 z=t, unloading, 4323,OS%CI, 0%1
+
700
600 500 400 n
300
200 100
i
0
90
60
30
30
0
60
90
e,
90
60
30
0
30
60
90
e,
(b) Figure 8.4. (a) Angular variation of contact pressure at the shankhole interface in Models 4s22 and 4323 at z = t, depth at which the pressures peak, (b) Variation of inplane slip between the panel hole and rivet in Model 4s19.
Structural Shear Joints
134

16
2
L + + t . . . t 90
60
+ tKm
30
0
30
60
90
Figure 8.5. (a) Variation of inplane slip amplitude at the shankhole interface with angular location and depth for Model 4S19, (b) Angular variation in Models 4S20,4S22 and 4S23 at depth z = t, where slip amplitudes peak.
135
Compilation of Results for Lap Joints
Model 4s19
z=O
OM
Peak OM (MPa) 429.9
,
Peak 612 (Pm) 25.7
0
533.2
30.4
z=t
0
594.8
34.7
z=O
35
95.0
2.7
z=0.5t
114
196.4
4.4
z=0.5t
4s20
Installation (MPa) 0
*Installation oeevalues are from the Isotropic response analyses
parameters at different locations through the hole depth. Composite effects are expressed by the mechanistic parameters, F1 and F2, whose variations with angular location at z = t are shown in Fig. 8.6. Table 8.12 shows peak values of the mechanistic parameters through the depth of the shankhole interface and their angular location. For the upper panel of Ctype models, Figs. 8.78.9 show the variations with angular location, 8,of the contact pressure and the inplane slip. Table 8.13 shows values of several parameters at different locations through the hole depth. Variations of the mechanistic parameters, F1 and F2, with angular location at z = t are shown in Fig. 8.10. Table 8.14 shows the peaks of the mechanistic parameters through the depth of the shankhole interface. Double RivetRow Lap Joints. Table 8.15 shows the peak values of some parameters across the hole depth. Note that +90° corresponds to the loading end for upper hole #1 but 90" corresponds to the loading end for lower hole #2. Figures 8.118.12 show variations of the contact pressure and inplane slip, with angular location, 8,in the critical holes in the two models. Table 8.16 lists the peak values of the tangential shear stress, F1 and F2 (the primary fretting parameters) across the hole depth in the critical holes of the two models. Figure 8.13 shows the angular variation of the local cyclic stress range, Ao and local mean stress, o m r at z = t in the critical holes. Variations with angular location at z = t for F1 and F2 are shown for the critical holes in Fig. 8.14. Table 8.17 summarizes the critical fretting fatigue conditions in single and doublerow assemblies with and without interference.
Structural Shear Joints
136

2.5
+3z=t,4s19 0% I +z=t,4s19 1%I 
2
E 1.5
t F t , 4 S  1 9 0.5% CI 0% I
~~
m
a, L i
1 
0.5
~
T 0
i
90
60
30
0
30
I
90
60
__
~
~
uz=t,4s19 0% I
+Z=t,4Sl9 1% I 70
+z=t,4Sl9 0.5% CI 0% I
60
+Z=t,4Sl9 0.5% CI I_%_ I .
30
20 10 0 90
60
30
0
30
60
I 90
0, o
(b) Figure 8.6. Variation of fretting parameters with angular location at z = t, the depth at which the parameters peak, for Models 4S19,4S20,4S22 and 4s23. (a) fretting wear parameter, F I , and (b) fretting fatigue parameter, F2.
Compilation of Results for Lap Joints
TABLE 8.12. SUMMARY OF MECHANISTIC PARAMETERS INDICATING LOCATIONS OF FRETTING WEAR AND CRACK INITIATION IN LAP JOINT ASSEMBLIES WITH NONCOUNTERSUNK RIVETS
137
Structural Shear Joints
138
900
7
+z=t,loading,0.5% 800 700
€ z=t,unloading,0.5%
4
\
600
2 500 Q
400
100
1 60
90
30
30
0
60
90
60
90
+z=O.unloading
sz=0.5t,loading 4 z=t,loading
c
90
60
30
0
30
8, *
(b) Figure 8.7. (a) Variation of contact pressure at the shankhole interface with angular location and depth for Model 4C24, (b) Angular variation of contact pressure at shankhole interface at depth z = t, where contact pressures peak, for Model 4C25.
Compilation of Results for Lap Joints
900
8oo 700
600
I +
139
I
I 7 1
8 z=t,unloading,0.5%
2 500 I
d
400
300 200 100 0
90
60
30
0
30
60
30
60
90
70
60
0
.
I lo 2
0 10
90
60
30
0
90
e,
(b) Figure 8.8. (a) Angular variation of contact pressure at the shankhole interface at depth z = t, where contact pressures peak Model 4C27, (b) Angular variation of inplane slip between the panel hole and rivet in Model 4C24.
140
Structural Shear Joints
40 I
5
e
30
20
10
0 90
50
40
30
5 lo
20
10
0 90
60
30
0
30
60
90
0, o
(b) Figure 8.9. (a) Angular variation of inplane slip amplitude in shankhole interface in Model 4C24, (b) Angular variation of inplane slip amplitude at the shankhole interface at z = t , in Models 4C25 and 4C27.
Compilation of Results for Lap Joints
TABLE 8.13. VARIATION OF PARAMETERS THROUGH THE DEPTH OF THE COUNTERSUNK HOLE
Installation
080
values are from the Isotropic response analyses
141
Structural Shear Joints
142
90
60
0
30
30
60
90
(4
300
250
200 E
h %
150
r
IiN
100
50
0
90
60
0
30
30
60
90
(b) Figure 8.10. Variation of fretting parameters with angular location at z = t, the depth at which the parameters peak, for Models 4C24,4C25 and 4C27. (a) fretting wear parameter, F I , and (b) fretting fatigue parameter, F2.
Compilation of Results for Lap Joints
143
TABLE 8.14. SUMMARY OF MECHANISTIC PARAMETERS INDICATING LOCATIONS OF FRETTING WEAR AND CRACK INITIATION IN LAP JOINT ASSEMBLIES WITH COUNTERSUNK RIVETS
Model
magnitude
e , O
(MW 4 c  z=o 24 z=0.5t
Peak F2 (10" Pa2.rn)
Peak F, (kPa.m)
Peak Tangential Stress (MPa)
magnitude (kPa.m)
e , O
99
45.0, 78.8
1.23
67.5,90.0
172
56.3, 45.0
0.63
22.5, 15.6
309
45.0
0.98
22.5
204
56.3, 78.8
0.21
78.8, 90.0
112
4.3, 15.6
0.15
15.6,22.4
134
22.5, 8.7
0.18
8.7, 4.3
7.50
108
45.0, 78.7
0.98
67.5,90.0
4.63
z=0.5t
199
45.0
0.53
22.5, 8.7
z=t
291
45.0
0.75
22.5
z=t 4 c  z=o 25 z=0.5t z=t 4 c  z=o 27

* two angular locations indicates the range over which a peak persists.  indicates compressive, bulk stresses, and Fz does not have any significance.
TABLE 8.15. FEATURES OF THE UPPER (COUNTERSUNK) AND LOWER (STRAIGHT) PANEL HOLES' DEFORMATION DUE TO 1%INTERFERENCE Model 5c3
z=o
Installation 088 (MW 0
Peak 088 (MW 199.6
upper hole
505.3
#1
609.8
5c4
z=o
265.5
upper hole
244.4
#1
418.1
5c4
z=t
lower hole #2
z=2t
Peak 812 (pm) 36.0
446.5 132
290.1
2.4
75
241.4
1.6
Structural Shear Joints
144
700
+z=O, loading
600
+ z=0.5t, loading & z=t, loading
+z=O,unloading
500
t z=0.5t, unloading
A z=0.5t, unloading
400
a
r L i
300
100
I
0 90
60
30
0
30
60
90
e, (a)
+z=t, loading, upper hole
700
R z=t, loading, lower hole
+z=t, unloading, upper h 600
500
400
a
z
r;
300 200
100
0
90
60
30
0
0,
30
60
90
j ’
(b)
Figure 8.11. (a) Variation of contact pressure at the shankhole (upper panel hole # 1) interface with angular location and depth for Model 5C3, (b) Variation of contact pressure with angular location in the two fatigue critical holes at depth z = t, where the contact pressures peak, for Model 5C4.
Compilation of Results for Lap Joints
145
45 40 35 30
z=0.5t, unloadin

25 
E,;u
20

15

A
10 5
0 5 90
60
30
0
30
60
90
e, (a)
z=t, 5C4, upper hole # I A z=t, 5C4, lower hole #2 35 30
E,
25
N
La 20
15 10 5 0 90
60
30
0
30
60
90
e, (b) Figure 8.12. (a) Angular variation of inplane slip between the upper panel hole # 1and rivet # 1 in Model 5C3, (b) Angular variation of inplane slip amplitudes in the fatigue critical holes at depth z = t, where slip amplitudes peak, in Models 5C3 and 5C4.
Structural Shear Joints
146
TABLE 8.16. VARIATION OF PARAMETERS THROUGH THE DEPTH OF THE HOLE Peak Tangential Stress (MPa) Model
magnitude
I
8, O
Peak F, (kPa.m) magnitude
I
8,
5c3 upper hole #I
5c4 upper hole # I
5c4 lower hole #2 two ang ar locations indicates the range over which a peak persists.
147
Compilation of Results for Lap Joints
90
60
30
0
30
90
60
e, (a) 400
300
2 I
200
E
h
%
100 L
0z=t, 5C3,upper hole #1 z=t, 5C4, upper hole #1 A z=t, 5C4, lower hole #2
0
100
I
90
I
l
I
J
,
I
60
I
l
1
1
1
8
30
I
I
<
1
I
0
1
1
1
1
1
30
1
1
1
1
1
60
1
1
1
1
1
1
~
90
e, (b)
Figure 8.13. Variation of conventional fatigue parameters in the fatigue critical holes in the Models 5C3 and 5C4 at z = t. (a) cyclic stress range, (b) mean stress.
Structural Shear Joints
148
0 z=t, 5C3,upper hole #I z=t, 5C4, upper hole #I A z=t, 5C4,lower hole #2 E li
4
1.0
LL
0.5
0.0
I
90
60
30
0
30
60
90
0 z=t, 5C3, upper hole #I 1 1 z=t, 5C4, upper hole #I A z=t, 5C4,lower hole #2
90
60
30
0
30
60
90
0, "
(b)
Figure 8.14. Angular variation of mechanistic fretting parameters at the frettingfatigue critical hole interfaces in Models 5C3 and 5C4 at z = t, the depth at which the parameters peak. (a) F1, (b) F2.
Compilation of Results for Lap Joints
TABLE 8.17. SUMMARY OF MECHANISTIC PARAMETERS INDICATING LOCATIONS OF FRETTING WEAR AND CRACK INITIATION IN LAP JOINT ASSEMBLIES WITH COUNTERSUNK RIVETS
Deformation
149
CHAPTER
SINGLERIVETROW LAP JOINTSUNDER BIAXIAL LOADING 9.1 SUMMARY OF CALCULATIONAL MODELS FOR 2D AND 3D LAP JOINTS UNDER BlAXlAL LOADING
Table A.8 presents a summary of the calculations done for 2D and 3D lap joints under biaxial loading. In the threedimensional analyses, countersunk and noncountersunk rivet geometries are treated. Interference and clamping stresses generated from rivet installation are not included. Three values of the biaxiality ratio, 4, (ratio of the longitudinal to the “hoop” stress) are considered. The finite element models used to obtain these data are described in detail in Chapter 13 [1,17181; the material properties for the various models are described in Chapter 15. 9.2 SUMMARY OF CALCULATION RESULTS FOR PINNED CONNECTIONS UNDER BlAXlAL LOADING
Table 12.5 presents the results for biaxial loading in a pinned connection. The data includes joint extension, slip at the pinpanel interface, peak tensile stresses and peak contact pressure [1,18]. Figure 9.1 shows the effects of biaxial loading on the variations of the contact pressure and interfacial slip at the pinpanel interface. 9.3 SUMMARY OF CALCULATION RESULTS FOR SINGLE RIVETROW LAP JOINTS UNDER BlAXlAL LOADING
Table 12.6 in Chapter 12 contains the results of calculations for single rivetrow lap joints under biaxial loading. The data includes joint compliance, rivet tilt, total inplane slip at the 151
152
Structural Shear Joints 700
1
600

2
500 400
300 Q
200 100
0 4 5
100
0
0 (degrees)
(a) 100,
80
90
75
60
45
30
15
1
0
15
30
45
60
75
90
(b)
Figure 9.1. Variation of the pinpanel (a) contact pressure, p , and (b) relative slip, A, with angular position, 8, in the 2D pinned connection as a function of the stress biaxiality, 9. Owing to symmetry, distributions between 90" I8 I180" and 0" I8 5 90" are identical to each other as are those between 90" i 8 I f 180" and 0" I 8I 90"
rivetpanel interface and the panelpanel interface, total outofplane slip, peak tensile stresses and peak contact pressure. Figures 9.2 and 9.3 show distributions of the contact pressure, p, and inplane rivetpanel slip, A, for the 3D riveted lap joint and noncountersunk and countersunk rivets, respectively. The plots shown are at a depth of z = 1.53 mm in the upper panel, where the parameters have
Single RivetRow Lap Joints Under Biaxial Loading
I4O0
153
1
1200
1000
800 A
m
n
600
4
400
200
0
45
0
200
0 (degrees)
(a)
1
loo
rn
90
75
60
45
30
15
I
0
\\
15
30
45
60
75
90
(b)
Figure 9.2. Variation of pinpanel (a) contact pressure, p , and (b) pinpanel slip, A, with angular position, 6, at z = 1.53 mm of the upper panel of the 3D riveted connection with a noncountersunk rivet.
Structural Shear Joints
154 2500
.
75
4 5
60
1 5
30
0
0 (degrees)
90
75
60
45
30
15
0
15
30
45
60
75
90
(b)
Figure 9.3. Variation of pinpanel (a) contact pressure,p, and (b) pinpanel slip, A, with angular position, 6, at z = 1.53 mm of the upper panel of the 3D riveted connection with a countersunk rivet.
Single RivetRow Lap Joints Under Biaxial Loading
155
TABLE 9.1. INFLUENCE OF STRESS BIAXIALITY ON CALCULATED STRESS CONCENTRATION FACTORS IN THE PANELS OF THE THREEDIMENSIONAL RIVETED LAP JOINT MODELS
* NPC = the negative ratio of the peak compressive stress to the nominal tensiile stress based one repeat section.
TABLE 9.2. IMPORTANT STRESSES GENERATED IN THE RIVET
been found to attain peak values and fretting fatigue cracks are known to initiate due to the presence of multiple, superposed stress concentrations arising from the rivetpanel contact and panel bending [17]. Table 9.1 shows the stress concentration factors obtained for the 3D lap joint models and Table 9.2 lists the maximum values of stresses that characterize the shearing and bending of the rivet.
CHAPTER
10 COMPILATIION OF RESULTS FOR LAP JOINTSWITH SEALANTS AND ADHESIVES
10.1 SUMMARY OF CALCULATIONAL MODELS FOR SINGLE RIVETROW LAP JOINTS WITH SEALANTS AND ADHESIVES
Table A.9 presents a summary of the calculations done for single rivetrow lap joints in the presence of sealants. The finite element models used to obtain these data are described in detail in Chapter 13 [68,21]; the material properties for the various models are described in Chapter 15. 10.2 SUMMARY OF CALCULATION RESULTS FOR PINNED CONNECTIONS WITH SEALANTS AND ADHESIVES
Table 12.7 contains the results of calculations for single rivetrow sealed lap joints. The data includes joint compliance, rivet tilt, total inplane slip at the rivetpanel interface and the panelpanel interface, total outofplane slip, peak tensile stresses and peak contact pressure. The term sealant is used to refer to nonlinear, rubberlike, low modulus, sticky polymers with pressure dependent shear properties. The term adhesive is used to refer to linear, higher modulus polymers. The joints discussed here are fastened or sealed with a low modulus sealant. The mechanical effects of both sealants and adhesives can be treated with the TALA method (described in Chapter 14) which has been applied to the finite element models presented in Chapter 13. The terms sealant and adhesive are used interchangeably since their effects on lap joints are qualitatively similar. Figure 10.1 shows the distribution of axial stress (normalized with respect to the applied nominal stress) at the upper panel hole surface for infinitely wide multiriveted lap joints. The axial stress is plotted as a function of angle (from 90" to 90) and depth (t = 0.0,0.765 and 1.53 mm). Figure 10.2 shows the curvature lines on the upper panel of the multiriveted lap joints with and without sealant. The peak stresses in the rivet elements are shown in Table 10.1.
157
Structural Shear Joints
158
+noadhesive
~
YI
%
, 8,"
(a) t
=0
. . . .
mm

+plusadhes ive noadhesive
____
__
8"
(b) t

0.765 mm
...
(f) I= 1 53mm
Figure 10.1. Angular variation of normal stress (011) around the surface of upper panel hole for infinitely wide multiriveted lap joints. (a), (b) and (c) are for models 4SA1 and 4s6 and (standard single rivetrow plusadhesive and noadhesive, respectively) at depth 0,0.765 and 1.53, respectively. (d), (e) and (f) are for models 4SA3 and 4C7 (countersunk single rivetrow plusadhesive and noadhesive) at depth 0,0.765 and 1.53, respectively.
(UILU) uogxipp
aue~djo~no
159
Structural Shear Joints
160
TABLE 10.1. STRESSES GENERATED IN RIVETS WITH AND WITHOUT A SEALANT LAYER
Model
Standard single rivetrow noadhesive (4S7, onerivet) Standard single rivetrow plusadhesive(4SA2, onerivet) Standard single rivetrow noadhesive(4S6, multiplerivet) Standard single rivetrow plusadhesive(4SA 1, multiplerivet) Countersunk single rivetrow noadhesive(4C8, onerivet) Countersunk single rivetrow plusadhesive (4CA4, onerivet) Countersunk single rivetrow noadhesive (4C7, multiplerivet) Countersunk single rivetrow plusadhesive(4CA3, multiplerivet)
Peak ShankHole Compressive Stress (S1 l), MPa
Peak Shear Stress (S 13), MPa
Peak Axial Tensile Stress (S33), MPa
Peak Axial Compressive Stress (S33), MPa
205.8
97.65
127.9
157.1
246.0
112.4
86.1
 1 19.0
212.1
105.6
127.2
135.6
252.3
114.8
85.81
111.3
332.4
121.0
180.4
191.2
364.2
130.0
87.28
128.9
3 14.4
123.7
181.9
190.8
373.6
133.1
87.77
107.8
CHAPTER
COMPILATION OF RESULTS FOR RIVETS 11.1 SUMMARY OF CALCULATIONAL MODELS FOR RIVETS
Table A.4 presents a summary of the calculations done to evaluate the effects of rivet installation. The finite element models used to obtain these data are described in detail in Chapter 13;the material properties for the various models are described in Chapter 15. 11.2 SUMMARY OF CALCULATIONAL RESULTS FOR RIVETS
Table 11.1summarizes important stresses generated in the rivet shank. Table 11.2 shows the variation in the distribution of in and outofplane load transmission with the number of rivetrows. The peak rivet shear stress, 013, indicative of inplane transmission, and the peak rivet axial stress, 033, indicative of outofplane transmission, are presented. Two parameters which are easily deduced and indicate the relative proportions of inand outofplane load transmission are listed.
161
a m
0
3
162
1 V
h
ca
h
e
v
"1 163
Figure 11.3.011,(~13 and 0 3 3 stresses generated in the shank of rivet ## 1 due to inplane and outofplane load transfer. The letters C and T are used to denote compressive and tensile regions, respectively (noncountersunk case), on,, = 125 MPa.
Compilation of Results for Rivets
165
Figure 11.4. Contour plots of 011 (normal stress, inplane direction) generated in rivets for infinitely wide multiriveted lap joints (a) model 4SA1 (standard rivet plusadhesive) and (b) model 4s6 (standard rivet noadhesive), on,, = 65 MPa.
166
Structural Shear Joints
Figure 11.5. Contour plots of 013 (shear stress) generated in rivets for infinitely wide multiriveted lap joints (a) model 4SA1 (standard rivet plusadhesive) and (b) model 4s6 (standard rivet noadhesive), on,, = 65 MPa.
Compilation of Results for Rivets
167
Figure 11.6. Contour plots of 0 3 3 (axial stress, outofplane direction) generated in rivets for infinitely wide multiriveted lap joints (a) model 4SA1 (standard rivet plusadhesive) and (b) model 4s6 (standard rivet noadhesive), onom = 65 MPa.
168
Structural Shear Joints
Figure 11.7. Contour plots of 011 (normal stress, inplane direction) generated in rivets for infinitely wide multiriveted lap joints (a) model 4CA3 (countersunk rivet plusadhesive) and (b) model 4C7 (countersunk rivet noadhesive), on,, = 65 MPa.
Compilation of Results for Rivets
169
Figure 11.8. Contour plots of 013 (shear stress) generated in rivets for infinitely wide multiriveted lap joints (a) model 4CA3 (countersunk rivet plusadhesive) and (b) model 4C7 (countersunk rivet noadhesive), onom = 60 MPa.
170
Structural Shear Joints
Figure 11.9. Contour plots of (333 (axial stress, outofplane direction) generated in rivets for infinitely wide multiriveted lap joints (a) model 4CA3 (countersunk rivet plusadhesive) and (b) model 4C7 (countersunk rivet noadhesive), on,, = 60 MPa.
Compilation of Results for Rivets
171
TABLE 11.1. IMPORTANT STRESSES GENERATED IN THE RIVET SHANK OF DOUBLE ROW LAP JOINTS
TABLE 11.2. COMPARISONS OF PROPORTIONS OF SHEAR AND ROTATION IN RIVETS IN SINGLE AND DOUBLE ROW LAP JOINT MODELS.
I
Model
I I I I I I 1
Double Row
I I Single Row
Double Row
0.77
0.72
0.61
0.59

0.72

0.59
160
0.78
1.09
0.61
0.74
224

0.64
#
4s1 or
1
5s1
2
4C1 or
1
5C1
2
u13
u33
239
309 
418

325
u33
Single Row
126
174
126
174
175 143
u13
4C2
I
1
I
I
168
I
200
I
5C2
1
2
I  I  1
133
I
266
I  I
388
I
489
0.79
I
I
0.54
0.84
I
I
0.64
I
0.5
I  I
0.45
I
0.62
CHAPTER
12
DATATABULATIONS The following tables present summaries of the results of many sof the finite element calculations described in this book. The model numbers refer to the joint configurations and fastener types (see Introduction for code keys and definitions of computational models). Details of each model number may be found in the tables in Appendix A. The finite element models used to obtain these data are described in detail in Chapter 13;the material properties for the various models are described in Chapter 15. The effects of rivet geometry (countersinking), rivet material and interfacial friction coefficient are included. Interference and lateral clamping are not treated. Load transfer through the joint, the joint compliance, rivet tilt, the local slips at rivetpanel and panelpanel interfaces, contact pressures and local stresses are presented. The excess compliance is defined as C = C'  C". C', the assembly compliance, is the ratio of the net extension, 6, to the load per repeat distance, P. C" is the compliance of a continuous panel having the same length, L, as the model joint (length of two panels minus the overlap) and the same cross sectional area, A, and elastic modulus, E, as a single panel. The excess compliance is related to the displacement, bending and deformation around the rivet. The rivet tilt is defined by the change in the slope of the line AB, illustrated in Fig. 12.1, which bisects the top of the rivet heads. The srress concentration factor (SCF) is defined as the ratio of the peak tensile stress to the nominal applied stress, based on one repeat section. The angular location convention is described in Figure 12.2.
12.1 SUMMARY CALCULATION RESULTS FOR SINGLE RIVETROW LAP JOINTS
The data presented in Table 12.1 are valid for elastic, and elasticplastic single rivetrow, aluminum alloy lap joints with C" = 93.4 d G N .
12.2 SUMMARY CALCULATION RESULTS FOR DOUBLE RIVETROW LAP JOINTS
The data presented in Table 12.2 are valid for elastic, double rivetrow, aluminum alloy lap joints with standard and countersunk aluminum and steel rivets and C" = 102.71 dGN.They are compared with similar analyses for single rivetrow joints.
173
Structural Shear Joints
174
I
0 \
.
. *\
Ax
I.
I
I
...............
. *.
I
I
.......
..
I
...........
I I
1.............. I
Figure 12.1. Schematic showing rivet displacements used to calculate tilt values reported in Table 12.2.A and B represent the coordinates of the end points of the line bisecting the rivet heads.
12.3 SUMMARY CALCULATION RESULTS FOR RIVET INSTALLATION RESIDUAL STRESSES
Tables 12.3 and 12.4present some of the effects of rivet installation for a single rivetrow aluminum lap joint for standard and countersunk rivet geometries, respectively. Contact pressures, slip amplitudes, bulk (circumferential) stresses, and the local cyclic stress range and mean stress adjacent to the rivet hole are evaluated during the first load cycle, after the application of interference and/or clamping with C" = 93.4 m/GN. They are compared with similar analyses for single rivetrow joints. 12.4 SUMMARY CALCULATION RESULTS FOR SINGLE RIVETROW LAP JOINTS UNDER BlAXlAL LOADING
Table 12.5 lists values of panel deformation characteristics of the twodimensional pinned connection for the three values of @ considered in the study, including the excess joint extension, 6. Table 12.6 summarizes the effects of load biaxiality, @, on the net longitudinal joint extension, excess longitudinal joint extension, rivet tilt, and the panel stresses, slips and pressures in 3D connections with noncountersunk rivets (models 4S16,4S17 and 4S18) and countersunk rivets (models 4C17,4C18 and 4C19).
Data Tabulations
175
Figure 12.2. Details of the mesh showing rivet type B and the panels. Values of peak stresses in elements E, E’,E and F’and slips at nodes ad and gh are presented in the tables in this chapter. Slips at nodes ad are calculated by subtracting the displacement of the rivet from the displacement of the sheet.
12.5 SUMMARY CALCULATION RESULTS FOR SINGLE RIVETROW LAP JOINTS WITH SEALANT
Table 12.7 shows the influence of the thin sealant layer on the distortion of the riveted lap joint. The local mechanical parameters: excess compliance, rivet tilt, inplane and outofplane slip at certain interesting points (a, a’, a”, b, b’, b”, c, c’, c”, d”, g, and h, in Figure 12.2), peak tensile stress in panel hole, peak contact pressure, panelpanel separation (observing from points m and n in Figure 12.4), stresses in the panel and in the rivet, and panel bending
176
Structural Shear Joints
TABLE 12.1. SINGLE RIVETROW LAP JOINT DISTORTION FEATURES 4C1 4C2 4C3 elastic, elastic, plastic, p=0.2 ~ ~ 0 . p=0.2 2 43.6 28.3 34.4
Model
4C4 4C5 4C6 plastic, elastic, elastic, p=0.4 p=0.2 p 0 . 2 32.8 36.74 41.18
i Feature
Location*
Joint Complianc (m/GN)
'
Total inplane slip at rivetpanel interface
h
I
1
17.7 14.6
hole (MPa) Peak Contact Pressure (MPa)
Contact Pressure (MPa)
shank hole (A)** panelpanel (B)** panelrivet head (C)**
t
I
11.6 9.17
1
53.1 44.84
1
13.4 7.22
1
44.77 41.4
1
65.7 60.5
766.8 706.6 706.8 767.1
765.6 661.5 667.5 767.25
549.4 517.3 516.8 549.8
1220.9 1097.4 614.4 690.2 1180.6 1059.8 671.7 738.9
633.8 549.3 593.6 563.5
614.4 522.1 592.7 551.5
1306.9 1512.4 641.0 499.4 1242.3 1357.3 707.8 597.4
779.2
641.6
744.24
1052.5
905.5
1141.5
963.7
1349.4
1953.4
350.7
347.2
364.4
334.9
378.2
445.6
324.1
822.7
1252.0
228.6
246.4
244.3
283.6
347.4
306.9
329.9
256.9
206.7
Data Tabulations
I
Model
Noncountersunk inum Rivets 5s1
Feature Single
Doutjlerow Rivet Rivet
I
1
1
I
177
Countersunk Countersunk Aluminum Rivets Steel Rivets 4c1 I 5C1 I 4C2 I 5C2 S ngi: Doubyrow Sngi: Doubyrow Rivet Rivet Rivet Rivet
I
1 1
1
1
27.46
Excess Compliance (m/GN) Rivet Tilt, degrees Total inplane slip at rivetpanel interface (PI
46.4
45.0
Total inplane slip at panelpanel interface (Pm) Total outofplane slip (Pm)
91.4
C C' C
d
Peak tensile stress in elements adjacent to rivet hole (MPa) Peak Conta ShankContact Pressure Panel(MPa) panel Contact Pressure (MPa)
Panelrivet head
5.9 2.7 8.7 2.6
706.6 767.1
779.2
471.7
1052.5
1052.5 719.1 496.5
905.5
561.2 478.1
350.7
188.3
334.9
334.9
125.1 177.9
378.2
115.0 213.5
228.6
121.0
283.6
283.6
78.8
347.4
106.9 174.4
I
I
I
*Locations identified in Fig. 12.2. **Contact field with which pressure is associated (Fig. 12.3)
133.3 I
I
I
I
J
178
Structural Shear Joints
TABLE 12.3. DISTORTION FEATURES FOR LAP JOINTS WITH NONCOUNTERSUNK RIVETS, = 100 MPa UNDER MAXIMUM LOAD, urnax Model
a 4s19
Feature
Locatior
*
Excess Compliance ( mi GN) Rivet Tilt, degrees Total inplane slip at rivetpanel interface (pm)
4s20
4822
4823
a a
7.92
a
32.3
I
I
I
5.65
I
I 23.91 I
4.60
b
30.7 . . b b
Total inplane slip at panelpanel interface (pm) Total outofplane slip (pm)
!:::I
h C
11.6 12.9
1 I 48.7
9.7
14.3
20.6
C
. . C
d
Peak tensile stress in elements adjacent to rivet hole (MPa)
2.2
e e
495.8
I
433.8
I
374.4
I
414.4
f ) .
f Peak Contact Pressure (MPa)
shankhole
(A)* panelpanel Contact Pressure (MPa)
o * panelrivet head
o *
denotes the contact field, sh vn in Fig.
I , with which the value is associated.
Data Tabulations
TABLE 12.4. DISTORTION FEATURES FOR LAP JOINTS WITH COUNTERSUNK RIVETS, UNDER MAXIMUM LOAD, urnax = 100 MPa Model
179
Structural Shear Joints
180
TABLE 12.5. DISTORTION FEATURES OF AN ELASTIC, TWODIMENSIONAL PINNED CONNECTION SUBJECTED TO A LONGITUDINAL STRESS OF UL = 125 MPa AND THREE VALUES OF TRANSVERSE STRESS, UT. BOTH THE PIN AND PLATE ARE MADE OF ALUMINUM AND p = 0.2
2D Model Feature Transverse farfield plate boundary displacement* (pm) Transverse, farfield plate boundary stress (MPa)
3P22 (4=0.25)
3P23 (4 = 0.50)
3P24 (4 = 0.75)
0.0'
k6.85
k13.66'
31.3
62.5'
93.8
50.4
55.4
53.1
6, excess longitudinal joint extension (pm) Angular location (range) over which panelpin contact is lost (") Peak tensile stress along the longitudinal direction in elements adjacent to hole (MPa) Angular location (range) of peak panel tensile stress (") Pinpanel contact pressure, p , at 8= 90"
I
I
[0,180]
I [4.5,+184.51
[9,+189]
802.2
794.7
730.8
LO1
[4.51
[ 14,91
522.2
1
573.0
I
593.2
Slip, A, at pinpanel interface at 8= 0" (pm)
34.9
39.0
39.3
Slip, d,at pinpanel interface at 8= 45" (pm)
6.35
7.66
7.91
applied transverse boundary condition.
Data Tabulations
181
TABLE 12.6. DISTORTION FEATURES OF ELASTIC, THREEDIMENSIONAL RIVETED LAP JOINTS
Feature
Location
*
Net longitudinal joint extension (pm) Transverse farfield plate boundary stress (MPa) Rivet tilt (“)


Total inplane slip at rivetpanel interface (Pm)
25.6
a a’
25.3
I
28.4
I
28.8
29.8
I
28.0
a
76.8
73.7
91.0
90.7
b b’ b” I
I
Total inplane slip at panelpanel interface ( P I Total outofplane slip
I
97.0
99.9
98.1
150.9
155.3
152.7
h
96.9
100.0
98.1
134.9
139.9
137.6
C
27.6
29.4
30.2
44.4
C’
24.8
26.4
27.0
25.52
C
4.2
4.5
4.9
1.16
d”
24.8
26.3
27.0
82.3
e
767.6
736.4
690.2
11 17.6
e
642.1
(Pm)
Peak tensile stress in elements adjacent to rivet hole (MPa)
I
I
I
1
618.5
I 572.4 I
706.5
f f” Peak Contact Pressure (MPa)
shankhole (A)** panel558.6 panel (B)** Contact Pressure (MPa) I panel210.2 ;vet head (C)** *Locations identified in Fig. 6.2. **Contact field with which value is associated.
I
ttt 576.3
580.6
532.9
I 208.0
I
198.6
I
285.0
I
I
Peak Contact Pressure (MPa)
Peak tensile stress in elements adjacent to rivet hole (MPa)
Total outofplane slip (mm)
Total inplane slip at rivetpanel interface (mm)
TABLE 12.7. INFLUENCE OF A THIN SEALANT LAYER ON THE DISTORTION OF INFINITELY WIDE AND FINITE WIDTH SINGLERIVETED LAP JOINTS (AN A IN THE MODEL NUMBER INDICATES THE PRESENCE OF ADHESIVE)
Data Tabulations
a) original mesh
1'
183
I
lower panel
b) deformed mesh
Figure 12.3. Illustrations of overlapping end opening and the curvature line abcd on the upper panel.
(observed from curvature line abcd in Figure 12.3) for each model are examined and compared at the same tensile loading. C" = 93.4 m/GN for these models. 12.6 SUMMARY CALCULATION RESULTS FOR VARIATION OF PANEL THICKNESS IN WIDE SINGLE RIVETROW JOINTS
Tables 12.8 and 12.9 show the affect of varying the panel thickness on the various mechanical parameters.The models employed are identical to (4s1) and (4C1) except for the panel thicknesses. 12.7 SUMMARY CALCULATION RESULTS FOR JOINT EXCESS COMPLIANCE AND RIVET TILT
Table 12.10 presents data for excess compliance and rivet tilt for several clamped and unclamped lap and butt joints.
TABLE 12.8. THE INFLUENCE OF PANEL THICKNESS ON VARIOUS PANEL PARAMETERS FOR STANDARD HEAD MODEL
Peak Contact Pressure (MPa) Contact Pressure (MPa)
rivet hole (MPa)
f’

Thickness Location
Shankhole (A) PanelPanel (B) PanelRivet head (C)
Model 4C 1 Feature Excess Compliance (m/GN) Rivet Tilt (degree) Total inplane slip at rivetpanel interface
494.2
635.7
0.77 39.77 4.27
0.0
629.6
0.92 36.10 4.26
0.0
640.0
1.07 33.78 4.14
552.2
655.8
1.15 32.89 4.20
754.0
748.1
1.53 30.82 4.31
866.6
818.4
1.91 29.09 4.38
870.6
894.2
2.30 28.07 4.43
787.2
967.7
2.68 27.45 4.46
TABLE 12.9.THE INFLUENCE OF PANEL THICKNESS ON VARIOUS PANEL PARAMETERS FOR COUNTERSUNK MODEL
628.8
1038.5
3.06 27.08 4.40
TABLE 12.10. JOINT EXCESS COMPLIANCE AND RIVET TILT AT SPECIFIED VALUES OF APPLIED STRESS
SECTION 3 CALCULATIONAL MODELS AND VALIDATION
CHAPTER
FINITEELEMENT MODELS This chapter presents the details of the finite element models used for the calculations tabulated in Appendix A. It includes information about the geometries of all the models. Differences among the models (e.g. friction coefficients) are given in the tables in Appendix A; Chapter 15 presents the details of the material behavior used for all of the models. All of the finite element models used for the data presented fall into the following three categories: 2D models of butt joints, attachment joints and open hole panels [18,19] 3D models of single rivetrow lap and butt joints (including standard and countersunk rivet heads, interference and clamping, sealants and adhesives, biaxial loading) (1,1316) 3D models of double rivetrow lap, butt and doubler joints (standard and countersunk rivet heads) [l, 13,14,19,20,35] For each category, a basic model was developed and modified as needed. The basic models will be described below, followed by the details of the various modifications.All models were created and run using the finite element code ABAQUS. 13.1 2D models of butt joints, attachment joints and open hole panels
Two types of butt joint models have been developed: 2D and 3D (described in Chapter 13.2). The 2D model can also be used to represent pinned butt and attachment joints and open hole panels. The twodimensional pinned connection finite element model used to represent butt joints is shown in Fig. 13.1. Only the center panel is treated and interaction with the side panels is neglected. For calculations treating a finite plate, the pin was held fixed at its center while a tensile stress of 60 MPa was applied at the far edge of the plate along its longitudinal (2) direction. This stress corresponds to a load per unit thickness of the plate, Q = 1836 kN/m for the 30.6 mm panel width. For an infinite plate, a statically equivalent concentrated load, Q = 1836 kN, was applied to the center of the pin while the far edge of the plate was held fixed in the 2direction. In addition, to represent the case where there is a row of pins, and not a single pin, some calculations were performed on the finite plate with its sides held fixed in the lateral (1) direction, in addition to the longitudinal, uniaxial stress. Both the pin and plate were considered to be in plane strain. The panel is 30.6 mm wide and 168.3 mm 1ong.The center of the hole (and pin) is 15.3 mm from the lower edge and each of the sides of the plate. The radius of the hole is R = 3.06 mm. Only the case of equal pin and 189
Structural Shear Joints
190
+90"
ttttt
*lxoo
L 90"
Figure 13.1. Twodimensional finite element model of the pinned connection. A section of the deformed mesh near the contact region is shown on the right. The angular location convention and tangential stress around the hole, 000,are also shown, onom = 125 MPa.
hole radii was considered. The pin/hole radius, R, and finite sheet dimensions were derived from typical airframe riveted connections. A Coulomb friction model was assumed. Attachment joints have the same geometry as butt joints, but are held in place by one or more rigid fasteners; i.e. the fasteners and support structure are rigid compared to the panel. Open hole panel models consist of the panel shown in Fig. 13.1 without the pin. Models Which Include Biaxial Loading. In addition to the pin being fixed at its center, a tensile stress, OL = 125 MPa, is applied at the far edge of the panel in the longitudinal (1) direction as shown in Fig. 13.1. This is considered to be the principal loading direction. In is also applied. Three types and values of transaddition, a transverse (secondary) load, q, verse loading are considered: (i) Case 1,in which the sides of the panel are held fixed in the transverse (2) direction. This is the symmetry boundary condition imposed by the two adjacent, identical units, (ii) Case 2. in which a tensile stress of 62.5 MPa is applied in the transverse direction along the sides of the panel, and (iii) Case 3 , in which a fixed displacement of k13.66 pm is applied all along the sides of the panel.The longitudinal and transverse loads are applied simultaneously in all cases. 13.2 3D models of single rivetrow lap and butt joints (standard and countersunk rivet heads)
The basic single rivetrow lap joint model is shown in Figure 13.2.The model geometry consists of two partially overlapping sheets (panels) coupled by a rivet. This represents one half
Finite Element Models
,
i
I
..... .....
I
191
, I I I , .
. . / /
I .
<
io ojo 0 ; ; j
./ I
1 1
I
;. ;.
I
I 1

modeled region
..
,
I 1
..
.....
anel
1': ' ' ' " ' "I
........
r2 1
0
I
Ll Halfsymmetry plane
C
E
F Multirivet symmetry plane
Figure 13.2. (a) Multiriveted, singlerowlap joint, of which onehalf unit is considered for the 3D halfsymmetry finite element model (b) the thickness of each panel is t = 1.53 mm; the rivet shank diameter is 6.12 mm; the rivet head diameter and height are 9.792 mm and 3.83 mm respectively (c) plan view of mesh. The overall length of the model is 306 mm; the length of the overlap region is 30.6 mm; the width of the model (half the repeat distance) is 15.3 mm.
unit of a multiriveted, single row, long panel extending infinitely in the positive and negative 2directions.The repeat distance between successive units is 30.6 mm. The upper panel may possess a countersunk hole. Finite element analysis (FEA) was performed using the ABAQUS code; 27noded brick elements were used to mesh the three bodies, and singlenoded slide surface elements were defined internally to solve the contact inequality constraints. The four rivet geometries considered are: (1) A double headed rivet with no countersinking, (2) A rivet with one standard head at its lower end and one head countersunk to a depth of half the thickness of a single sheet, the included angle being loo", (3) A rivet with one standard head at its lower end and one head countersunk to a depth of the thickness of a single sheet. In this case, the maximum and minimum diameter remain unchanged, resulting in an included countersink angle of 61.6", and, (4) A rivet with one standard head at its lower end and one head countersunk to a depth of the thickness of a single sheet which contains a 100" angle. A nominal tensile stress is applied at the nonlapping end face (DF) of the upper sheet, while the corresponding face belonging to the lower sheet (CE) is fixed along the 1axis. Figure 13.2 shows the main features of the models. For the infinite panel, planes (13) CD and EF are symmetry planes and are constrained against motion in the 2direction. In
192
Structural Shear Joints
F
i
+15 I.E+OB
Figure 13.3. (a) Schematic of the 3D butt joint model as derived from the existing lap joint model including only the shaded portion of the sheets and half the rivet, (b) 011 stress contours for the 3D butt joint model (deformations are magnified 3x, applied stress is 60 MPa).
addition, the edges parallel to the 2axis, and on 23 planes DF and CE are fixed in the 3direction to prevent unrestrained rotation of the body in space. All the boundary conditions are symmetric. For finitewidth panels, the multirivet symmetry plane (13) along EF, shown in Figure 13.2, is further constrained against motion in the 1 and 3directions, so that it is no longer a symmetry plane. Values of the friction coefficients used in the various models along with applied nominal tensile stress are presented in the tables in Appendix A. The finite element meshes might typically consist of 3171 user defined nodes, 252 user defined elements and 609 internally generated contact elements. A typical figure for the total number of variables is 11,340. Models Which Represent Butt Joints. Figure 13.3a shows a schematic of the butt joint model. The shaded portion and half the river are considered in the model. This model was
Finite Element Models
193
TABLE 13.1. THE FINITE ELEMENT MODELS WHICH INCLUDE INTERFERENCE AND CLAMPING ~~~~
Rivet Heads
4C26 4C27 4C28
I 1 standard 1 countersunk (100') to half panel thickness 1 standard 1 countersunk ( 100') to half panel thickness 1 standard 1 countersunk (100') to half panel thickness
2
0
0
0.5
2
0.5
derived from the existing lap joint model by deleting the lower head of the rivet. The loads are shown for the resulting butt joint. Since the crosssectional area of the central sheet is trwice that of the abutting sheets, the nominal strress in all the sheets is identical. For 0.5% clamping, a nominal applied stress of 60 MPa and frictionless contsct, the net section peak stess is 330.8 Mpa (SCF = 5.5) and the fross section peak stress ie 67.4 MPa (SCF = 1).Both these values are obtained from sheet #l. The peak net section stress is in sheet #1; the peak gross section stress could be in sheet #2. The length of sheet #1 can be easily shortened for future calculations. Figure 13.3b shows the 6 1 1 stress contours for this analysis. Models Which Include Interference And Clamping. Table 13.1 indicates the values of initial residual stresses considered for the interference and clamping analyses. Forcing radial conformity between an initially oversized rivet shank and the panel holes simulated the effects of rivetpanel interference stresses. In this case the interference is produced only in the radial direction. Clamping stresses were generated by forcing the elongation of a rivet whose initial shank height is slightly less than the combined depth of the two panels (z = 2t). The clamping forces were also introduced by an interference (misfit) method. Table 13.1 indicates the individual amounts of interference and clamping misfits analyzed, where the misfit is expressed as a percentage of the panel hole diameter (6.12 mm) or combined panel thickness (3.06 mm). For these analyses a nominal, remote cyclic load defined by d o = 90 MPa and R = 0.1 was applied at the nonlapping end face of the upper sheet while the corresponding face
194
.....
Structural Shear Joints
A .I ,.
I '
!
onehalf repeat distance
+ +
I
....
I
I;
I . . I
I . ' I I .
I
. . . . .I
..... ...
/ /
/i. ..
1 00 0 0
! I ;
I
, I
anel
. /
I ,
I
;. ;. o m o d e l e d region
I
I ,
I
.....
.. I , ..
Halfsymmetry plane
C
CT E Multirivet symmetry plane
i .
Figure 13.4. (a) Multiriveted, singlerow lap joint, of which onehalf unit is considered for the 3D halfsymmetry finite element model (b) the thickness of each panel is t = 1.53 mm; the rivet shank diameter is 6.12 mm; the rivet head diameter and height are 9.792 mm and 3.83 mm respectively (c) plan view of mesh. The overall length of the model is 306 mm; the length of the overlap region is 30.6 mm; the width of the model (half the repeat distance) is 15.3mm.
belonging to the lower sheet was fixed along the xaxis; the Cartesian systems (1,2,3) and (x,y,z) are equivalent. Ballonflat fretting tests conducted for aluminum rubbing against itself have shown the friction coefficient, p, to vary from 0.2 to 0.5 [20]. The slip amplitude in these tests ranged between 10 ym and 80 ym and the normal load between 28.2 N and 34 N; the frequency was 1 Hz. For this study, the variation in p was neglected, and the Coulomb friction model with a constant value of p = 0.4 was assumed for all interfaces. Models Which Include Sealants and Adhesives. The modeling of sealants and adhesives was performed using the TALA method; this approach is described in detail in Chapter 14. These studies used the basic single rivetrow lap joint model described above with some variations in nominal applied load, panel thickness and material properties. These details are presented in Table A.9. Models Which Include Biaxial Loading. Figure 13.4 shows the additional loading applied along the panel length for the biaxial case.Table 13.2 indicates the magnitudes of transverse
195
Finite Element Models
TABLE 13.2. THE FINITE ELEMENT MODELS Model
Rivet Heads
Transverse Boundary Condition
4S16
Both panels' sides constrained
2 standard
4S 17
Transverse stress applied to panel sides
2 standard
4S18
Transverse displacement applied to panel sides
2 standard
4C 17
Both panels' sides constrained
1 standard, 1 countersunk (100') to half panel thickness
4C18
Transverse stress applied to panel sides
1 standard, 1 countersunk (100') to half panel thickness
4C19
Transverse displacement applied to panel sides
1 standard, 1 countersunk (100') to half panel thickness
loading; three types and values of transverse loading are considered: (i) Case 1,in which the sides of the panel are held fixed in the transverse (2) direction. This is the symmetry boundary condition imposed by the two adjacent, identical units, (ii) Case 2, in which a tensile stress of 62.5 MPa is applied in the transverse direction along the sides of the panel, and (iii) Case 3, in which a fixed displacement of f13.66 pm is applied all along the sides of the panel. The longitudinal and transverse loads are applied simultaneously in all cases. 13.3 Double rivetrow lap joints (standard and countersunk rivet heads)
The model geometry consists of two partially overlapping sheets (panels) fastened by two twoheaded, noncountersunk rivets, shown in Fig. 13.5. This represents one half unit of a multiriveted, double row, long panel extending infinitely in the positive and negative 2directions. The repeat distance between successive units is 30.6 mm. Finite element analysis (FEA) was performed using the ABAQUS code; twentyseven noded brick elements were used to mesh the three bodies and singlenoded slide surface elements were defined internally to solve the contact inequality constraints.Two rivet geometries are treated: (1)A double headed rivet with no countersinking, and, (2) A rivet with one standard head at its lower end and one head countersunk to a depth of the thickness of a single sheet which contains a 100" angle. A nominal tensile stress is applied at the nonlapping end face of the upper sheet, while the corresponding face belonging to the lower sheet is fixed along the laxis. Figure 13.5 shows the main features of the models. Planes (13) CD and EF are symmetry planes and are constrained against motion in the 2direction. In addition, the edges parallel to the 2axis on (23) planes DF and CE are fixed in the 3direction to prevent unrestrained rotation of the body in space. All the boundary conditions are symmetric for infinitely wide panels.
Structural Shear Joints
196
._
...
rivet
1
rivet
C
E
multirivet symmetry plane
Figure 13.5. (a) Multiriveted, doublerow riveted lap joint, of which onehalf unit is considered for the 3D halfsymmetry finite element model (b) the model consists of two rivets (#1 and #2) installed in two holes (#1 and #2 respectively).The thickness of each panel is t = 1.53 mm. The noncountersunk rivet shank diameter is 6.12 mm and the countersunk rivet diameter is 7.94 mm; the rivet head diameter and height are 9.792 mm and 3.83 mm respectively (c) plan view of mesh. The overall length of the model is 336.6 mm and the width of the model is 15.3 mm (half the repeat distance); the length of the overlap is 61.2 mm.
Values of the friction coefficients used in the various models along with applied nominal tensile stress are presented in the tables in Appendix A. A typical finite element mesh for a double rivetrow lap joint consists of 5832 user defined nodes, 472 user defined elements and 1213 internally generated contact elements. The total number of variables is 21,135.
CHAPTER
14 THINADHESIVE LAYER ANALYSIS (TALA) FOR MODELING SEALANTS AND ADHESIVES INSTALLED IN JOINTS 14.1 DEVELOPMENT OF A THIN ADHESIVE LAYER ANALYSIS (TALA)
Modeling of a sealant layer using FEA is not practical because the thickness of the sealant layer is so small compared to the panel dimensions. TALA avoids this problem by representing the sealant using spring elements connecting two contacting surfaces, eliminating solid element representation of the sealant layer in the finite element models (see Figure 14.1).Thus, each pair of coincident nodes between two contacting surfaces in the finite element models is connected by spring elements (defined as SPRING2 element in ABAQUS). The mechanical behavior of the springs must be defined in local normal and local shear directions in the finite element models. The stresses and strains in the springs are converted to forces and displacements interacting between the two contacting surfaces. The properties of the adhesive are treated as isotropic and time and load rate independent. This chapter is based on References [6] and [21]. The nomenclature for this chapter is listed at the end of the chapter. 14.2 CONVERSION OF ADHESIVE SOLID ELEMENTTO SPRING ELEMENT FOR 2D FEM
Two methods are used for changing the solid adhesive element to spring elements: one for interfacing 4noded elements and the other for 8noded elements. Each method requires different values for Ai as described below. 197
198
Structural Shear Joints
Local directions
1z’
Solid element i
Force in spring i
Displacement in spring i
Figure 14.1. Schematic of spring representation of solid adhesive element.
1. One solid element to one spring method (for 4noded elements). This method is used to change one solid adhesive element to one spring as shown in Figure 14.2(a). It changes adhesive element i (bonding elements Ui and Li) to spring Si. A spring Si is composed of two spring elements, connecting node ui with node Zi, a normal and a shear spring element. The area for spring Si is equal to
Where
w = the width of each element (in y’direction) along the interface line d = the depth of each element (in x’direction); this value is always one unit for twodimensional plane strain.
2. One solid element to three spring method (for 8noded elements).This method is used to change one solid adhesive element to three springs, as shown in Figure 14.2(b). It changes adhesive element i (bonding panel elements Ui and Li) to springs Si  I, Si and Si + I. The spring Si 1 is composed of two spring elements connecting node ui1with node li 1 , a normal and a shear spring element. The area for spring Si  I is:
Where w = is the width of each element (in y’direction) and d = depth of each element (in x’direction). Similarly, the spring Si is composed of two spring elements connecting node ui with node li in the normal and shear directions. The area for spring Si is
These two surfaces are coincident
' X Y
I
I
b'
These two surfaces are coincident
Thickness of thin adhesive layer, h
Figure 14.2. Schematic of springs between two interfacing surfaces for two dimensional finite element model (a) using one spring, and (b) using three springs.
a'
a
b'
Thickness of thin adhesive layer, h
200
Structural Shear Joints
Aj = (wj/2). d
(3)
[(w~+I /4)+ (wj/4)/* d
(4)
The area for spring S;+l is Ai+l =
Conversion of adhesive solid element to spring element for 3D FEM. For the threedimensional finite element model, the change from thin solid adhesive elements to spring elements is based on the same idea used for the twodimensional problem; however, the area for each spring (Ai) must be calculated differently. Figure 14.3 shows the features of the threedimensional finite element with elements Uj and L; bonded by a thin adhesive layer. Nodes on surface abcd of element Uj and a’b’c’d’ of element Lj are coincident.The thin adhesive element i bonding the two surfaces of elements Uj and Lj are changed to 9 springs for use with 27 node isoparametric elements, etc. Spring (Si) connects nodes uj and li together, etc. Each spring is composed of three spring elements, one normal spring, and two shear springs. Areas D;through Di+8 are shown schematically in Figure 14.3 and are used to obtain Aj through A;+8for the springs, as shown in Table 14.1.
14.3 CONVERSION OF STRESSSTRAIN RELATIONSHIP TO FORCEDISPLACEMENT RELATIONSHIP FOR THIN ADHESIVE LAYER
The adhesive layer is assumed to be very thin. Thus, the stresses a,, oy,,,z, zXy,zyr, zyn, E,, yxy, 3/yz, and yy,, as shown in Figure 14.1 are neglected using TALA. Only o,,T,, and zzy act between the two nodes. The normal stress (oz)is changed to normal force, while the shear stresses (z,,, zzy) are changed to shear force in each spring element. The normal and shear x ) are changed to normal and shear relative displacements in spring i. strains (E,, E ~f i, The equations used for converting the stresses and strains in the solid element to forces and displacements to define the properties of the spring element are presented below. In the normal direction (tension and compression spring), by Hooke’s law:
Where Fn,jisthe normal force transmitted in spring element i, vn,i is the relative displacement of spring element i in the normal direction, Kn,jis the local stiffness of spring element i in the
.+
14
.n
6
.3
3
1
201
Structural Shear Joints
202
Spring SI
I I
Spring Area A, =(Dl)/16
S+I
Al+I= (Dl)/l6+(D,+l)/16+(Dl+2)/1 6+(Dl+4)/16
s1+2
A,+*= (D1)/8+(D1+2)/8
sl+3 sl+4
I Al+3 (Dl)/16+(Dl+~)/16+(Dl+~)/16+(D,+~)/16 I I Al+4=(D1)/8+(Dl+4)/8 I =
local normal direction, and E is the elastic modulus of the adhesive. In the shear direction (shear spring) in x'y' plane zzxand zzyare equal in magnitude because the material is isotropic.
Where Fji is the shear force transmitted in spring element i, uji is the relative displacement of spring element i in the shear direction, Kji is the local stiffness of spring element i in the shear direction, and G is the shear modulus of the adhesive. For the case of a linear material, the values of Kn,iand Kji can be defined directly for spring element i in the normal and shear directions. However, for a nonlinear material Kn,i and Kj;i vary. Then, in order to define the nonlinear behavior for spring element i, pairs of forcerelative displacement values are required over a sufficiently wide range of relative displacement values. For more information about defining spring properties see Reference [86]. 14.4 MECHANICAL BEHAVIOR OF THIN SEALANT LAYER
In order to use TALA and ABAQUS to simulate the mechanical behavior of the layer, the actual behavior of the thin sealant coating must be fully described. Low weight aerospace
TALA for Modeling Sealants and Adhesives Installed in Joints
203
1.4 9 1.2
 1
$ 0.8 v v)
2 0.6 v,
G
0.4 0.2 0 0
1
2
3
4
5
strain (%)
1 100 n (d
a
z
200
8 CA
300
m
m
Figure 14.4.The uniaxial stressstrain relationship for a thin sealant coating layer 170 pm thick.
sealant (PR1776 B2 model 654) supplied by PRCDeSoto International, Inc. is used here. In the normal direction, the stressstrain relationship for a thin sealant coating layer of this material subjected to uniaxial static tension and compression loading is obtained by Fongsamootr [7], as shown in Figure 14.4. In the shear direction?data for the sealant, subjected to combined torsion and compression loading, are obtained by Kamnerdtong [8] as shown in Figure 14.5.
Structural Shear Joints
204
Shear stressstrain relationship of thin sealant coating layer at contact pressure 0 to 350 MPa __ . +Pressure=O MPa +Pressure=150 MPa I
7
5
+Pressure200 MF'a
*Pressur~300MPa
3
++ Pressur~350MF'a
1
0.5
0.25
7
0.75
1
5
shear stressstrainrelationshipof thin sealant coating 1 a F at contactpessure4OOto6OOMPa JJ
I
tpKsudooMPa
+Pnsm==450MPa n
5
+plEaE=mMPa
plesw&mMPa
W I
IA
g 1.25
0.25
1
0.5
0.75
1
1
1
c
G
JJ
strain (%) Figure 14.5. The shear stressstrain relationships for a thin sealant coating layer 100 pm thick.
TALA for Modeling Sealants and Adhesives Installed in Joints
205
14.5 SHEAR SPRING DEPENDENCE OF CONTACT PRESSURE
A procedure for the determination of the pressure dependent stressstrain behavior for the shear spring is described here. Figure 14.5 gives shear stressstrain relationships for various pressures (inbetween values are obtained through interpolation). To start with, the contact pressure is assumed to be zero. After the first ABAQUS run, the normal force in each spring is output (DAT file). If the value of the normal force (F,,j) is tensile or zero, the forcedisplacement relationship for the shear spring is kept constant. This is because shear behavior data was not obtained as a function of tension, thus the assumption is made that tension has a negligible affect on the sealant shear properties. If the value of the normal force (F,,i) is compressive, the compressive force is divided by the small area (Ai) to get the new value of the contact pressure (Pi) for that spring element. Then, for the next run, the shear spring of that element is redefined to have a new shear forcedisplacement relationship from the new contact pressure. Using this idea, the model is run repeatedly and the shear spring is redefined until the new contact pressure and previous contact pressure for each spring converge. EXCEL is used to provide a new input file for each new run and to define new shear spring pressure dependence following Pinewfor each spring. Symbols A, = Nominal area for ith spring E = elastic modulus of adhesive F,,i, Ff,i = normal, shear force transmitted in ith spring element G = shear modulus of adhesive K,,i, Kf,i = local stiffness of ith spring element in the local normal, shear directions n, f = normal, shear forces pi = contact pressure for i'h spring S, = ithspring ufi = relative displacement of ith spring element in shear direction Ui, li = nodes connected by ith spring Ui, L,= Elements bonded by ith spring v,j = relative displacement of ithspring element in the normal direction wi = width of ith element (in y'direction) along the interface line o,y = normal, shear stresses
CHAPTER
MATERIAL MODELS FOR THE FINITE ELEMENT CALCULATIONS This chapter presents the details of the material behaviors used in the finite element and TALA calculations. The sealant properties for the TALA calculations are described in Figures 14.4 and 14.5. 15.1 Materials used in the finite element calculations
There are a total of 5 pinpanel material combinations used in the calculations summarized in Chapter 7: (1) (2) (3) (4)
Aluminum pinAluminum panel Steel pinAluminum panel Titanium pinAluminum panel Aluminum pinEpoxy panel ( 5 ) Steel pinSteel panel
Of these, the only nonlinear treatments are for the AluminumAluminum models for which most are linear with a few examples of elasticisotropicplastic (EIP) and elasticlinearkinematic hardeningplastic (ELKP). The material properties used for all of the uniaxial tension cases, except as noted in Table A.7, are presented in Table 151. In the case of biaxial loading for butt joints, the combinations of linear material properties used are shown in Table.152.
207
Structural Shear Joints
208
Material Aluminum (linear) Aluminum WP) AA7075T6
Elastic modulus, E (GPa)
Poisson’s ratio, v
Yield strength (MP4
70
0.30

70
0.30
53 1
0.70
0.30
369.9
57.5
0.25 0.3 1 0.36
_ __ _

\ 70 (ELKP) Steel Titanium Epoxy
207 117 3
Plastic modulus, M (slope, GPa)
TABLE 15.2. SUMMARY OF MATERIAL PROPERTIES IN BIAXIAL LOADING CASES FOR BUTT JOINTS
_
___
CHAPTER
16 VALIDATION OF
FINITEELEMENT CALCULATIONS AND TALA 16.1 FINITE ELEMENT MODEL VALIDATION
The validity of the finite element analyses has been tested in a number of ways: 1. The 2D finite element model of a large panel with an empty, open hole was compared with the closed form solution described by Timoshenko [29]. The SCF derived from the finite element model, SCF = 3.0 is identical to the closed form solution value. 2. The 2D finite element model of a pinned connection was compared with strain gage and photoelastic measurements [87]. Table 16.1 summarizes the calculated and measured SCFvalues. The two sets of results are in good accord when the differences in P1/D are accounted for. 3. The 2D finite element analysis of a frictionless, pinned connection [1,18] was compared with the corresponding, closed form solution of Cavaella and Decuzzi [25]. As illustrated in Figure 16.1, the finite element model accurately reproduces the pressure distribution of the closed form solution. 4. To test the adequacy of the 3D model mesh refinement, the mesh was employed to analyze a finite, pinned connection with friction under in plane loading. The results are compared in Figure 16.2 with those obtained with the more refined mesh of the 2D finite element analysis. The two sets of results for contact pressure and slip distributions are in good agreement. The difference in SCF obtained using the 2D and less refined 3D mesh under inplane loading is about 7%. 5. To test the adequacy of the 3D finite element analysis for treating outofplane distortions an analysis of a single, rivetrow lap joint was compared with experimental measurements of the joint inplane and outof plane displacements [1,16]. The results are summarized in Figure 16.3. The calculations predict the variations of displacement with load and the absolute values of displacement within 10%. 6. A further test of the 3D finite element analysis of a single, rivetrow lap joint is obtained by comparing the results of Fung and Smart [88,89] with another 3D finite element model of a different lap joint. Table 16.2 illustrates that the finite element calculations produce comparable SCF values when differences in Pl/D and D/t are taken into account.
209
Structural Shear Joints
210
TABLE 16.1. COMPARISON OF THE MEASURED STRESS ELEVATION IN A BUTT JOINT [87] WITH FINITE ELEMENT ANALYSIS VALUES [18] METHOD Strain gages
I PANEL/FASTENER 1 I Steel/Steel I
Photoelastic
Fosterite/Fosterite
Finite element analysis (Model 3P 16)
AluminudAluminum
a
PI/D 3.76 5.0" 4.2 4.2 5.0 4.2"
I
eo 1 0" 0" 0" 14" 4"
I
a/olor SCF 5.1
5.5 5.0 6.3 6.6 6.3
4"
Estimate for PJD=5 obtained with Figure 5.2.
.
0.7
.  I

Closedform solution 0.3 t
02
t
+ 01 I
I
b
Figure 16.1. Finite element and analytical solutions for the contact pressure distribution in a pinned connection with an infinite sheet.
16.2 VALIDATION OF THE THIN ADHESIVE LAYER ANALYSIS (TALA)
The validity of TALA was tested by comparing its predictions with two previous analytical studies and with experimental measurements.
Analysis of Reinforced Cantilever Beam. Cornell [90] has analyzed the response of a filleted brazed tab specimen: two cantilevered steel beams bonded using a brazed layer (see Fig. 16.4).Cornell's model consisted of two linear elastic beams bonded with an infinite number of linear tension and shear springs. In order to verify TALA, the brazed tab specimen was analyzed as a twodimensional plane strain finite element model with no fillet. The model uses 150 elements for the steel tab and 570 elements for the steel base bar. The braze bonding layer was transformed into 51 linear tensioncompression spring elements and 51
Validation of Finite Element Calculations and TALA
21 1
6 I,
A 5
3D solution at z = 0 mrn 3D solution at z = 0.765 rnm A 3D solution at z 2D
= 1.53 mm
Solution
0
\ 1.00E07
\ 90
75
60
45
30
15
0
15
30
45
60
75
90
8 (degrees)
(b) Figure 16.2. Comparisons of computed distributions of (a) the normalized contact pressure, p / o and (b) interfacial slip distance obtained from the twodimensional (2D) and threedimensional (3D) finite element models.
212 130 120
P
0
/
U
/
__1/__4 80 70
/
1
5
6
:
Structural Shear Joints
0
i:
ri 0
60 50 40
30 20
[+ 
~~~
n
&
Measured F E A (21 17 rivet) F E A (7075.T6 rivet)
10 0
np1000 1500 2000
1
::: 90
130
,
120 110 100 90 80 70
60 50 40
U
F E A (node 445)
A F E A (node 460)
30
20 10
2500
0
0
500
1
XiMeasured F E A (node 2954) +F E A (node 2969)
+
~
0
100
200
300
400
500
600
A. prn
Figure 16.3. Validity of the threedimensional finite element model based on comparisons of measured and computed values of (a) overall inplane joint displacement, and (b) and (c) outofplane panel movement near the rivet location.
linear shear spring elements using TALA [6,21J.The shear spring behavior is independent of contact pressure. / zxylomUx c ~ ~in the ~ braze ~ bonding layer The nondimensional stress distributions c ~ ~ and are compared in Fig. 16.4 with the analytical closedform solution obtained by Cornell [90]. It may be seen that the Cornell and TALA analyses are essentially in agreement. Small differences in the magnitude and location of the stresses are due to the fact that TALA does not include the braze layer fillet at the tab ending.
Validation of Finite Element Calculations and TALA
213
TABLE 16.2. COMPARISON OF SCFS OBTAINED BY IYER [l, 161 AND FUNG AND SMART [88]
I
I
Iyer (1,16)
Fung and Smart (76)
PI/D
5
4.4
Dlt
4
1.99
“(L)’
10
2
6.1 18.1’
7.3
9.8 I 10.7’
10.5
Joint F.E. Model ~~
E t
I Iyer FE model results are adjusted for Fung and Smart joint model geometry using Figures 2.5 and 2.6.
,
v r E
X=O
Base bar
0.8 0.7 0.6
0.5
. TALA normal h = 0.01 inch
0.4
0.3 0.2 0.1
0
0.1 0.2 Distance i?om tab ending (mch)
Figure 16.4. Normal and shear stress in braze bonding layer,h (thickness of braze layer) = 0.01.
Structural Shear Joints
214
r
\
Aluminum
I Y
\ Adhesive layer
TALA
2
04 0
steel
h=O.OlL
8 FEA'sE?aker&Hatth=O.OIL
8
0.25
0.5
0.75
I
N o n d i m i d Distance ( XiL)
I
1
it TALA
0.25
h = 0.001L
0.5
0.75
I 1
Nmdimensimal Distance x/L
(b)
Figure 16.5. Shear stress in thin adhesive layer, (a) h (thickness of adhesive layer) = 0.01L inch (0.254 mm), h = 0.001L inch (0.0254 mm). L is the overlapping length and 0 I x I L.
Analysis of Bimetallic Stepped Lap Joint. Baker and Hatt [91] use a linear elastic finiteelement analysis to evaluate the behavior of a twodimensional stepped lap joint (see Fig. 16.5).The aluminum and steel panels are fastened with a thin, linear high modulus adhesive layer. A special element is used which acts like a combined normal and shear spring between two plates (this method differs from TALA in the definition of the connections between coincident and adjacent nodes).
Validation of Finite Element Calculations and TALA
215
TALA was applied to a twodimensional plane strain finite element model of the stepped joint using 500 elements for the aluminum panel and 500 for the steel [6,21].Within TALA, the adhesive layer is transformed to 50 linear tensioncompression and 50 linear shear spring elements connecting the lower surface of steel to the upper surface of aluminum using the one spring method, as shown in Figure 14.2(a). The results of Baker & Hatt are compared with the TALA analyses in Figure 16.5 showing normalized shear stress (zlpo) along the overlapping length (nlL)for two different adhesive thicknesses.The TALA analysis results are in agreement with Baker and Hatt’s analysis in both shape and magnitude along the overlapping length. Measurements of lap joints. Experimental validation was obtained by comparing TALA calculations with the measured stressstrain behaviors of 3 aluminum lap joints fastened with a polymer adhesive:
(i) An ordinary lap joint (ii) A stepped lap joint, and (iii) A single rivetrow lap joint augmented with adhesive. The joints were fastened with thin, 6CL180 pm thick, layers of a low modulus, pressure sensitive, adhesive sealant (PRCDesoto PR1776 B2 model 654). The joint configurations, finite element models and the properties of the aluminum panels and the adhesive are described in detail elsewhere [6,21]. Figure 16.6 shows a comparison of the experimental and finite element relative inplane and outofplane displacement results at the same tensile loads. The calculations agree with the measurements for small applied loads. Small divergences for high loads are probably caused by stress relaxation in the sealant layer during the period of time that the displacements were held constant to allow for reading of the dial gauges.
Structural Shear Joints
216
Stress ( M P a )
Snns (MPaI 20
.,
20 IX
I6
14
TALA
12
tExperiment
IU
x 6 4
2
nin
000
Stress ( M P a )
060
050
Stress ( M P a )
90 1
1
90
020 030 040 Displacement ( m m )
TALA tExperiment
40 30
i 
7
o no
0 05
0 I0 Dirplacemenl (mm)
0 I5
0 20
o
n2
n4
06
ox
I
I2
Displacement (mm)
tress (MPa)
Strcss ( M P a )
O' 1
TALAI
rivet
tExperiment3 rivets tTALAI rwel
7 7
0.00
0 05
0 in
Displacement (mm)
0 15
0.20
no0
n 20
041) 060 D isplaccment
0 KO
1.00
Figure 16.6. (a), (b) and (c) compare the measured and calculated inplane displacementnominal stress relation for adhesive lap joint, adhesive stepped lap joint, riveted lap joint, respectively. (d), ( e ) and (f) compare the measured and calculated outofplane displacementnominal stress relation for adhesive lap joint, adhesive stepped lap joint, riveted lap joint, respectively.
CHAPTER
17 STRESSCONCENTRATION FACTORS IN MULTIPLE Row JOINTS 17.1 ANALYSES OF MULTIPLE ROW JOINTS
The distribution of fastener loads acting at the several rows of multiple row attachment, butt and lap joints and doublers can be used to estimate SCFs in these joints. Chapter 17.1 outlines a general analytical approach. Chapter 17.2 describes a semianalytical procedure and 1dimesional, 2springs models for estimating the fastener load distribution of joints with 3dimensional deformation. Chapter 17.3 describes a superposition method which, together with the fastener load distribution and the numerical result for the SCF of singlerow joints, provides estimates of the SCFs in multiple row joints. The reliability of the SCF predictions is examined in Chapter 17.4. 17.2 ESTIMATING FASTENER LOADS IN MULTIPLE ROW JOINTS
Equilibrium. The load applied to the panel of a multiple row shear joint is progressively transferred to the facing panel(s) by the successive rows of fasteners. The quantities Q1, Q2, and Q, are the loads transmitted to the fasteners in the first, second and subsequent rows: Q = Q 1 + Q2
.... + Qn
(17.1)
where Q = CY t P1 is the total fastener load. Equation (17.1) is the onedimensional equilibrium statement. It is convenient to describe these quantities in terms of fi, the fraction of the total fastener load supported by fasteners in the different rows, i.e., fi = Qi /Q.
Compatibility. The total extension of the segment of panel between any two specific fastener rowsthe distortion of the fastenerfastener hole combination plus that of the panelmust equal the total extension of the facing segment between the same two rows. The fraction, fi, is then defined by imposing two conditions: (1) the matching of the extensions of 217
218
Structural Shear Joints
facing segments of panel, and (2) static equilibrium. Estimates of the fastener load distribution can be obtained for butt joints with the equilibrium and compatibility conditions described above,This procedure is described by Kulak, Fisher and Struik [51]. In joints which exhibit nonnegligible outofplane movements, 3D equilibrium and compatibility conditions must be satisfied and a closedform analysis of the problem is complex. In the next section, a semiempirical procedure for estimates of the values of f j for the general case involving threedimensional panel and fastener deformations is provided.
17.3 ESTIMATING FASTENER LOADS WITH 3D DEFORMATIONS
Under conditions involving threedimensional deformations, the elastic behavior of the fastenedfastener hole combination can be expressed in terms of the excess compliance, C: the difference in the compliance of a single fastenerrow structural joint and the compliance of a single uniform panel with the same overall dimensions (see the introduction to Chapter 12). ThoSprings Models of Shear Joints. Swift [24], Muller [34] and the present authors have implemented equilibrium and compatibility using the excess compliance idea and the onedimensional, 2 (linear)spring models of shear joints shown in Fig. 17.1. One set of springs simulates the fastenerfastener hole response and the other the intervening panel. The models are essentially the same though the terminology used is slightly different. Swift and Muller formulate the problem in terms of C, the compliance of the spring simulating the fastenedfastener hole and Cp, the compliance of the intervening strip of panel.They refer to the two compliance values as the fastener (or rivet) flexibility and the sheet flexibility. Similar to concepts and models have previously been proposed by Huth [92] and Swift [24]. The present authors have formulated the problem in terms of k and K, the stiffness of the springs simulating the fastenedfastener hole and the intervening strip of panel, and the k/Kratio, where: k = el,K
=
Cpl, and k/K = Cp/C.........
(17.2A, B, and C)
These parameters can be evaluated in a number of ways. The quantity C is identical to the excess compliance of a single, rivetrow joint which the authors have evaluated with the finite element models (see Chapter 12 for definition and tabulated values). Alternatively, Huth [92] and Muller [34] have obtained values of C from load displacement measurements of joints. The value, k = 17 MN/m derived from a finite element analysis for a lap joint with countersunk rivets is in accord with the value, k = 14MN/m derived by Huth [92] from measurements for a similar joint. Empirical expressions for C have been formulated by Huth [90,92],Tate and Rosenfield (931 and workers at Boeing [34,94].The value of K is estimated as: K
= qE
t P1/P2 .........
(17.3)
where E is the elastic modulus of the panel material; t is the panel thickness; PI is the fastener pitch (spacing); P2 is the fastener row spacing, and q accounts for the effects of the none uniform stress distribution and other features neglected by the simplified model. Muller [34] employs the approximation, q = 1. The authors evaluated the quantity, q, by
Stress Concentration Factors in Multiple Row Joints
219
c
Q
Figure 17.1. Examples of 2spring models for estimating fastener loads of multiple row, shear joints: (a) Model of a %row attachment joint, (b) Model of a 3row butt or lap joint, and (c) Model of a 3row doubler.
comparing the fastener load predictions of the 2spring models of attachment joints with results of finite element calculations.Values of C, k and the k/Kratio for different types of joints are summarized in Table 17.1 for cases where the panels composing the joint are the same thickness. Once the values of k and K are known, the fastener loads, fi, can be estimated solving the appropriate linear 2spring problem. Huth [92], Swift [24] and Muller [34] present the esti
Structural Shear Joints
220
TABLE 17.1. EXCESS COMPLIANCE, STIFFNESS AND k/K RATIOS OF DIFFERENT SHEAR JOINTS FOR Pi/D = 5, D/t = 4, AND P2/P1= 1 JOINTiHEAD r s PIID, MPa Al, buttistd 30 5 Al. buttistd 5 Al, buttistd 30 5 Steel, butvstd 126 5
D$t
C k K M/GN MN/m MNim 16 63 343 13 88 224 343 5 200 1.9 526 1013
Method' %CI %X
2 2.4 2 2
FE M FE FE
0 0 0.5 0.9
0 0 0 0
0 0.5 0 0
0 0 0 0
Al, lapistd Al, lapistd Al, lapistd Steel, butt/std
30 30 126 126
5 5 5 5
4 4 4 4
FE FE FE FE
Al, lapicsk Al, lapicsk Al, lapicsk Al, lapicsk Al, lapicsk Al, lapicsk Al, lapicsk Al, lapicsk
100
5 5 5 5 5 5 5 5
4 4(t=l) 2.2 (t=2.2) 2.4 2 I .2 4(t=l) 2.2 (t=2.2)
FE M M M M M M M
0 0 0 0 0 0 0 0 0 0 0 0 0 Yes' 0 Yes2
WK Reference 0.18 3sI (33) 0.39 (70) 0.58 3s2 (33) 0.52 3s3 ( I )
35 25 35 12
29 40 29 83
171 171 171 507
0.17 0.23 0.17 0.16
33 56 30 32 40 21 34 16
30
172 112 246 172 172 172 112 246
0.17 0.16 0.13 0.18 0.15 0.28 0.26 0.26
18
33 31 25 48 29 63
4S29(33) 4S30(33) 4s1 (1) 4S5(1)
~
FEfinite element calculation; Mmeasured *With hole expansion, amount not specified I
mates of fi derived from the 2spring models for different joints, but they do not document the relations between fi and the k/K (or Cp/C) ratio defined by the models. The expressions for the fastener loads and load fractions for different types of multiple row joints are summarized in Tables 17.2,17.3 and 17.4.Estimates of the values of f, for different joints and number of fastener rows are summarized in Table 2.5 in Chapter 2.6.
TABLE 17.2. EXPRESSIONS FOR THE FASTENER LOAD RATIOS, fi, DERIVED FROM THE 2SPRING MODEL FOR MULTIPLE ROW LAP AND BUTT JOINTS NUMBER OF ROWS
PROPERTY
ROW 1
2
FASTENER LOAD, Q FASTENER LOAD FRACTION, t;
0.5
0.5
FASTENER LOAD, Q FASTENER LOAD FRACTION, t;
QI I / [3WK]
QI [lWKI [Ik/K] / [3WK]
3
4
ROW 2
QI
FASTENER LOAD, Q QI FASTENER LOAD FRACTION, t; I / [42WK]
Qz
=
ROW 3
QI
Q~FQI l/[3kK]
QI [IWKI Q I [ 1 k/KI [IWK] / [42WK] [ l  k K ] / [42k/K]
* Expressions apply to joints consisting of panels of equal thickness.
ROW 4
Q4=Qi
1 [42WK]
Stress Concentration Factors in Multiple Row Joints
221
TABLE 17.3. EXPRESSIONS FOR THE RATIOS, Qi / Q1, AND FASTENER LOAD FRACTIONS, fi, DERIVED FROM THE 2SPRING MODEL FOR MULTIPLE ROW A'ITACHMENT JOINTS NUMBER OF ROWS
ROW1
ROW 2
ROW 3
2
1
1 / [I+!dK]
3
1
A**
A / [l+k/K]
4
1
B***
AB
ROW 4
AB / [I+WK]
*Note: the fastener load fraction, f = (Qi /Q1)/ (ZQiiQ1) ** A = 1 / { 1 + k / K + k / K [ I+k/K]}
*** B=l/(l+WK+Ak/K+Ak/W[Ik/K])
TABLE 17.4. EXPRESSIONS FOR THE FASTENER LOAD FRACTIONS, Fi, DERIVED FROM THE 2SPRING MODEL FOR MULTIPLE ROW DOUBLERS FASTENER LOAD FRACTION, fi NUMBER OF ROWS
ROW1
ROW 2
2
P k&
P WKS
6
a[k/K+ f,]
a[k/K2kf,iK+f3]
ROW 3
ROW 4
ROW 5
ROW 6
P k/Ks[12f,2f2]
fl k/Ks[12f,2f,]
a[kK2kf,K+f3]
a[k/K+ f2]
a = [ 1+2WK]', P=[ 1+2k/KS]'l The quantity K is the stiffness of the strip of panel between 2 adjacent fastener rows; Ks is the stiffness of the stri[ of panel between the symmetry axis and the adjacent row of fasteners (see Figure 17.1).
17.4 A SUPERPOSITION METHOD FOR ESTIMATING SCFs
With knowledge of the fastener load distribution, the SCFs in a multiplefastenerrow joint can be estimated. A method that superposes the effects of fastener loading and load transmitted to the next fastener row is provided.
Bearing Mode. Panel stresses generated at a particular row of fastener holes by the bearing mode component of the fastener load arise from the superposition of two stress fields. One component is produced by the fastener load, Qi, the other is produced by the bypass
Structural Shear Joints
222
load QBP, the portion of the load on the panel reaching a particular row that is not transferred to the fasteners but remains in the panel and is transmitted across the fastener holes and down the panel to the next row of fasteners: QBP,A
=
Q  Qi, QBP, B = Q  Qi  Q2, and QBP, c = Q  QI
 Q2  Q3,
etc
(17.4)
where QBP, A, Q B B~ and QBP, c are the bypass loads for the leading and successive rows of holes, respectively. The bypass load acting on the fastener hole produces a stress field approximated by the field of a filled, open hole panel (see Figure 1.4b) An estimate of the SCF is obtained by summing the SCFs produced by the two components of the field: 1. Contribution of Fastener Load. The reductions of the fastener loads acting in multiple row joints are accompanied by reductions in the peak panel stresses. The SCF produced by the fastener load at a particular row i, SCFFL,~ is approximated by the SCF of a comparable single row joint diminished by the factor, fi : SCFFL,~ = f i (SCFSINGLE ROW) .............
(17.5)
In this context, comparable implies that the SCF for the single row joint reflects the same mix of bearing frictional load existing in the multiple row joint. 2. Contribution of Bypass Load. An estimate of the S C F B ~the ~ , SCF produced at row i by the bypass load, is obtained by assuming that it is comparable to the SCF of a filled (open) hole panel', SCF = 2.5, diminished by fgP,i = Qsei/Q, the fraction of the total load that bypasses that row. SCFBei = fBei (SCFFILLED HOLE)= 2.5 fBl?i .. .....
(17.6)
where: fFB,A =
1  f l , fFB,B = 1 f l
 f2,
etc. ......
(17.7)
The SCF at a particular row of a multiple row joint, SCFi, is the sum of these 2 contributions:
+ SCFBP,(=fi (SCFSINGLE ROW) SCFi = SCFFL,~
+ 2.5 fBP,i ....
(17.8)
The quantity, SCFi = o*i/o,relates the peak local stress to the nominal (gross section) stress applied to the paneL2 Estimates of the SCF of different multiple row joints derived from the 2spring model and the superposition method are listed in Table 2.5. Clamped Mode. Clamping shields the edge of the fastener hole from stress. The finite element calculations show that the SCFs for a fully clamped, single fastener row and doublerow butt joint, P'/Ds = 5 , Ds/t = 4, (Table 3.4, Chapter 3.1) are the same. According to the superposition method, this means that relevant bypass SCF for the clamping mode is
'
Earlier findings for a narrow, single fastener butt joint with free edges showed that the SCF of a filled hole panel is 2.85 at 22" and 158". 2.1 at 0" and 180". Since the peak values of single row shear joints generally fall between these 2 locations, the SCF of the filled hole was approximated by the average value, SCF = 2.5. This value was used to estimate the SCFs listed in Tables 2.5 and 17.5. More recent findings for a wide butt joint (see Figure 17.2) show the filledhole SCF = 2.6 at 0" and 180". The authors believe the 4% difference is within the uncertainty of the estimation procedure. It should be noted that the reductions of the SCFs of multiple row joints arise from the reductions of the fastener loads rather than a reduction of the stress concentrating power of the fastenerhole configuration.
Stress Concentration Factors in Multiple Row Joints
223
SCFBP= 1.8 compared to SCFBP= 2.5 for the bearing mode. The implication is that the benefits of multiple fastener rows are meager for clamped butt because their single row SCF, (SCF = 1.8 for P1/Ds = 5, Ds/t = 4) is close to the bypass value. The bearing mode SCF is dominant when load transfer proceeds by a combination of the bearing and clamping mode. In that case, estimates of the bearing mode SCF can be obtained following the methods described above after reducing the fastener load by the amount supported by clamping.
Hole Expansion. Estimates of the fastener and bypass loads of multi row joints fabricated with hole expansion can be derived from the 2springs models with the appropriate stiffness ratio. These loads may ultimately be helpful for predicting the strength reduction factor (SRF) of multi row joints (see Chapter 4.3). The analytical approach presents problems because the SCF is not a valid descriptor of the elasticplastic, stressstrain states of joints with expanded holes. Alternative descriptors, such as the peak plastic strain amplitude, are difficult to evaluate with existing finite element capabilities.The experimental approach, correlation of the SRF with number of fastener rows, is obviated by the absence of data for hole expanded joints. 17.5 VALIDATION
Load distributions derived from the 2spring model are validated by finite element calculations and estimates from other analyses by Swift [24] and others [92941 as shown in Tables 17.5 and 17.6. The finite element calculations of the SCFs of multiple row attachment joints in Table 17.5 are also in good agreement with the values obtained with the superposition method.
TABLE 17.5. COMPARISONS OF ESTIMATES OF THE FASTENER LOAD FRACTIONS, fi, AND SCFS FOR MULTIPLE ROW ATTACHMENT JOINTS DERIVED FROM THE 2SPRING MODEL, FOR k/K = 0.5, AND THE SUPERPOSITION METHOD WITH FINITE ELEMENT CALCULATIONS. NUMBER OF ROWS
SOURCE
1
(2PI)
2
2 Spring Model + Superposition (2P2) FEA
3
4
ROW1 SCF
f,
2 Spring Model + Superposition (2P3) FEA SpringMode'+ Superposition (2P4) FEA
1
ROW2
ROW3 SCF
fi SCF fi
ROW4
fi SCF
6.2
0.60 4.7 0.40 2.5 0.60 4.7 0.40 2.4 0.52 4.4 0.29 2.3 0.19 1.2 0.52 4.5 0.29 2.2 0.19 1.2 0.54 4.5 0.24 2.0 0.13 1.0 0.09 0.06 0.50 4.4 0.26 2.2 0.15 1.1 0.10 0.06
* Aluminum joint with q/D = 4, D/t = 5, and P 2 P I= 1.
Structural Shear Joints
224
TABLE 17.6. COMPARISONS OF ESTIMATES OF THE FASTENER LOAD FRACTIONS, fi, FOR MULTIPLE ROW JOINTS DERIVED FROM THE 2SPRING MODEL WITH PREVIOUSLY REPORTED VALUES JOINT TYPE
FASTENER LOAD FRACTION, f,
2Springs Model
Reported Value* (Reference)
3 rivetrow lap joint leading or lagging row intermediate row
0.36 0.28
0.35 (92), 0.36 (95), 0.375 (24) 0.28 (95), 0.295 (92)
4 rivetrow lap joint leading or lagging row
0.3 1,0.28
0.32 (24)
4 rivetrow doubler leading or lagging row intermediate rows
0.19 0.06
0.14 (92) 0.04 (92)
*Note: The reported values are for similar but not identical panel and fastener dimensions.
CHAPTER
18 ANALYSIS OF FASTENER TENSION AND CLAMPING STRAIN 18.1 NOMENCLATURE
EF = fastener material elastic modulus Ep = panel material elastic modulus As = fastener shank crosssectional area. As = 7rDs2/4 Ap = crosssectional area of panels under the fastener head. Ap = x [ D B~Ds2]/4 A H = fastener head crosssectional area. A H = Ap H H = fastener head height HO= fastener shank height 2t = combined thickness of panels. 2t = HO kl = Fastener shank stiffness. kl = AsEF/Ho k2 = Combined panels stiffness. k2 = ApEp/2t
k3 = Fasteiler head stiffness. k3 = AHEF/HH
x = nominal fastener shank misfit. x = H o E N , ~ ~
residual shank extension combined panels compression QN= tension applied to shank to produce nominal shank extension. QN= klx Qc = residual tension in fastener shank. Qc = klx’ &N,cl = nominal clamping strain. EN,^^ = o/XL/lOO E = residual shank strain XI=
XI’=
225
226
Structural Shear Joints
...........................................................................
*...................
..............
Figure 18.1. Elasticloadingunloading model of the clamping process using linear springs k l , k2 and k3 to represent the fastener shank, panels and fastener head, respectively. The initial shank height misfit, x, is overcome by tensile loading. Unloading the fastener shank generates compression in the panels and fastener heads.
QN
ON.^^ = nominal clamping stress. (SN.~I = E s & ~ , c=i 
As
QN 0s = residual tensile stress in fastener shank. 0s = E S E= 
As
18.2 CLAMPING MODEL
Closedform expressions for the average fastener tension and clamping strain are derived. The equations relate average clamping state parameters to fastener and panel material properties, thicknesses and diameters. They account for the compliance of the panels and nonuniform fastener head deformation.
The Model. The generation of the clamped condition in a shear joint can be modeled as
a 2step process using a system of linear springs arranged in series and parallel, as shown in
Analysis of Fastener Tension and Clamping Strain
227
Figure 18.1.The first step is the tensile loading of the fastener shank (minus fastener heads) until the nominal value of the axial (clamping) strain is reached.The second step is the transfer of load to the panels and the two fastener heads which are compressed allowing the fastener shank to partially relax.
Affects of Panel Compliance and NonUniform Fastener Head Deformation. The fastener shank is first loaded in tension to (QN= klx) to overcome the initial misfit, x.The portions of the panels outside the boundaries of the fastener heads, and frictional slip between the fastenedhead and paneupanel interfaces are neglected. The following equilibrium and deformation compatibility conditions must be satisfied after relaxation (see Figure 18.1(b)): Equilibrium: Qc = klx’ = x’’ Compatibility: x  x’ = x’’
(18.1) (18.2)
After relaxation, the resultant load is shared by the panels, the fastener shank and the fastener head. Substituting for x“ from (18.2) in (18.1) and noting 2t Ho, we get L
(18.3)
(18.4)
(18.5)
Deformation of the fastener head is nonuniform. Since most of it is distributed across the annular region that surrounds the shank diameter i.e., the ring of fastener head material that directly overlaps the panels, only this portion of the fastener heads is considered, = APEF/HH. i.e., k3 = AHEF/HH 18.3 FASTENER TENSION AND CLAMPING STRAIN PREDICTIONS
Influence of Panel Compliance. The equations derived above can be applied to a typical aluminum alloy lap or butt joint considered in this book: EF = Ep = 70 GPa, Ds = 6.12 mm, Ho 2t = 3.06 mm, D B = 9.792 mm. Setting k3 = 0, This gives, L
x’
&
0s
x
&N,cl
0N.d
kl = 672.93 kN / mm, k2 = 1049.8 kN / mm, and K*= 0.61 =  = = This means that the clamping strain in this case is only 61% of the nominal value (assuming a rigid fastener head). Alternately, 39% of the nominal clamping strain is lost due to compressive deformation of the panels underneath the fastener head. *Forthe prototypical lap joint considered in this book with a shank height of 3.06 mm and a nominal clamping strain
Structural Shear Joints
228
EN^^ = 0.005 (0.5%), the corresponding value of shank extension is x = 0.0153 mm, and Equation (18.9) can be used to define the effective clamping state parameters as follows: E:
0.0031 (0.31% clamping)
X’:
0.0093 mm
I 4F:
I 213.3 MPa
I panels deformation: I 0.0060 mm
I
I
The average fastener shank stress due to clamping is 61% of the nominal value, ON = 350 MPa. Using Equations (18.4) and (18.9), it is possible to estimate the influence of different material combinations on the effective clamping. If the fastener material is steel ( E F= 206 GPa) instead of aluminum, K* = 0.35 and the effective clamping strain would be only 0.18% for a nominal clamping strain of 0.5%. Despite the reduction in K*, the steel fastener shank stress, os = 356.8 MPa, is still higher than with an aluminum fastener. This distinction between K* and the actual clamping stress, os,is an important one and must be kept in mind when interpreting K*. Influence of NonUniform Fastener Head Deformation. For the prototypical lap joint considered in this book, H H = 3.83 mm. This gives kl = 838.72 kN/mm which
0.00155 (0.155% clamping) 0.004743 mm 107.8 MPa
Qc = osAs
3189.9 N
panels deformation:
(Qc/k*=) 0.003038 mm
fastener heads deformation:
(2 Qc/ks) = 0.007519 mm
means that the shank strain is only about 0.16% for a nominal clamping of 0.5%; compressive deformation of the panels and fastener head cause a loss of about 20% and 49%, respectively, of the nominal clamping strain. With a steel fastener, K* = 0.22, the shank strain is O.ll%.The steel fastener shank stress, os = 229.3 MPa, is higher than with an aluminum fastener. Other examples are presented in Table 3.1. In Table 18.1,the values of (TS and Qs obtained with this analysis for several joints (including the one described in the above table) are compared with the average tension at the shank midsection and corresponding Q s derived from the finite element analyses. The analytical values for the relatively short rivets (first three entries) understate the more reliable finite element values by from 10% to 20%. The analytical values overstate the experimentally measured (TS for the long bolt (4thentry) by 70%. This discrepancy is attributed to significant departures from elastic behavior. The %C1= 1.3 clamping caused the bolt to undergo plastic deformation. The authors believe this both increases the accommodation at the bolt head and reduces the elastic stretch of the shank, features not accounted for by the analysis.
Analysis of Fastener Tension and Clamping Strain
229
TABLE 18.1. DISTRIBUTION OF ACCOMMODATIONS TO THE INITIAL CLAMPING MJSFIT MATERIAL
Aluminum Aluminum Steel Steel I
JOINT
CLAMPING
H, D, DB %CL (mm) (mm) (mm)
Misfit (mm)
3.06 6.12 6.12
6.12 6.12 6.12
9.79 9.79 9.79
0.5 0.5 0.85
0.0153 0.0306 0.052
108
22
33
1.3
1.4
MODEL
k,
k2
k,
K'
Qs
FEA'IANAL 'IEXP
QC
FEA'/ANAL 'IEXP
(kNlmm) (kN/mm 4s30 3s3 3s4
672.9 336.5 990.2
1049.8 524.9 1544.7
725.1
906.3
2468.2
120/108/170/143/85417 161
3.5/3.2/5.0/4.2/2512 I/I4451270
' ANAL.. Analyses FEA  Finite element analyses
' EXP  Experimental determination for a A354BD bolt (43)
18.4 SUMMARY OF PROCEDURE
The methodology for estimating the average fastener tension, clamping strain and distribution of deformations (compression of the panels, shank and fastener head) can be summarized as follows: 1. Using the fastener elastic modulus ( E F ) fastener , shank crosssectional area ( A s ) ,fastener shank nominal height (Ho), panels' elastic modulus ( E p ) , panel crosssectional ~ and fastener head height area underneath the fastener head ( A H = T C [ D B Ds2]/4) ( H H ) ,obtain stiffness values for the fastener shank ( k l ) , the panels (k2) and fastener head (k3) using kl = Fastener shank stiffness = A ~ E F / H ~ k2 = Combined panels stiffness = AHEP/Ho k3 = Fastener head stiffness = A H E F / H H
Note that the initial combined panel thickness (2t for a lap joint) has been approximated with HO in the expression for k2. This approximation simplifies the mathematical procedure without significant loss in accuracy and is reasonable for typical clamping misfit values. 2. Using the equations below, obtain K*
Obtain clamping strain, E, and fastener tension, Qc.
230
Structural Shear Joints
3. Obtain the deformation of the panels and fastener head as Qclk2 = combined deformation of panels = xp 2Qclk3 = combined deformation of 2 fastener heads = xh
4. The total deformation is (x’+ xP + xh) and should equal the nominal clamping misfit (CL). The proportions of deformations are given by x’ICL (fastener shank) xPICL (panels) xhlCL (fastener heads)
INDEX A Abbreviations xi, 225,226,231,253256 Adhesiveplusbearing mode calculational models 239 compliance 28 definition 10 design considerations 91 fastener tilt 28 polymer sealant 27 stress concentration factor, SCF 27,28 Alphanumeric code ix, 231 Angular conventions 14 Assembly variability 88 Attachment joint definition 3 multiple row 221
B Back panel definition 4 Bearing mode 1339 definition 13 design considerations 90 peak local stresses 13 Bearingplusadhesive mode (see adhesiveplusbearing mode) Biaxial loading 5,30,31,32,151,190,194, 238 lap joint 151,152 butt joint 151,153,154 Biaxial stress ratio 32 Bolt tension (see clamping force) Builtup joint 6 Butt joints (double shear)
calculational models 223 clamped butt joint 4 1 4 7 contact pressure 110112 definition 3 fretting factors 118123 gross section SCF 15 hole expansion (interference) 54,114 net section SCF 15 multiple rows 29,221 nondestructive evaluation, NDE 30 pitch 24,26 slip 117 stress concentration factor, SCF 14,15, 113115 Bypass load 222
C Calculation models 231240 Calibrating steel bolts 42 Clamping mode (frictional mode, slip resistant or slip critical mode calculational models 237 clearance 54 compliance 53 definition 9 design considerations 91 doublerow butt joint 54 fastener load 0 fastener stresses 54 force (bolt tension) 13,41, 225230 hysteresis 53 microslip 47,50 microtilt 47 misfit 229 multiple row joint 222
263
264
Structural Shear Joints
Clamping mode (continued) nominal clamping 41 residual stresses 42 shank strain 41 spring model 226 stress carrying capacity 95 stress field 49,50 stress concentration factor, SCF 4754 transition to bearing mode 46 Clearance 54 Compliance 13,23,28,53,59,94,173,183 definition 173 Contact pressure 13,50,56,59,63,110 Countersunk fastener 9,21,23,26,28, 29,3335,38,85,99105,128131, 138149,155,162,163,168171, 175177,179,181,182,185,191,220 Crack growth 67 Crack initiation 67 life 70 Cyclic life 90 Cyclic loading 53 Cyclic stressstrain behavior 7 D Damage tolerance 87 Design considerations 6.8795 Diameter/thicknessratio 24 Double rivetrow joint 24,54,135,173, 195,236 Doubler definition 3 finger 6 multiple row 217,221 stress concentration factor, SCF 19, 221 E Excess compliance (see compliance) Experimental validation 209 F Fail safe design 92 Fastener (also see rivet) cyclic stress capacity 91 flexibility 218 headshank corner 69 influence on panel SCF load 8,9,29,222
load in multiplerow joints 217 pitch 8,13,92, stresses 33,38.39,54,161171 tension, average 229 tilt 28 tilt angle 3 type xi,231 Fatigue cracks, detection of 91 durability 87 failure modes 6770 fretting 8286 Gerber diagram 245 life 11,28,70,87 multiple site damage, MSD 70 SCFFS Analysis, 7180,241247 SN curves of aluminum alloys 246 SN curves of open hole panels 243, 244 SN curves of shear joints 72,73,75,77, 80,247 strength of panels 7080 strength of fasteners 80,81 Filled open hole 14 Finite element models adhesiveplusfasteners (TALA) 197205 2D models of butt and attachment joints and open hole panels 189 3D models of butt and lap joints 190193,195 hole expansion (interference) and clamping 193 validation 209216,223 Fracture mechanics analyses 67 Free edge 30,31 Fretting 59,92 factors 12,250 wear 12,81 Fretting fatigue 12,82,249 double strap, bolted butt joint 85 rivet lap joint 85 single rivet row lap joint 85 factor (parameter) 118,119,120 Friction 6,13 stress carrying capacity 45 Frictional mode (see clamping mode) Front panel 4
Index
G Gerber diagram 71,245 Gross section location definition 50 failure 69
H Hole expansion (interference) 6,5459, 129,193,237 contact pressure 56 influence on bearing mode stresses 58 residual stresses 56,58 mandrel 55 modified net section failure 69 upset and squeeze 55 Hysteresis 53 I Interference (see hole expansion)
J Joint attachment 3 built up 6 butt (double shear) 3,14,15,24,26, 29,30,4147, 54,110112,233 compliance 13,28 configuration xi, 88,231 double row butt 54 double shear (see butt joint) failure 16 lap 3,20,33,37,234,235 measurement of lap 215 multiple row 3,8,29,32,217,232 narrow 5 selection 90 singlerow 31 single shear (see lap joint) variables xi, 231 wide 5 K k/Kratio 218
L Lagging row of fastener holes definition 4 loading 5,8,24 fastener stresses 38
265
Lap joint (single shear) calculational models 234236 clamped 4147 compliance 23 definition 3 double fastener row joint 24,177,236 fastener stresses 3338 fretting 8188 multiple row joint 29,221 nondestructive evaluation, NDE 20, 30 pitch 2426 single fastenerrow joint 17,18,2023, 173,178186 stress concentration factor, SCF 17,18, 2026,29,221 Leading row of fastener holes definition 4 loading 5,8,24,223 fastener stresses 33 Load transfer analysis 99105 load path 105 Load transfer mode bearing 8,13,90,99105 clamping 9,91 clampingplusbearing 10,91 adhesiveplusbearing 10,27,91 Local deformation 47
M Mandrel (see hole expansion) Material models and properties 207 Material variability 90 Microslip 6,7,47,50,59 Microtilt 47 Mode of load transfer adhesiveplusbearing 10,91 bearing 8,13,90,221 bearingplusadhesive 27 clamped 222 clampingplusbearing 10,50,51 definition 9 failure 67 fasteners in clamping 54 frictional 9,lO selection 90 slip critical 9 slip resistant 9,20
Structural Shear Joints
266
Monotonic strength 87 Multiple row joints analysis 217221 bearing mode 221 clamping mode 222 definition 3 fastener load 8,29,217,221 nondestructive evaluation, NDE 30 biaxial loading 32 stress concentration factors, SCF 29, 221224 Multiple Site Damage (MSD) 70
N Net section location butt and lap joints 50 definition 50 failure 67 peak stress 47 Nomenclature 225,253 Nominal stress 93 NonDestructive Evaluations (NDE) 20, 82,85,87,91 Normalized tangential stress 113 Nucleation of cracks 70 Number of fastener rows 93, 217224
0 Onedimensional spring models 30 Open hole panel empty 6,107,108,232 filled 6, 14,. 109,232 Outofplane deformation 3,6 P Panel back 4 configuration 88 definition 3 fastener 88 front 4 material 39,93,94 open hole 6,14,107109,232 thickness 24,92,183 Peak local stresses 13 Pinned connections with sealants and adhesives 157
Pitch 8 Pitchldiameter ratio 13,24,26, 92 Plasticity 7 Poisson’s contraction 29 Polymer sealants 27 Pressure dependent shear modulus 27
R Rratio 90 Rivet (also see fastener) countersunk fastener 9,21,23,26,28, 29,3335,38,85,99105,128131, 138149,155,162,163,168171, 175177,179,181,182,185,191,220 head 23 installation residual stresses 174 selfpiercing 63,65 shape 38 squeeze 54,55 stresses 161171 upset 55 vs. bolts 95 tilt 13,23,173,183
S SN curve aluminum alloys 246 open hole panels, aluminum 243244 shear joints, riveted aluminum lap 72, 73,77,79,80, 247 shear joints, bolted steel butt 75,76 SCFFS analysis of shear joint adhesiveplusbearing mode 74 bearing mode 71 clamping mode 74 SCFFS analysis of open hole panel 243244 Sealant modeling of 197 Sealants and adhesives 239 modeling of 194 Selfpiercing rivet lap joint fatigue 80 stress concentration factor, SCF 63 SNcurve 80 Shank failures 70 Shank strain 41
Index
Shear spring dependence of contact pressure 205 Shear stressstrain relationships for a thin sealant coating layer 204 Selfpiercing rivet, 6365 Installation 65 Single rivetrow 20 lap joints under biaxial loading 31,174 lap joints 125,129,173,176179,182, 184186 lap joints with sealants 175 lap joints with sealants and adhesives 157 Slip 13 Slip resistant mode (see clamping mode) Slip critical mode (see clamping mode) Solid adhesive spring element 197 Spring models of shear joint, 30,218 Standard head 33 Steel joints 38,75,76,93 Strength Reduction Factor Fatigue Strength (SRFFS) analysis with selfpiercing rivets 79 Stress Concentration Factor (SCF) 11, 14,1520,25,26,173,241 gross section 15
267
influence of adhesive stiffness 27 net section 15,30,51 superposition method for estimating 221 Stress ratio 245 Stiffness ratio 30 Symbols 225,226,231,253256
T Thin Adhesive Layer Analysis (TALA) 197 validation of 210 Thread root failure 69 3D finite element models 190196 Tilt 94,174 2D models attachment joints 189 butt joints 189 open hole panels 189
U Units 253256
V Validation of finite element models 209219